# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_audit_block_doi                 10.5517/cc13892r
_database_code_depnum_ccdc_archive 'CCDC 1020863'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C10 H24 Co2 N15 O44.50 Si W12'
_chemical_formula_sum            'C10 H15 Co2 N15 O44.50 Si W12'
_chemical_formula_weight         3418.40

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_H-M_alt        'P 2/n'
_space_group_name_Hall           '-P 2yac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y, -z+1/2'
'-x, -y, -z'
'x-1/2, -y, z-1/2'

_cell_length_a                   10.6100(5)
_cell_length_b                   11.8040(5)
_cell_length_c                   20.6980(5)
_cell_angle_alpha                90
_cell_angle_beta                 102.821(5)
_cell_angle_gamma                90
_cell_volume                     2527.60(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.7
_cell_measurement_theta_max      25.0

_exptl_crystal_description       acicular
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    4.480
_exptl_crystal_F_000             2984
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.14
_exptl_absorpt_coefficient_mu    27.963
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.009
_exptl_absorpt_correction_T_max  0.02
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            12249
_diffrn_reflns_av_unetI/netI     0.0905
_diffrn_reflns_av_R_equivalents  0.0754
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_theta_min         1.725
_diffrn_reflns_theta_max         25.030
_diffrn_reflns_theta_full        25.030
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             4456
_reflns_number_gt                2914
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 The restraint commands 'DELU' and 'SIMU' were 
refined the atoms N2,N6,C4 and C5,
 and the restraint command 'ISOR' was used
 to refine C3,N4,O4,O6,O13,O16,O2,O10,O12,O15 
and O20 atoms. The restraint orders 'SIMU' were 
refined the atoms O15,W3,W5,Co1,and N3. The 'DFIX' 
command was used to bind N6 and N2. 
 The 'OMIT' order was used to confirm the data 
completeless.
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0459P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         4456
_refine_ls_number_parameters     386
_refine_ls_number_restraints     106
_refine_ls_R_factor_all          0.0891
_refine_ls_R_factor_gt           0.0481
_refine_ls_wR_factor_ref         0.1058
_refine_ls_wR_factor_gt          0.0927
_refine_ls_goodness_of_fit_ref   0.967
_refine_ls_restrained_S_all      0.973
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.1078(12) 0.4243(15) 1.0348(8) 0.057(5) Uani 1 1 d . . . . .
O2 O -0.1139(14) -0.2374(18) 0.8889(8) 0.068(5) Uani 1 1 d . U . . .
O1W O -0.5523(12) 0.2566(16) 1.1465(6) 0.049(5) Uani 1 1 d . . . . .
O3 O -0.0116(15) 0.0308(15) 0.8212(10) 0.072(6) Uani 1 1 d . . . . .
O2W O -0.2280(13) 0.4242(15) 0.8530(8) 0.054(5) Uani 1 1 d . . . . .
O4 O -0.071(2) 0.030(2) 0.9246(10) 0.020(6) Uani 0.5 1 d . U P . .
O3W O -0.2500 -0.227(5) 1.2500 0.060(13) Uiso 0.5 2 d S . P . .
O5 O 0.2361(14) 0.2306(18) 1.0141(7) 0.070(6) Uani 1 1 d . . . . .
O6 O 0.4346(15) 0.1542(15) 0.9610(8) 0.056(5) Uani 1 1 d . U . . .
O7 O -0.2940(18) 0.0385(13) 1.0612(6) 0.057(5) Uani 1 1 d . . . . .
O8 O -0.3475(18) -0.0448(14) 0.9403(7) 0.060(5) Uani 1 1 d . . . . .
O9 O -0.2944(17) 0.1744(13) 0.9591(7) 0.055(5) Uani 1 1 d . . . . .
O10 O -0.4329(14) 0.0997(15) 0.8374(7) 0.051(5) Uani 1 1 d . U . . .
O11 O -0.3260(13) 0.2660(12) 1.0787(6) 0.030(3) Uani 1 1 d . . . . .
O12 O -0.1024(15) 0.1531(17) 1.1287(8) 0.071(5) Uani 1 1 d . U . . .
O13 O -0.069(2) -0.102(2) 1.0296(11) 0.021(6) Uani 0.5 1 d . U P . .
O14 O 0.0153(14) 0.2839(18) 0.9314(8) 0.073(6) Uani 1 1 d . . . . .
O15 O -0.1027(13) 0.2911(16) 1.0300(7) 0.058(4) Uani 1 1 d . U . . .
O16 O -0.020(2) 0.118(2) 1.0431(11) 0.023(6) Uani 0.5 1 d . U P . .
O17 O -0.1751(16) 0.1686(15) 0.8595(10) 0.076(6) Uani 1 1 d . . . . .
O18 O 0.0050(14) 0.2604(16) 0.7961(7) 0.055(5) Uani 1 1 d . . . . .
O19 O 0.148(2) -0.024(2) 1.0084(10) 0.021(6) Uani 0.5 1 d . . P . .
O20 O -0.2318(16) -0.0471(16) 0.8435(9) 0.070(5) Uani 1 1 d . U . . .
O21 O 0.1811(16) 0.1485(17) 0.8954(7) 0.075(7) Uani 1 1 d . . . . .
O22 O -0.0994(11) -0.1746(14) 0.7645(6) 0.036(4) Uani 1 1 d . . . . .
Co1 Co -0.3680(2) 0.3376(3) 1.16810(12) 0.0269(7) Uani 1 1 d . . . . .
W1 W 0.00218(8) 0.17313(8) 0.86102(4) 0.0298(2) Uani 1 1 d . . . . .
W2 W -0.07218(8) -0.11674(9) 0.83891(4) 0.0326(3) Uani 1 1 d . . . . .
W3 W -0.22158(7) 0.18248(8) 1.04972(4) 0.0274(2) Uani 1 1 d . U . . .
W4 W 0.29492(7) 0.10697(8) 0.97364(4) 0.0244(2) Uani 1 1 d . . . . .
W5 W 0.07166(8) 0.29162(8) 1.02193(4) 0.0302(2) Uani 1 1 d . U . . .
W6 W -0.29324(7) 0.06906(8) 0.88780(4) 0.0245(2) Uani 1 1 d . . . . .
Si1 Si 0.0000 0.0000 1.0000 0.0158(16) Uani 1 2 d S . P . .
N1 N -0.1800(15) 0.4144(15) 1.1850(7) 0.030(4) Uiso 1 1 d . . . . .
N2 N -0.4575(15) 0.4701(18) 1.1094(8) 0.041(4) Uani 1 1 d D U . . .
N3 N -0.524(2) 0.634(2) 1.0721(12) 0.092(7) Uani 1 1 d . U . . .
H3 H -0.5248 0.7059 1.0672 0.110 Uiso 1 1 calc R U . . .
N4 N -0.2994(14) 0.1932(15) 1.2205(7) 0.030(4) Uani 1 1 d . U . . .
N5 N -0.2500 0.011(2) 1.2500 0.051(8) Uani 1 2 d S T P . .
H5 H -0.2500 -0.0615 1.2500 0.061 Uiso 1 2 calc R U P . .
N6 N -0.5682(19) 0.460(2) 1.0615(10) 0.084(7) Uani 1 1 d D U . . .
N7 N -0.0924(15) 0.4094(15) 1.2457(7) 0.029(4) Uani 1 1 d . . . . .
N8 N -0.0011(16) 0.4896(17) 1.1726(8) 0.039(5) Uiso 1 1 d . . . . .
H8 H 0.0567 0.5200 1.1548 0.047 Uiso 1 1 calc R U . . .
C1 C -0.117(2) 0.464(2) 1.1441(13) 0.058(7) Uiso 1 1 d . . . . .
H1 H -0.1532 0.4787 1.0997 0.070 Uiso 1 1 calc R U . . .
C2 C 0.012(2) 0.458(2) 1.2374(10) 0.039(6) Uani 1 1 d . . . . .
H2 H 0.0849 0.4706 1.2708 0.047 Uiso 1 1 calc R U . . .
C3 C -0.326(2) 0.083(2) 1.2055(11) 0.045(6) Uani 1 1 d . U . . .
H3A H -0.3891 0.0592 1.1693 0.054 Uiso 1 1 calc R U . . .
C4 C -0.442(2) 0.577(2) 1.1149(13) 0.064(6) Uani 1 1 d . U . . .
H4 H -0.3777 0.6113 1.1469 0.076 Uiso 1 1 calc R U . . .
C5 C -0.613(3) 0.556(3) 1.0338(14) 0.082(8) Uani 1 1 d . U . . .
H5A H -0.6841 0.5697 0.9990 0.098 Uiso 1 1 calc R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 W5 1.620(17) . ?
O2 W2 1.870(18) . ?
O2 W5 1.911(16) 3_557 ?
O1W Co1 2.133(13) . ?
O3 W1 1.863(17) . ?
O3 W2 1.920(17) . ?
O4 Si1 1.61(2) . ?
O4 O19 1.76(3) 3_557 ?
O4 O13 1.78(3) 3_557 ?
O4 W6 2.36(2) . ?
O4 W1 2.37(2) . ?
O4 W2 2.48(2) . ?
O5 W4 1.858(16) . ?
O5 W5 1.927(14) . ?
O6 W4 1.658(15) . ?
O7 W4 1.862(15) 3_557 ?
O7 W3 1.902(16) . ?
O8 W4 1.893(15) 3_557 ?
O8 W6 1.897(16) . ?
O9 W3 1.866(14) . ?
O9 W6 1.932(15) . ?
O10 W6 1.652(13) . ?
O11 W3 1.690(13) . ?
O11 Co1 2.168(12) . ?
O12 W3 1.865(16) . ?
O12 W2 1.874(16) 3_557 ?
O13 Si1 1.60(2) . ?
O13 O4 1.78(3) 3_557 ?
O13 O19 1.81(4) 3_557 ?
O13 W1 2.37(2) 3_557 ?
O13 W4 2.39(2) 3_557 ?
O13 W5 2.47(3) 3_557 ?
O14 W5 1.838(16) . ?
O14 W1 1.939(16) . ?
O15 W5 1.894(14) . ?
O15 W3 1.905(15) . ?
O16 Si1 1.69(3) . ?
O16 W3 2.30(2) . ?
O16 W5 2.35(3) . ?
O16 W2 2.42(2) 3_557 ?
O17 W1 1.875(15) . ?
O17 W6 1.902(15) . ?
O18 W1 1.698(15) . ?
O19 Si1 1.57(2) . ?
O19 O4 1.76(3) 3_557 ?
O19 O13 1.81(4) 3_557 ?
O19 W6 2.41(2) 3_557 ?
O19 W4 2.42(2) . ?
O19 W3 2.44(3) 3_557 ?
O20 W6 1.847(17) . ?
O20 W2 1.904(16) . ?
O21 W4 1.858(15) . ?
O21 W1 1.896(15) . ?
O22 W2 1.651(11) . ?
Co1 N4 2.064(18) . ?
Co1 N2 2.076(18) . ?
Co1 N7 2.101(16) 2_457 ?
Co1 N1 2.149(16) . ?
W1 O13 2.37(2) 3_557 ?
W2 O12 1.874(16) 3_557 ?
W2 O16 2.42(2) 3_557 ?
W3 O19 2.44(3) 3_557 ?
W4 O7 1.862(15) 3_557 ?
W4 O8 1.893(15) 3_557 ?
W4 O13 2.39(2) 3_557 ?
W5 O2 1.911(16) 3_557 ?
W5 O13 2.47(3) 3_557 ?
W6 O19 2.41(2) 3_557 ?
Si1 O19 1.57(2) 3_557 ?
Si1 O13 1.60(3) 3_557 ?
Si1 O4 1.61(2) 3_557 ?
Si1 O16 1.69(3) 3_557 ?
N1 C1 1.33(3) . ?
N1 N7 1.39(2) . ?
N2 C4 1.28(3) . ?
N2 N6 1.364(10) . ?
N3 C4 1.28(3) . ?
N3 C5 1.43(4) . ?
N3 H3 0.8600 . ?
N4 C3 1.35(3) . ?
N4 N4 1.42(3) 2_457 ?
N5 C3 1.38(3) 2_457 ?
N5 C3 1.38(3) . ?
N5 H5 0.8600 . ?
N6 C5 1.31(4) . ?
N7 C2 1.29(2) . ?
N7 Co1 2.101(16) 2_457 ?
N8 C1 1.28(3) . ?
N8 C2 1.37(3) . ?
N8 H8 0.8600 . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3A 0.9300 . ?
C4 H4 0.9300 . ?
C5 H5A 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W2 O2 W5 139.1(10) . 3_557 ?
W1 O3 W2 136.9(10) . . ?
Si1 O4 O19 55.1(10) . 3_557 ?
Si1 O4 O13 55.9(10) . 3_557 ?
O19 O4 O13 94.4(14) 3_557 3_557 ?
Si1 O4 W6 124.9(11) . . ?
O19 O4 W6 69.7(10) 3_557 . ?
O13 O4 W6 136.9(16) 3_557 . ?
Si1 O4 W1 123.7(12) . . ?
O19 O4 W1 137.0(16) 3_557 . ?
O13 O4 W1 67.8(11) 3_557 . ?
W6 O4 W1 96.2(8) . . ?
Si1 O4 W2 117.8(13) . . ?
O19 O4 W2 127.2(15) 3_557 . ?
O13 O4 W2 125.9(13) 3_557 . ?
W6 O4 W2 93.3(8) . . ?
W1 O4 W2 93.0(7) . . ?
W4 O5 W5 137.1(10) . . ?
W4 O7 W3 138.0(8) 3_557 . ?
W4 O8 W6 138.6(10) 3_557 . ?
W3 O9 W6 136.9(10) . . ?
W3 O11 Co1 143.7(7) . . ?
W3 O12 W2 141.3(10) . 3_557 ?
Si1 O13 O4 56.6(11) . 3_557 ?
Si1 O13 O19 54.4(11) . 3_557 ?
O4 O13 O19 95.1(17) 3_557 3_557 ?
Si1 O13 W1 124.6(12) . 3_557 ?
O4 O13 W1 68.0(10) 3_557 3_557 ?
O19 O13 W1 136.0(14) 3_557 3_557 ?
Si1 O13 W4 123.2(14) . 3_557 ?
O4 O13 W4 137.3(14) 3_557 3_557 ?
O19 O13 W4 68.8(10) 3_557 3_557 ?
W1 O13 W4 95.9(8) 3_557 3_557 ?
Si1 O13 W5 118.7(11) . 3_557 ?
O4 O13 W5 126.1(15) 3_557 3_557 ?
O19 O13 W5 126.8(13) 3_557 3_557 ?
W1 O13 W5 93.8(9) 3_557 3_557 ?
W4 O13 W5 92.9(8) 3_557 3_557 ?
W5 O14 W1 138.8(11) . . ?
W5 O15 W3 136.7(10) . . ?
Si1 O16 W3 122.1(12) . . ?
Si1 O16 W5 120.8(11) . . ?
W3 O16 W5 98.6(10) . . ?
Si1 O16 W2 117.2(13) . 3_557 ?
W3 O16 W2 96.6(8) . 3_557 ?
W5 O16 W2 95.8(9) . 3_557 ?
W1 O17 W6 137.7(12) . . ?
Si1 O19 O4 57.6(10) . 3_557 ?
Si1 O19 O13 56.1(11) . 3_557 ?
O4 O19 O13 97.0(16) 3_557 3_557 ?
Si1 O19 W6 124.5(11) . 3_557 ?
O4 O19 W6 66.9(10) 3_557 3_557 ?
O13 O19 W6 135.6(15) 3_557 3_557 ?
Si1 O19 W4 123.1(13) . . ?
O4 O19 W4 134.7(15) 3_557 . ?
O13 O19 W4 67.0(11) 3_557 . ?
W6 O19 W4 94.6(8) 3_557 . ?
Si1 O19 W3 120.4(12) . 3_557 ?
O4 O19 W3 127.8(15) 3_557 3_557 ?
O13 O19 W3 125.9(12) 3_557 3_557 ?
W6 O19 W3 93.5(9) 3_557 3_557 ?
W4 O19 W3 92.6(7) . 3_557 ?
W6 O20 W2 139.6(10) . . ?
W4 O21 W1 140.4(10) . . ?
N4 Co1 N2 172.5(7) . . ?
N4 Co1 N7 90.0(6) . 2_457 ?
N2 Co1 N7 92.4(7) . 2_457 ?
N4 Co1 O1W 86.6(6) . . ?
N2 Co1 O1W 86.3(7) . . ?
N7 Co1 O1W 90.7(6) 2_457 . ?
N4 Co1 N1 93.2(6) . . ?
N2 Co1 N1 93.7(7) . . ?
N7 Co1 N1 92.6(6) 2_457 . ?
O1W Co1 N1 176.7(6) . . ?
N4 Co1 O11 90.7(6) . . ?
N2 Co1 O11 87.0(6) . . ?
N7 Co1 O11 179.1(6) 2_457 . ?
O1W Co1 O11 89.9(5) . . ?
N1 Co1 O11 86.8(6) . . ?
O18 W1 O3 102.1(8) . . ?
O18 W1 O17 101.4(8) . . ?
O3 W1 O17 89.2(7) . . ?
O18 W1 O21 101.4(8) . . ?
O3 W1 O21 90.1(8) . . ?
O17 W1 O21 156.8(9) . . ?
O18 W1 O14 100.1(9) . . ?
O3 W1 O14 157.8(9) . . ?
O17 W1 O14 86.3(7) . . ?
O21 W1 O14 85.6(6) . . ?
O18 W1 O13 156.4(9) . 3_557 ?
O3 W1 O13 94.7(9) . 3_557 ?
O17 W1 O13 95.2(8) . 3_557 ?
O21 W1 O13 61.7(8) . 3_557 ?
O14 W1 O13 64.1(9) . 3_557 ?
O18 W1 O4 159.3(8) . . ?
O3 W1 O4 66.5(8) . . ?
O17 W1 O4 62.6(8) . . ?
O21 W1 O4 96.0(8) . . ?
O14 W1 O4 92.3(9) . . ?
O13 W1 O4 44.2(8) 3_557 . ?
O22 W2 O2 100.8(8) . . ?
O22 W2 O12 101.1(7) . 3_557 ?
O2 W2 O12 88.0(7) . 3_557 ?
O22 W2 O20 104.6(7) . . ?
O2 W2 O20 88.8(8) . . ?
O12 W2 O20 154.2(8) 3_557 . ?
O22 W2 O3 101.2(8) . . ?
O2 W2 O3 158.0(8) . . ?
O12 W2 O3 86.0(8) 3_557 . ?
O20 W2 O3 87.5(7) . . ?
O22 W2 O16 152.5(8) . 3_557 ?
O2 W2 O16 62.0(8) . 3_557 ?
O12 W2 O16 59.5(8) 3_557 3_557 ?
O20 W2 O16 96.7(8) . 3_557 ?
O3 W2 O16 96.9(9) . 3_557 ?
O22 W2 O4 158.4(8) . . ?
O2 W2 O4 95.8(8) . . ?
O12 W2 O4 93.2(8) 3_557 . ?
O20 W2 O4 61.8(8) . . ?
O3 W2 O4 63.4(8) . . ?
O16 W2 O4 49.0(8) 3_557 . ?
O11 W3 O12 99.7(7) . . ?
O11 W3 O9 103.2(7) . . ?
O12 W3 O9 157.1(8) . . ?
O11 W3 O7 99.3(7) . . ?
O12 W3 O7 86.5(8) . . ?
O9 W3 O7 89.5(6) . . ?
O11 W3 O15 101.6(7) . . ?
O12 W3 O15 87.7(7) . . ?
O9 W3 O15 88.0(7) . . ?
O7 W3 O15 159.0(8) . . ?
O11 W3 O16 154.9(8) . . ?
O12 W3 O16 62.1(8) . . ?
O9 W3 O16 96.1(8) . . ?
O7 W3 O16 96.7(9) . . ?
O15 W3 O16 62.8(9) . . ?
O11 W3 O19 158.1(7) . 3_557 ?
O12 W3 O19 93.5(8) . 3_557 ?
O9 W3 O19 64.6(7) . 3_557 ?
O7 W3 O19 63.9(7) . 3_557 ?
O15 W3 O19 96.3(8) . 3_557 ?
O16 W3 O19 46.8(8) . 3_557 ?
O6 W4 O21 101.8(8) . . ?
O6 W4 O5 102.1(9) . . ?
O21 W4 O5 88.1(6) . . ?
O6 W4 O7 100.2(8) . 3_557 ?
O21 W4 O7 87.7(7) . 3_557 ?
O5 W4 O7 157.7(8) . 3_557 ?
O6 W4 O8 101.1(8) . 3_557 ?
O21 W4 O8 157.1(8) . 3_557 ?
O5 W4 O8 86.4(7) . 3_557 ?
O7 W4 O8 89.0(6) 3_557 3_557 ?
O6 W4 O13 158.8(9) . 3_557 ?
O21 W4 O13 61.8(8) . 3_557 ?
O5 W4 O13 66.1(8) . 3_557 ?
O7 W4 O13 92.8(9) 3_557 3_557 ?
O8 W4 O13 95.9(8) 3_557 3_557 ?
O6 W4 O19 157.0(9) . . ?
O21 W4 O19 95.3(8) . . ?
O5 W4 O19 93.7(9) . . ?
O7 W4 O19 64.9(8) 3_557 . ?
O8 W4 O19 63.0(8) 3_557 . ?
O13 W4 O19 44.2(8) 3_557 . ?
O1 W5 O14 103.1(9) . . ?
O1 W5 O15 100.9(8) . . ?
O14 W5 O15 89.2(7) . . ?
O1 W5 O2 99.7(9) . 3_557 ?
O14 W5 O2 157.1(9) . 3_557 ?
O15 W5 O2 86.4(6) . 3_557 ?
O1 W5 O5 100.9(8) . . ?
O14 W5 O5 89.5(6) . . ?
O15 W5 O5 157.8(9) . . ?
O2 W5 O5 86.2(7) 3_557 . ?
O1 W5 O16 154.8(8) . . ?
O14 W5 O16 95.3(9) . . ?
O15 W5 O16 61.8(8) . . ?
O2 W5 O16 63.0(8) 3_557 . ?
O5 W5 O16 96.3(9) . . ?
O1 W5 O13 157.5(8) . 3_557 ?
O14 W5 O13 63.0(8) . 3_557 ?
O15 W5 O13 96.6(8) . 3_557 ?
O2 W5 O13 95.3(8) 3_557 3_557 ?
O5 W5 O13 63.3(8) . 3_557 ?
O16 W5 O13 47.7(8) . 3_557 ?
O10 W6 O20 102.4(8) . . ?
O10 W6 O8 100.0(8) . . ?
O20 W6 O8 86.7(7) . . ?
O10 W6 O17 103.3(9) . . ?
O20 W6 O17 88.7(7) . . ?
O8 W6 O17 156.7(9) . . ?
O10 W6 O9 100.6(8) . . ?
O20 W6 O9 156.9(8) . . ?
O8 W6 O9 88.0(6) . . ?
O17 W6 O9 87.4(7) . . ?
O10 W6 O4 160.0(7) . . ?
O20 W6 O4 65.0(8) . . ?
O8 W6 O4 95.0(8) . . ?
O17 W6 O4 62.6(8) . . ?
O9 W6 O4 93.1(8) . . ?
O10 W6 O19 156.7(7) . 3_557 ?
O20 W6 O19 93.0(9) . 3_557 ?
O8 W6 O19 63.2(8) . 3_557 ?
O17 W6 O19 94.3(9) . 3_557 ?
O9 W6 O19 64.6(8) . 3_557 ?
O4 W6 O19 43.4(7) . 3_557 ?
O19 Si1 O19 180.0(19) . 3_557 ?
O19 Si1 O13 69.5(12) . 3_557 ?
O19 Si1 O13 110.5(12) 3_557 3_557 ?
O19 Si1 O13 110.5(12) . . ?
O19 Si1 O13 69.5(12) 3_557 . ?
O13 Si1 O13 180.0(19) 3_557 . ?
O19 Si1 O4 67.3(11) . 3_557 ?
O19 Si1 O4 112.7(11) 3_557 3_557 ?
O13 Si1 O4 112.6(12) 3_557 3_557 ?
O13 Si1 O4 67.4(12) . 3_557 ?
O19 Si1 O4 112.7(11) . . ?
O19 Si1 O4 67.3(11) 3_557 . ?
O13 Si1 O4 67.4(12) 3_557 . ?
O13 Si1 O4 112.6(12) . . ?
O4 Si1 O4 180.0 3_557 . ?
O19 Si1 O16 109.4(12) . . ?
O19 Si1 O16 70.6(12) 3_557 . ?
O13 Si1 O16 72.7(12) 3_557 . ?
O13 Si1 O16 107.3(11) . . ?
O4 Si1 O16 75.9(12) 3_557 . ?
O4 Si1 O16 104.1(12) . . ?
O19 Si1 O16 70.6(12) . 3_557 ?
O19 Si1 O16 109.4(12) 3_557 3_557 ?
O13 Si1 O16 107.3(11) 3_557 3_557 ?
O13 Si1 O16 72.7(12) . 3_557 ?
O4 Si1 O16 104.1(12) 3_557 3_557 ?
O4 Si1 O16 75.9(12) . 3_557 ?
O16 Si1 O16 180.0 . 3_557 ?
C1 N1 N7 105.4(17) . . ?
C1 N1 Co1 131.6(15) . . ?
N7 N1 Co1 122.7(12) . . ?
C4 N2 N6 103(2) . . ?
C4 N2 Co1 131.4(17) . . ?
N6 N2 Co1 124.7(18) . . ?
C4 N3 C5 109(3) . . ?
C4 N3 H3 125.7 . . ?
C5 N3 H3 125.7 . . ?
C3 N4 N4 106.0(13) . 2_457 ?
C3 N4 Co1 129.8(14) . . ?
N4 N4 Co1 123.9(5) 2_457 . ?
C3 N5 C3 104(3) 2_457 . ?
C3 N5 H5 128.2 2_457 . ?
C3 N5 H5 128.2 . . ?
C5 N6 N2 115(3) . . ?
C2 N7 N1 106.4(16) . . ?
C2 N7 Co1 129.1(14) . 2_457 ?
N1 N7 Co1 124.5(12) . 2_457 ?
C1 N8 C2 105(2) . . ?
C1 N8 H8 127.3 . . ?
C2 N8 H8 127.3 . . ?
N8 C1 N1 112(2) . . ?
N8 C1 H1 123.9 . . ?
N1 C1 H1 123.9 . . ?
N7 C2 N8 110.4(18) . . ?
N7 C2 H2 124.8 . . ?
N8 C2 H2 124.8 . . ?
N4 C3 N5 112(2) . . ?
N4 C3 H3A 123.9 . . ?
N5 C3 H3A 123.9 . . ?
N3 C4 N2 113(3) . . ?
N3 C4 H4 123.3 . . ?
N2 C4 H4 123.3 . . ?
N6 C5 N3 100(2) . . ?
N6 C5 H5A 129.9 . . ?
N3 C5 H5A 129.9 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
W2 O3 W1 O18 -156.7(14) . . . . ?
W2 O3 W1 O17 -55.1(15) . . . . ?
W2 O3 W1 O21 101.6(15) . . . . ?
W2 O3 W1 O14 23(3) . . . . ?
W2 O3 W1 O13 40.0(15) . . . 3_557 ?
W2 O3 W1 O4 5.1(13) . . . . ?
W6 O17 W1 O18 155.4(14) . . . . ?
W6 O17 W1 O3 53.2(15) . . . . ?
W6 O17 W1 O21 -35(3) . . . . ?
W6 O17 W1 O14 -105.1(15) . . . . ?
W6 O17 W1 O13 -41.5(15) . . . 3_557 ?
W6 O17 W1 O4 -10.6(13) . . . . ?
W4 O21 W1 O18 156.9(17) . . . . ?
W4 O21 W1 O3 -100.7(18) . . . . ?
W4 O21 W1 O17 -12(3) . . . . ?
W4 O21 W1 O14 57.5(17) . . . . ?
W4 O21 W1 O13 -5.4(15) . . . 3_557 ?
W4 O21 W1 O4 -34.4(18) . . . . ?
W5 O2 W2 O22 153.7(14) 3_557 . . . ?
W5 O2 W2 O12 52.7(16) 3_557 . . 3_557 ?
W5 O2 W2 O20 -101.7(16) 3_557 . . . ?
W5 O2 W2 O3 -21(3) 3_557 . . . ?
W5 O2 W2 O16 -3.4(13) 3_557 . . 3_557 ?
W5 O2 W2 O4 -40.3(16) 3_557 . . . ?
Co1 O11 W3 O12 -3.3(14) . . . . ?
Co1 O11 W3 O9 176.3(12) . . . . ?
Co1 O11 W3 O7 84.7(13) . . . . ?
Co1 O11 W3 O15 -93.0(13) . . . . ?
Co1 O11 W3 O16 -44(3) . . . . ?
Co1 O11 W3 O19 122.8(18) . . . 3_557 ?
W2 O12 W3 O11 -153.1(18) 3_557 . . . ?
W2 O12 W3 O9 28(3) 3_557 . . . ?
W2 O12 W3 O7 108.1(19) 3_557 . . . ?
W2 O12 W3 O15 -51.7(18) 3_557 . . . ?
W2 O12 W3 O16 8.5(16) 3_557 . . . ?
W2 O12 W3 O19 44.5(19) 3_557 . . 3_557 ?
W6 O9 W3 O11 -153.5(12) . . . . ?
W6 O9 W3 O12 26(3) . . . . ?
W6 O9 W3 O7 -54.0(13) . . . . ?
W6 O9 W3 O15 105.1(14) . . . . ?
W6 O9 W3 O16 42.7(14) . . . . ?
W6 O9 W3 O19 7.1(12) . . . 3_557 ?
W1 O21 W4 O6 -160.3(17) . . . . ?
W1 O21 W4 O5 -58.3(18) . . . . ?
W1 O21 W4 O7 99.8(17) . . . 3_557 ?
W1 O21 W4 O8 18(3) . . . 3_557 ?
W1 O21 W4 O13 5.4(15) . . . 3_557 ?
W1 O21 W4 O19 35.3(18) . . . . ?
W5 O5 W4 O6 152.8(15) . . . . ?
W5 O5 W4 O21 51.1(16) . . . . ?
W5 O5 W4 O7 -28(3) . . . 3_557 ?
W5 O5 W4 O8 -106.7(16) . . . 3_557 ?
W5 O5 W4 O13 -8.7(13) . . . 3_557 ?
W5 O5 W4 O19 -44.1(15) . . . . ?
W1 O14 W5 O1 154.4(14) . . . . ?
W1 O14 W5 O15 -104.6(15) . . . . ?
W1 O14 W5 O2 -26(3) . . . 3_557 ?
W1 O14 W5 O5 53.3(15) . . . . ?
W1 O14 W5 O16 -42.9(15) . . . . ?
W1 O14 W5 O13 -6.7(13) . . . 3_557 ?
W3 O15 W5 O1 -157.3(12) . . . . ?
W3 O15 W5 O14 99.5(13) . . . . ?
W3 O15 W5 O2 -58.1(13) . . . 3_557 ?
W3 O15 W5 O5 13(2) . . . . ?
W3 O15 W5 O16 3.1(11) . . . . ?
W3 O15 W5 O13 36.8(13) . . . 3_557 ?
W2 O20 W6 O10 156.8(16) . . . . ?
W2 O20 W6 O8 -103.6(16) . . . . ?
W2 O20 W6 O17 53.5(17) . . . . ?
W2 O20 W6 O9 -27(3) . . . . ?
W2 O20 W6 O4 -6.6(14) . . . . ?
W2 O20 W6 O19 -40.8(17) . . . 3_557 ?
W4 O8 W6 O10 -154.0(14) 3_557 . . . ?
W4 O8 W6 O20 104.0(14) 3_557 . . . ?
W4 O8 W6 O17 25(3) 3_557 . . . ?
W4 O8 W6 O9 -53.5(14) 3_557 . . . ?
W4 O8 W6 O4 39.4(14) 3_557 . . . ?
W4 O8 W6 O19 8.9(12) 3_557 . . 3_557 ?
O4 O19 Si1 O13 126.9(15) 3_557 . . 3_557 ?
W6 O19 Si1 O13 125.7(18) 3_557 . . 3_557 ?
W4 O19 Si1 O13 1.4(12) . . . 3_557 ?
W3 O19 Si1 O13 -115.1(14) 3_557 . . 3_557 ?
O4 O19 Si1 O13 -53.1(15) 3_557 . . . ?
O13 O19 Si1 O13 179.999(10) 3_557 . . . ?
W6 O19 Si1 O13 -54.3(18) 3_557 . . . ?
W4 O19 Si1 O13 -178.6(12) . . . . ?
W3 O19 Si1 O13 64.9(14) 3_557 . . . ?
O13 O19 Si1 O4 -126.9(15) 3_557 . . 3_557 ?
W6 O19 Si1 O4 -1.2(14) 3_557 . . 3_557 ?
W4 O19 Si1 O4 -125.5(18) . . . 3_557 ?
W3 O19 Si1 O4 118.0(17) 3_557 . . 3_557 ?
O4 O19 Si1 O4 180.002(18) 3_557 . . . ?
O13 O19 Si1 O4 53.1(15) 3_557 . . . ?
W6 O19 Si1 O4 178.8(14) 3_557 . . . ?
W4 O19 Si1 O4 54.5(18) . . . . ?
W3 O19 Si1 O4 -62.0(17) 3_557 . . . ?
O4 O19 Si1 O16 64.8(15) 3_557 . . . ?
O13 O19 Si1 O16 -62.2(13) 3_557 . . . ?
W6 O19 Si1 O16 63.5(18) 3_557 . . . ?
W4 O19 Si1 O16 -60.8(15) . . . . ?
W3 O19 Si1 O16 -177.3(12) 3_557 . . . ?
O4 O19 Si1 O16 -115.2(15) 3_557 . . 3_557 ?
O13 O19 Si1 O16 117.8(13) 3_557 . . 3_557 ?
W6 O19 Si1 O16 -116.5(18) 3_557 . . 3_557 ?
W4 O19 Si1 O16 119.2(15) . . . 3_557 ?
W3 O19 Si1 O16 2.7(12) 3_557 . . 3_557 ?
O4 O13 Si1 O19 53.0(14) 3_557 . . . ?
O19 O13 Si1 O19 180.000(11) 3_557 . . . ?
W1 O13 Si1 O19 54.5(18) 3_557 . . . ?
W4 O13 Si1 O19 -178.6(12) 3_557 . . . ?
W5 O13 Si1 O19 -63.4(15) 3_557 . . . ?
O4 O13 Si1 O19 -127.0(14) 3_557 . . 3_557 ?
W1 O13 Si1 O19 -125.5(18) 3_557 . . 3_557 ?
W4 O13 Si1 O19 1.4(12) 3_557 . . 3_557 ?
W5 O13 Si1 O19 116.6(15) 3_557 . . 3_557 ?
O19 O13 Si1 O4 127.0(14) 3_557 . . 3_557 ?
W1 O13 Si1 O4 1.5(13) 3_557 . . 3_557 ?
W4 O13 Si1 O4 128.4(17) 3_557 . . 3_557 ?
W5 O13 Si1 O4 -116.4(16) 3_557 . . 3_557 ?
O4 O13 Si1 O4 179.998(2) 3_557 . . . ?
O19 O13 Si1 O4 -53.0(14) 3_557 . . . ?
W1 O13 Si1 O4 -178.5(13) 3_557 . . . ?
W4 O13 Si1 O4 -51.6(17) 3_557 . . . ?
W5 O13 Si1 O4 63.6(16) 3_557 . . . ?
O4 O13 Si1 O16 -66.1(14) 3_557 . . . ?
O19 O13 Si1 O16 60.9(13) 3_557 . . . ?
W1 O13 Si1 O16 -64.6(17) 3_557 . . . ?
W4 O13 Si1 O16 62.3(15) 3_557 . . . ?
W5 O13 Si1 O16 177.4(12) 3_557 . . . ?
O4 O13 Si1 O16 113.9(14) 3_557 . . 3_557 ?
O19 O13 Si1 O16 -119.1(13) 3_557 . . 3_557 ?
W1 O13 Si1 O16 115.4(17) 3_557 . . 3_557 ?
W4 O13 Si1 O16 -117.7(15) 3_557 . . 3_557 ?
W5 O13 Si1 O16 -2.6(12) 3_557 . . 3_557 ?
O19 O4 Si1 O19 179.999(18) 3_557 . . . ?
O13 O4 Si1 O19 -54.2(16) 3_557 . . . ?
W6 O4 Si1 O19 178.7(15) . . . . ?
W1 O4 Si1 O19 -52.7(19) . . . . ?
W2 O4 Si1 O19 62.2(16) . . . . ?
O13 O4 Si1 O19 125.8(16) 3_557 . . 3_557 ?
W6 O4 Si1 O19 -1.3(15) . . . 3_557 ?
W1 O4 Si1 O19 127.3(19) . . . 3_557 ?
W2 O4 Si1 O19 -117.8(16) . . . 3_557 ?
O19 O4 Si1 O13 -125.8(16) 3_557 . . 3_557 ?
W6 O4 Si1 O13 -127.1(19) . . . 3_557 ?
W1 O4 Si1 O13 1.5(13) . . . 3_557 ?
W2 O4 Si1 O13 116.4(15) . . . 3_557 ?
O19 O4 Si1 O13 54.2(16) 3_557 . . . ?
O13 O4 Si1 O13 180.000(2) 3_557 . . . ?
W6 O4 Si1 O13 52.9(19) . . . . ?
W1 O4 Si1 O13 -178.5(13) . . . . ?
W2 O4 Si1 O13 -63.6(15) . . . . ?
O19 O4 Si1 O16 -61.6(14) 3_557 . . . ?
O13 O4 Si1 O16 64.2(13) 3_557 . . . ?
W6 O4 Si1 O16 -62.9(17) . . . . ?
W1 O4 Si1 O16 65.7(15) . . . . ?
W2 O4 Si1 O16 -179.4(11) . . . . ?
O19 O4 Si1 O16 118.4(14) 3_557 . . 3_557 ?
O13 O4 Si1 O16 -115.8(13) 3_557 . . 3_557 ?
W6 O4 Si1 O16 117.1(17) . . . 3_557 ?
W1 O4 Si1 O16 -114.3(15) . . . 3_557 ?
W2 O4 Si1 O16 0.6(11) . . . 3_557 ?
W3 O16 Si1 O19 -177.1(13) . . . . ?
W5 O16 Si1 O19 57.4(16) . . . . ?
W2 O16 Si1 O19 -58.7(14) 3_557 . . . ?
W3 O16 Si1 O19 2.9(13) . . . 3_557 ?
W5 O16 Si1 O19 -122.6(16) . . . 3_557 ?
W2 O16 Si1 O19 121.3(14) 3_557 . . 3_557 ?
W3 O16 Si1 O13 122.8(16) . . . 3_557 ?
W5 O16 Si1 O13 -2.7(12) . . . 3_557 ?
W2 O16 Si1 O13 -118.8(14) 3_557 . . 3_557 ?
W3 O16 Si1 O13 -57.2(16) . . . . ?
W5 O16 Si1 O13 177.3(12) . . . . ?
W2 O16 Si1 O13 61.2(14) 3_557 . . . ?
W3 O16 Si1 O4 -117.8(16) . . . 3_557 ?
W5 O16 Si1 O4 116.7(15) . . . 3_557 ?
W2 O16 Si1 O4 0.6(11) 3_557 . . 3_557 ?
W3 O16 Si1 O4 62.2(16) . . . . ?
W5 O16 Si1 O4 -63.3(15) . . . . ?
W2 O16 Si1 O4 -179.4(11) 3_557 . . . ?
C4 N2 N6 C5 6(3) . . . . ?
Co1 N2 N6 C5 175(2) . . . . ?
C1 N1 N7 C2 2(2) . . . . ?
Co1 N1 N7 C2 176.7(14) . . . . ?
C1 N1 N7 Co1 -179.2(15) . . . 2_457 ?
Co1 N1 N7 Co1 -5(2) . . . 2_457 ?
C2 N8 C1 N1 -2(3) . . . . ?
N7 N1 C1 N8 0(3) . . . . ?
Co1 N1 C1 N8 -173.7(16) . . . . ?
N1 N7 C2 N8 -4(2) . . . . ?
Co1 N7 C2 N8 177.8(14) 2_457 . . . ?
C1 N8 C2 N7 4(3) . . . . ?
N4 N4 C3 N5 -1(2) 2_457 . . . ?
Co1 N4 C3 N5 173.4(9) . . . . ?
C3 N5 C3 N4 0.5(10) 2_457 . . . ?
C5 N3 C4 N2 4(4) . . . . ?
N6 N2 C4 N3 -6(3) . . . . ?
Co1 N2 C4 N3 -173.9(17) . . . . ?
N2 N6 C5 N3 -4(3) . . . . ?
C4 N3 C5 N6 0(3) . . . . ?

_refine_diff_density_max         2.967
_refine_diff_density_min         -2.186
_refine_diff_density_rms         0.415

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_audit_block_doi                 10.5517/cc13893s
_database_code_depnum_ccdc_archive 'CCDC 1020864'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C20 H48 N30 O98 Si2 W24 Zn5'
_chemical_formula_sum            'C20 H48 N30 O98 Si2 W24 Zn5'
_chemical_formula_weight         7072.11

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   P-1

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   13.0880(5)
_cell_length_b                   13.7640(5)
_cell_length_c                   15.9630(5)
_cell_angle_alpha                99.833(5)
_cell_angle_beta                 99.520(5)
_cell_angle_gamma                101.798(5)
_cell_volume                     2713.05(5)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.90
_cell_measurement_theta_max      25.000

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.20
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.322
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3106
_exptl_absorpt_coefficient_mu    26.551
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.002
_exptl_absorpt_correction_T_max  0.004
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'

_exptl_special_details           
;
 Many kinds of restrict commands we used lead to the high R1 and wR2.   
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            14228
_diffrn_reflns_av_R_equivalents  0.0587
_diffrn_reflns_av_sigmaI/netI    0.1131
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_theta_min         1.87
_diffrn_reflns_theta_max         25.00
_reflns_number_total             9447
_reflns_number_gt                6075
_reflns_threshold_expression     >2σ(I)

_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97

_refine_special_details          
;
 The restraint command 'DELU' was refined the atoms n11 and c8, 
and the restraint command 'ISOR' was used to refine O2, O7, o8, O9,
o10, O12, O13, O14, O15, O17, o22, O25, O28, O29, O31, O33, O35, O39, N1, N2,
n3, N6, N7, n8, C1, C2, C3, C4, C5, C6, c7, C8 and C21 atoms.
The restraint order 'SIMU' was refined the atoms 
n15, c9, c10, N16, N13, n11, n10 and c8.
The 'DFIX' command was used to bind N13, N26,C9, N15,C10,O1W and O5w.
 The 'OMIT' order was used to confirm the data completeless.
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2σ(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0512P)²+31.2380P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00016(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         9447
_refine_ls_number_parameters     809
_refine_ls_number_restraints     503
_refine_ls_R_factor_all          0.1062
_refine_ls_R_factor_gt           0.0574
_refine_ls_wR_factor_ref         0.1401
_refine_ls_wR_factor_gt          0.1156
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_restrained_S_all      0.983
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.1111(15) 0.8456(13) 0.6334(11) 0.032(5) Uani 1 1 d . . .
O2 O 0.2593(13) 0.9750(11) 0.9377(10) 0.019(4) Uani 1 1 d U . .
O3 O 0.2181(13) 0.8183(12) 0.7906(11) 0.022(4) Uani 1 1 d . . .
O4 O 0.3324(13) 0.8620(11) 0.6776(10) 0.019(4) Uani 1 1 d . . .
O5 O 0.4075(12) 0.9285(10) 0.8410(10) 0.015(4) Uani 1 1 d . . .
O6 O 0.5286(14) 0.8790(12) 0.6440(11) 0.026(4) Uani 1 1 d . . .
O7 O 0.6084(12) 0.9478(11) 0.8133(10) 0.015(4) Uani 1 1 d U . .
O6W O -0.2616(14) 0.1340(13) 0.7296(12) 0.037(5) Uani 1 1 d . . .
H6WC H -0.2382 0.1211 0.7784 0.044 Uiso 1 1 d R . .
H6WD H -0.2936 0.1814 0.7385 0.044 Uiso 1 1 d R . .
O8 O 0.0930(12) 0.6591(11) 0.6751(10) 0.018(4) Uani 1 1 d U . .
O7W O -0.1793(18) 0.2890(15) 0.6354(16) 0.060(7) Uani 1 1 d . . .
O9 O 0.4193(13) 0.8805(11) 0.9978(10) 0.018(4) Uani 1 1 d U . .
O8W O 0.1941(15) 0.1561(12) 0.9163(12) 0.032(5) Uani 1 1 d . . .
H8WC H 0.2203 0.1050 0.9202 0.039 Uiso 1 1 d R . .
H8WD H 0.1359 0.1465 0.9341 0.039 Uiso 1 1 d R . .
O10 O 0.2117(13) 0.6998(11) 0.5589(10) 0.021(4) Uani 1 1 d U . .
O9W O 0.2666(14) 0.0965(14) 0.7520(12) 0.035(5) Uani 1 1 d . . .
H9WC H 0.2993 0.1311 0.8021 0.042 Uiso 1 1 d R . .
O11 O 0.6243(16) 0.7560(12) 0.5469(11) 0.030(5) Uani 1 1 d . . .
O12 O 0.2527(14) 0.5469(12) 0.4454(10) 0.024(4) Uani 1 1 d U . .
O13 O 0.4138(12) 0.6887(11) 0.5710(10) 0.017(4) Uani 1 1 d U . .
O14 O 0.6776(13) 0.8004(11) 0.7246(10) 0.021(4) Uani 1 1 d U . .
O15 O 0.1598(13) 0.5133(11) 0.5842(10) 0.022(4) Uani 1 1 d U . .
O16 O 0.2908(13) 0.6555(11) 0.6999(10) 0.014(4) Uani 1 1 d . . .
O17 O 0.5900(13) 0.8366(11) 0.9367(10) 0.020(4) Uani 1 1 d U . .
O18 O 0.5716(13) 0.8148(12) 1.1081(10) 0.025(4) Uani 1 1 d . . .
O19 O 0.7888(13) 0.8915(11) 0.8920(11) 0.024(4) Uani 1 1 d . . .
O20 O 0.1574(13) 0.5976(10) 0.8197(10) 0.018(4) Uani 1 1 d . . .
O21 O 0.3716(12) 0.7242(10) 0.8715(10) 0.013(3) Uani 1 1 d U . .
O22 O 0.4886(13) 0.7679(11) 0.7552(11) 0.022(4) Uani 1 1 d U . .
O23 O 0.3673(13) 0.5080(11) 0.5970(10) 0.021(4) Uani 1 1 d . . .
O24 O 0.5608(13) 0.6129(12) 0.6474(12) 0.026(4) Uani 1 1 d . . .
O25 O 0.4393(12) 0.5786(11) 0.7808(10) 0.017(4) Uani 1 1 d U . .
O26 O 0.2260(13) 0.4571(11) 0.7336(11) 0.022(4) Uani 1 1 d . . .
O27 O 0.5379(13) 0.6551(11) 0.9616(10) 0.022(4) Uani 1 1 d . . .
O28 O 0.3043(13) 0.5250(11) 0.8945(11) 0.022(4) Uani 1 1 d U . .
O29 O 0.6515(12) 0.6946(10) 0.8491(10) 0.017(4) Uani 1 1 d U . .
O30 O 0.5319(14) 0.4034(13) 0.5913(12) 0.032(5) Uani 1 1 d U . .
O31 O 0.6002(12) 0.5016(11) 0.7667(10) 0.017(4) Uani 1 1 d U . .
O32 O 0.4003(13) 0.3909(11) 0.7105(10) 0.019(4) Uani 1 1 d . . .
O33 O 0.4812(12) 0.4573(11) 0.8813(10) 0.015(4) Uani 1 1 d U . .
O34 O 0.0090(14) 0.4564(12) 0.6846(12) 0.031(5) Uani 1 1 d . . .
O35 O 0.4800(14) 1.0526(12) 0.7286(11) 0.029(4) Uani 1 1 d U . .
O36 O 0.6975(14) 0.5479(12) 0.9398(11) 0.030(5) Uani 1 1 d . . .
O37 O 0.2859(13) 0.3158(12) 0.8283(12) 0.023(4) Uani 1 1 d . . .
O38 O 0.3702(13) 0.6922(11) 1.0237(10) 0.017(4) Uani 1 1 d . . .
O39 O 0.2212(12) 0.7679(10) 0.9453(10) 0.014(4) Uani 1 1 d U . .
O40 O 0.1564(12) 0.5824(11) 0.9910(10) 0.018(4) Uani 1 1 d . . .
Si1 Si 0.3983(5) 0.6822(4) 0.7774(4) 0.0077(13) Uani 1 1 d U . .
W1 W 0.19676(9) 0.77653(7) 0.66827(7) 0.0187(3) Uani 1 1 d . . .
W2 W 0.47390(9) 0.93209(7) 0.74148(7) 0.0197(3) Uani 1 1 d . . .
W3 W 0.31021(8) 0.87363(7) 0.90214(7) 0.0170(3) Uani 1 1 d . . .
W4 W 0.28309(9) 0.59215(7) 0.55451(6) 0.0200(3) Uani 1 1 d . . .
W5 W 0.13202(8) 0.53753(7) 0.69855(7) 0.0180(3) Uani 1 1 d . . .
W6 W 0.24572(8) 0.63414(7) 0.93291(6) 0.0152(2) Uani 1 1 d . . .
W7 W 0.49607(8) 0.77573(7) 1.00373(6) 0.0164(3) Uani 1 1 d . . .
W8 W 0.66006(8) 0.83241(7) 0.84286(7) 0.0190(3) Uani 1 1 d . . .
W9 W 0.55988(9) 0.74731(7) 0.62840(7) 0.0212(3) Uani 1 1 d . . .
W10 W 0.59164(8) 0.57285(7) 0.88054(7) 0.0177(3) Uani 1 1 d . . .
W11 W 0.49230(9) 0.48628(7) 0.66470(7) 0.0183(3) Uani 1 1 d . . .
W12 W 0.34305(8) 0.43199(7) 0.80925(7) 0.0157(2) Uani 1 1 d . . .
Zn1 Zn -0.1239(2) 0.1606(2) 0.6732(2) 0.0254(7) Uani 1 1 d . . .
Zn2 Zn 0.1532(2) 0.17365(19) 0.78530(19) 0.0200(7) Uani 1 1 d . . .
Zn3 Zn 0.0000 0.5000 1.0000 0.0568(17) Uani 1 2 d S . .
N1 N 0.0152(18) 0.2070(15) 0.6219(14) 0.029(3) Uani 1 1 d U . .
N2 N 0.1180(18) 0.2019(15) 0.6538(14) 0.026(3) Uani 1 1 d U . .
N3 N 0.1223(18) 0.2694(16) 0.5388(15) 0.033(4) Uani 1 1 d U . .
H3 H 0.1427 0.2940 0.4966 0.039 Uiso 1 1 calc R . .
N7 N -0.0429(18) 0.2602(15) 0.7903(14) 0.029(3) Uani 1 1 d U . .
N8 N 0.0638(18) 0.2685(15) 0.8306(15) 0.029(3) Uani 1 1 d U . .
N9 N 0.004(2) 0.3818(17) 0.9089(16) 0.041(4) Uani 1 1 d U . .
N10 N -0.2196(18) 0.0630(15) 0.5593(14) 0.029(3) Uani 1 1 d U . .
N11 N -0.1903(19) 0.0205(16) 0.4811(15) 0.034(3) Uani 1 1 d U . .
N12 N -0.3532(19) -0.0429(16) 0.4652(15) 0.034(4) Uani 1 1 d U . .
H12 H -0.4168 -0.0788 0.4422 0.041 Uiso 1 1 calc R . .
C1 C 0.021(2) 0.2480(19) 0.5552(19) 0.035(6) Uani 1 1 d U . .
H1 H -0.0374 0.2616 0.5216 0.042 Uiso 1 1 calc R . .
C2 C 0.182(3) 0.243(2) 0.6041(19) 0.038(6) Uani 1 1 d U . .
H2 H 0.2555 0.2518 0.6137 0.045 Uiso 1 1 calc R . .
C3 C -0.076(2) 0.3266(19) 0.8431(18) 0.033(5) Uani 1 1 d U . .
H3A H -0.1462 0.3341 0.8358 0.039 Uiso 1 1 calc R . .
C4 C 0.089(3) 0.345(2) 0.897(2) 0.042(5) Uani 1 1 d U . .
H4 H 0.1568 0.3708 0.9314 0.051 Uiso 1 1 calc R . .
C7 C -0.325(2) 0.0189(19) 0.5436(18) 0.030(5) Uani 1 1 d U . .
H7 H -0.3701 0.0298 0.5814 0.036 Uiso 1 1 calc R . .
C8 C -0.270(2) -0.0412(18) 0.4279(18) 0.027(4) Uani 1 1 d U . .
H8 H -0.2696 -0.0779 0.3734 0.033 Uiso 1 1 calc R . .
N13 N 0.144(2) 0.4555(17) 1.1765(18) 0.079(5) Uani 1 1 d DU . .
H13 H 0.1791 0.5180 1.1936 0.095 Uiso 1 1 calc R . .
N15 N 0.084(2) 0.2966(17) 1.1792(19) 0.076(5) Uani 1 1 d DU . .
C10 C 0.154(3) 0.384(2) 1.2197(19) 0.076(5) Uani 1 1 d DU . .
H10 H 0.2033 0.3922 1.2713 0.091 Uiso 1 1 calc R . .
C9 C 0.033(3) 0.3208(19) 1.110(2) 0.072(4) Uani 1 1 d DU . .
H9 H -0.0242 0.2765 1.0702 0.086 Uiso 1 1 calc R . .
N16 N 0.075(2) 0.4185(18) 1.1041(16) 0.067(4) Uani 1 1 d DU . .
O2W O -0.5345(18) -0.1926(14) 0.3944(14) 0.056(7) Uani 1 1 d . . .
O3W O 0.1296(18) 0.3316(15) 0.3834(15) 0.061(7) Uani 1 1 d . . .
O4W O -0.364(2) 0.2965(18) 0.7877(16) 0.083(9) Uani 1 1 d . . .
O5W O 0.003(2) 0.100(2) 0.9802(18) 0.092(10) Uani 1 1 d . . .
N4 N -0.0712(18) 0.0318(15) 0.7092(14) 0.029(3) Uani 1 1 d U . .
C5 C -0.123(2) -0.061(2) 0.7073(19) 0.036(6) Uani 1 1 d U . .
H5 H -0.1938 -0.0876 0.6794 0.043 Uiso 1 1 calc R . .
N6 N -0.0659(18) -0.1105(16) 0.7476(15) 0.034(4) Uani 1 1 d U . .
H6 H -0.0860 -0.1713 0.7552 0.041 Uiso 1 1 calc R . .
N5 N 0.0273(18) 0.0409(15) 0.7549(14) 0.028(3) Uani 1 1 d U . .
C6 C 0.034(2) -0.046(2) 0.7763(18) 0.034(6) Uani 1 1 d U . .
H6A H 0.0950 -0.0611 0.8051 0.041 Uiso 1 1 calc R . .
O1W O -0.2008(19) 0.1147(16) 0.8947(14) 0.064(7) Uani 1 1 d . . .


_geom_special_details            
;
 All s.u.'s (except the s.u. in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell s.u.'s are taken
 into account individually in the estimation of s.u.'s in distances, angles
 and torsion angles; correlations between s.u.'s in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell s.u.'s is used for estimating s.u.'s involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 W1 1.697(17) . ?
O2 W3 1.717(15) . ?
O3 W1 1.895(16) . ?
O3 W3 1.912(16) . ?
O4 W1 1.886(15) . ?
O4 W2 1.926(15) . ?
O5 W3 1.848(15) . ?
O5 W2 1.936(16) . ?
O6 W2 1.913(16) . ?
O6 W9 1.923(17) . ?
O7 W2 1.885(15) . ?
O7 W8 1.947(16) . ?
O6W Zn1 2.137(19) . ?
O6W H6WC 0.8500 . ?
O6W H6WD 0.8500 . ?
O8 W1 1.919(14) . ?
O8 W5 1.923(15) . ?
O7W Zn1 2.182(19) . ?
O9 W3 1.885(15) . ?
O9 W7 1.925(15) . ?
O8W Zn2 2.139(18) . ?
O8W H8WC 0.8500 . ?
O8W H8WD 0.8499 . ?
O10 W4 1.904(16) . ?
O10 W1 1.942(16) . ?
O9W Zn2 2.080(18) . ?
O9W H9WC 0.8500 . ?
O11 W9 1.671(17) . ?
O12 W4 1.696(16) . ?
O13 W4 1.888(15) . ?
O13 W9 1.919(15) . ?
O14 W9 1.908(15) . ?
O14 W8 1.926(16) . ?
O15 W5 1.907(16) . ?
O15 W4 1.929(16) . ?
O16 Si1 1.644(17) . ?
O16 W4 2.313(15) . ?
O16 W1 2.338(15) . ?
O16 W5 2.356(15) . ?
O17 W8 1.879(16) . ?
O17 W7 1.918(16) . ?
O18 W7 1.725(16) . ?
O19 W8 1.703(17) . ?
O20 W6 1.902(15) . ?
O20 W5 1.914(15) . ?
O21 Si1 1.635(16) . ?
O21 W6 2.307(15) . ?
O21 W7 2.343(15) . ?
O21 W3 2.362(14) . ?
O22 Si1 1.621(16) . ?
O22 W8 2.346(16) . ?
O22 W2 2.351(16) . ?
O22 W9 2.363(17) . ?
O23 W4 1.887(17) . ?
O23 W11 1.913(17) . ?
O24 W11 1.878(15) . ?
O24 W9 1.927(16) . ?
O25 Si1 1.629(16) . ?
O25 W12 2.309(15) . ?
O25 W11 2.348(15) . ?
O25 W10 2.361(16) . ?
O26 W5 1.896(17) . ?
O26 W12 1.916(17) . ?
O27 W10 1.891(16) . ?
O27 W7 1.903(16) . ?
O28 W6 1.880(16) . ?
O28 W12 1.910(17) . ?
O29 W10 1.885(14) . ?
O29 W8 1.898(14) . ?
O30 W11 1.711(18) . ?
O31 W11 1.921(16) . ?
O31 W10 1.944(16) . ?
O32 W12 1.905(16) . ?
O32 W11 1.918(15) . ?
O33 W12 1.906(16) . ?
O33 W10 1.922(14) . ?
O34 W5 1.717(17) . ?
O35 W2 1.693(15) . ?
O36 W10 1.675(18) . ?
O37 W12 1.720(15) . ?
O37 Zn2 2.253(16) . ?
O38 W7 1.913(15) . ?
O38 W6 1.920(15) . ?
O39 W6 1.915(14) . ?
O39 W3 1.965(14) . ?
O40 W6 1.725(14) . ?
O40 Zn3 2.169(14) . ?
Zn1 N7 2.09(2) . ?
Zn1 N10 2.10(2) . ?
Zn1 N1 2.14(2) . ?
Zn1 N4 2.16(2) . ?
Zn2 N8 2.04(2) . ?
Zn2 N5 2.12(2) . ?
Zn2 N2 2.19(2) . ?
Zn2 H9WC 2.1001 . ?
Zn3 N9 2.00(2) . ?
Zn3 N9 2.00(2) 2_567 ?
Zn3 O40 2.169(14) 2_567 ?
Zn3 N16 2.35(2) . ?
Zn3 N16 2.35(2) 2_567 ?
N1 C1 1.29(3) . ?
N1 N2 1.38(3) . ?
N2 C2 1.35(3) . ?
N3 C2 1.34(3) . ?
N3 C1 1.38(3) . ?
N3 H3 0.8600 . ?
N7 C3 1.33(3) . ?
N7 N8 1.41(3) . ?
N8 C4 1.30(3) . ?
N9 C4 1.34(3) . ?
N9 C3 1.35(3) . ?
N10 C7 1.35(3) . ?
N10 N11 1.43(3) . ?
N11 C8 1.28(3) . ?
N12 C8 1.32(3) . ?
N12 C7 1.33(3) . ?
N12 H12 0.8600 . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3A 0.9300 . ?
C4 H4 0.9300 . ?
C7 H7 0.9300 . ?
C8 H8 0.9300 . ?
N13 N16 1.299(17) . ?
N13 C10 1.314(18) . ?
N13 H13 0.8600 . ?
N15 C9 1.316(18) . ?
N15 C10 1.340(18) . ?
C10 H10 0.9300 . ?
C9 N16 1.371(18) . ?
C9 H9 0.9300 . ?
N4 C5 1.31(3) . ?
N4 N5 1.34(3) . ?
C5 N6 1.28(3) . ?
C5 H5 0.9300 . ?
N6 C6 1.38(3) . ?
N6 H6 0.8600 . ?
N5 C6 1.31(3) . ?
C6 H6A 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W1 O3 W3 150.9(9) . . ?
W1 O4 W2 151.9(9) . . ?
W3 O5 W2 154.7(8) . . ?
W2 O6 W9 122.1(9) . . ?
W2 O7 W8 122.2(7) . . ?
Zn1 O6W H6WC 103.8 . . ?
Zn1 O6W H6WD 118.5 . . ?
H6WC O6W H6WD 108.1 . . ?
W1 O8 W5 122.2(8) . . ?
W3 O9 W7 122.4(8) . . ?
Zn2 O8W H8WC 112.8 . . ?
Zn2 O8W H8WD 105.7 . . ?
H8WC O8W H8WD 108.1 . . ?
W4 O10 W1 121.8(8) . . ?
Zn2 O9W H9WC 79.6 . . ?
W4 O13 W9 151.9(9) . . ?
W9 O14 W8 122.8(9) . . ?
W5 O15 W4 121.9(8) . . ?
Si1 O16 W4 125.1(8) . . ?
Si1 O16 W1 122.8(8) . . ?
W4 O16 W1 92.5(5) . . ?
Si1 O16 W5 123.7(8) . . ?
W4 O16 W5 91.8(5) . . ?
W1 O16 W5 91.5(6) . . ?
W8 O17 W7 152.9(8) . . ?
W6 O20 W5 150.8(10) . . ?
Si1 O21 W6 124.3(8) . . ?
Si1 O21 W7 125.0(8) . . ?
W6 O21 W7 92.2(5) . . ?
Si1 O21 W3 122.9(8) . . ?
W6 O21 W3 92.5(5) . . ?
W7 O21 W3 90.4(5) . . ?
Si1 O22 W8 123.1(9) . . ?
Si1 O22 W2 125.8(9) . . ?
W8 O22 W2 91.2(5) . . ?
Si1 O22 W9 124.6(8) . . ?
W8 O22 W9 91.2(6) . . ?
W2 O22 W9 90.8(6) . . ?
W4 O23 W11 152.6(9) . . ?
W11 O24 W9 151.7(10) . . ?
Si1 O25 W12 125.4(9) . . ?
Si1 O25 W11 124.1(9) . . ?
W12 O25 W11 91.8(5) . . ?
Si1 O25 W10 122.9(8) . . ?
W12 O25 W10 90.9(5) . . ?
W11 O25 W10 91.9(5) . . ?
W5 O26 W12 153.5(9) . . ?
W10 O27 W7 152.8(9) . . ?
W6 O28 W12 154.6(10) . . ?
W10 O29 W8 153.0(9) . . ?
W11 O31 W10 122.3(8) . . ?
W12 O32 W11 122.0(7) . . ?
W12 O33 W10 120.9(8) . . ?
W12 O37 Zn2 147.5(10) . . ?
W7 O38 W6 121.9(8) . . ?
W6 O39 W3 120.7(8) . . ?
W6 O40 Zn3 152.0(9) . . ?
O22 Si1 O25 110.6(9) . . ?
O22 Si1 O21 109.9(8) . . ?
O25 Si1 O21 109.0(8) . . ?
O22 Si1 O16 108.4(8) . . ?
O25 Si1 O16 108.3(8) . . ?
O21 Si1 O16 110.6(9) . . ?
O1 W1 O4 103.6(8) . . ?
O1 W1 O3 101.7(8) . . ?
O4 W1 O3 86.8(7) . . ?
O1 W1 O8 98.1(8) . . ?
O4 W1 O8 158.3(7) . . ?
O3 W1 O8 88.1(7) . . ?
O1 W1 O10 101.4(8) . . ?
O4 W1 O10 89.0(7) . . ?
O3 W1 O10 156.8(7) . . ?
O8 W1 O10 87.5(7) . . ?
O1 W1 O16 169.3(7) . . ?
O4 W1 O16 85.2(6) . . ?
O3 W1 O16 84.7(6) . . ?
O8 W1 O16 73.4(6) . . ?
O10 W1 O16 72.2(6) . . ?
O35 W2 O7 101.0(8) . . ?
O35 W2 O6 100.8(8) . . ?
O7 W2 O6 88.9(7) . . ?
O35 W2 O4 102.2(8) . . ?
O7 W2 O4 156.7(6) . . ?
O6 W2 O4 88.6(7) . . ?
O35 W2 O5 102.0(7) . . ?
O7 W2 O5 90.1(6) . . ?
O6 W2 O5 156.9(6) . . ?
O4 W2 O5 83.2(6) . . ?
O35 W2 O22 172.3(8) . . ?
O7 W2 O22 73.8(6) . . ?
O6 W2 O22 73.7(6) . . ?
O4 W2 O22 83.3(6) . . ?
O5 W2 O22 83.9(6) . . ?
O2 W3 O5 102.3(7) . . ?
O2 W3 O9 102.2(7) . . ?
O5 W3 O9 91.9(7) . . ?
O2 W3 O3 100.8(7) . . ?
O5 W3 O3 85.2(7) . . ?
O9 W3 O3 156.9(7) . . ?
O2 W3 O39 99.7(7) . . ?
O5 W3 O39 157.7(6) . . ?
O9 W3 O39 86.9(7) . . ?
O3 W3 O39 87.1(6) . . ?
O2 W3 O21 171.1(6) . . ?
O5 W3 O21 85.9(6) . . ?
O9 W3 O21 73.7(6) . . ?
O3 W3 O21 83.2(6) . . ?
O39 W3 O21 72.4(6) . . ?
O12 W4 O23 103.8(8) . . ?
O12 W4 O13 102.7(7) . . ?
O23 W4 O13 85.4(6) . . ?
O12 W4 O10 98.7(8) . . ?
O23 W4 O10 157.5(7) . . ?
O13 W4 O10 89.0(7) . . ?
O12 W4 O15 98.9(7) . . ?
O23 W4 O15 90.4(7) . . ?
O13 W4 O15 158.3(7) . . ?
O10 W4 O15 86.9(7) . . ?
O12 W4 O16 169.1(7) . . ?
O23 W4 O16 84.4(6) . . ?
O13 W4 O16 85.0(6) . . ?
O10 W4 O16 73.4(6) . . ?
O15 W4 O16 73.4(6) . . ?
O34 W5 O26 102.3(7) . . ?
O34 W5 O15 101.7(8) . . ?
O26 W5 O15 90.2(7) . . ?
O34 W5 O20 100.8(8) . . ?
O26 W5 O20 85.2(7) . . ?
O15 W5 O20 157.5(7) . . ?
O34 W5 O8 101.4(8) . . ?
O26 W5 O8 156.1(6) . . ?
O15 W5 O8 87.7(7) . . ?
O20 W5 O8 87.7(6) . . ?
O34 W5 O16 172.0(7) . . ?
O26 W5 O16 83.8(6) . . ?
O15 W5 O16 72.8(6) . . ?
O20 W5 O16 84.8(6) . . ?
O8 W5 O16 72.9(6) . . ?
O40 W6 O28 102.7(7) . . ?
O40 W6 O20 100.0(7) . . ?
O28 W6 O20 85.2(7) . . ?
O40 W6 O39 99.4(7) . . ?
O28 W6 O39 157.8(7) . . ?
O20 W6 O39 89.7(6) . . ?
O40 W6 O38 100.8(7) . . ?
O28 W6 O38 90.4(7) . . ?
O20 W6 O38 159.2(7) . . ?
O39 W6 O38 86.6(6) . . ?
O40 W6 O21 171.6(6) . . ?
O28 W6 O21 83.6(6) . . ?
O20 W6 O21 86.0(6) . . ?
O39 W6 O21 74.5(6) . . ?
O38 W6 O21 73.4(6) . . ?
O18 W7 O27 102.4(7) . . ?
O18 W7 O38 100.5(7) . . ?
O27 W7 O38 88.3(7) . . ?
O18 W7 O17 102.7(7) . . ?
O27 W7 O17 84.4(7) . . ?
O38 W7 O17 156.7(6) . . ?
O18 W7 O9 101.6(7) . . ?
O27 W7 O9 156.0(7) . . ?
O38 W7 O9 87.7(7) . . ?
O17 W7 O9 90.0(7) . . ?
O18 W7 O21 171.4(7) . . ?
O27 W7 O21 82.8(6) . . ?
O38 W7 O21 72.6(6) . . ?
O17 W7 O21 84.5(6) . . ?
O9 W7 O21 73.5(6) . . ?
O19 W8 O17 102.7(7) . . ?
O19 W8 O29 103.5(7) . . ?
O17 W8 O29 84.9(7) . . ?
O19 W8 O14 99.2(7) . . ?
O17 W8 O14 158.1(7) . . ?
O29 W8 O14 89.1(6) . . ?
O19 W8 O7 100.1(7) . . ?
O17 W8 O7 89.9(7) . . ?
O29 W8 O7 156.4(6) . . ?
O14 W8 O7 87.2(7) . . ?
O19 W8 O22 169.4(7) . . ?
O17 W8 O22 85.4(6) . . ?
O29 W8 O22 83.8(6) . . ?
O14 W8 O22 73.0(6) . . ?
O7 W8 O22 72.8(6) . . ?
O11 W9 O14 99.5(8) . . ?
O11 W9 O13 103.9(8) . . ?
O14 W9 O13 156.5(7) . . ?
O11 W9 O6 98.6(7) . . ?
O14 W9 O6 88.4(7) . . ?
O13 W9 O6 88.9(7) . . ?
O11 W9 O24 103.3(8) . . ?
O14 W9 O24 88.8(7) . . ?
O13 W9 O24 85.0(7) . . ?
O6 W9 O24 158.0(7) . . ?
O11 W9 O22 168.8(7) . . ?
O14 W9 O22 72.9(6) . . ?
O13 W9 O22 83.9(6) . . ?
O6 W9 O22 73.3(6) . . ?
O24 W9 O22 85.1(7) . . ?
O36 W10 O29 102.7(8) . . ?
O36 W10 O27 104.7(8) . . ?
O29 W10 O27 85.9(7) . . ?
O36 W10 O33 101.0(8) . . ?
O29 W10 O33 156.3(7) . . ?
O27 W10 O33 90.1(7) . . ?
O36 W10 O31 98.7(8) . . ?
O29 W10 O31 87.5(6) . . ?
O27 W10 O31 156.6(7) . . ?
O33 W10 O31 87.0(6) . . ?
O36 W10 O25 169.5(7) . . ?
O29 W10 O25 83.0(6) . . ?
O27 W10 O25 84.4(6) . . ?
O33 W10 O25 73.3(6) . . ?
O31 W10 O25 72.5(6) . . ?
O30 W11 O24 102.3(8) . . ?
O30 W11 O23 102.5(8) . . ?
O24 W11 O23 85.2(7) . . ?
O30 W11 O32 99.5(7) . . ?
O24 W11 O32 158.1(7) . . ?
O23 W11 O32 88.0(6) . . ?
O30 W11 O31 100.8(8) . . ?
O24 W11 O31 90.2(7) . . ?
O23 W11 O31 156.7(7) . . ?
O32 W11 O31 87.9(6) . . ?
O30 W11 O25 169.9(7) . . ?
O24 W11 O25 86.1(7) . . ?
O23 W11 O25 83.7(6) . . ?
O32 W11 O25 72.5(6) . . ?
O31 W11 O25 73.2(6) . . ?
O37 W12 O32 100.7(7) . . ?
O37 W12 O33 100.0(7) . . ?
O32 W12 O33 89.5(7) . . ?
O37 W12 O28 102.8(7) . . ?
O32 W12 O28 156.3(6) . . ?
O33 W12 O28 89.8(7) . . ?
O37 W12 O26 101.2(7) . . ?
O32 W12 O26 89.1(7) . . ?
O33 W12 O26 158.7(6) . . ?
O28 W12 O26 83.1(7) . . ?
O37 W12 O25 172.2(7) . . ?
O32 W12 O25 73.6(6) . . ?
O33 W12 O25 74.9(6) . . ?
O28 W12 O25 83.3(6) . . ?
O26 W12 O25 84.3(6) . . ?
N7 Zn1 N10 174.2(9) . . ?
N7 Zn1 O6W 88.0(8) . . ?
N10 Zn1 O6W 86.7(8) . . ?
N7 Zn1 N1 87.5(9) . . ?
N10 Zn1 N1 97.6(8) . . ?
O6W Zn1 N1 172.9(8) . . ?
N7 Zn1 N4 94.1(8) . . ?
N10 Zn1 N4 88.5(8) . . ?
O6W Zn1 N4 93.7(8) . . ?
N1 Zn1 N4 92.1(8) . . ?
N7 Zn1 O7W 86.8(9) . . ?
N10 Zn1 O7W 90.6(9) . . ?
O6W Zn1 O7W 85.9(8) . . ?
N1 Zn1 O7W 88.3(9) . . ?
N4 Zn1 O7W 179.1(9) . . ?
N8 Zn2 O9W 170.1(8) . . ?
N8 Zn2 N5 94.9(9) . . ?
O9W Zn2 N5 94.3(8) . . ?
N8 Zn2 O8W 86.4(8) . . ?
O9W Zn2 O8W 89.7(7) . . ?
N5 Zn2 O8W 91.1(8) . . ?
N8 Zn2 N2 92.4(8) . . ?
O9W Zn2 N2 90.9(8) . . ?
N5 Zn2 N2 92.6(8) . . ?
O8W Zn2 N2 176.2(7) . . ?
N8 Zn2 O37 83.1(7) . . ?
O9W Zn2 O37 87.5(7) . . ?
N5 Zn2 O37 175.6(8) . . ?
O8W Zn2 O37 84.9(7) . . ?
N2 Zn2 O37 91.4(7) . . ?
N8 Zn2 H9WC 147.6 . . ?
O9W Zn2 H9WC 23.5 . . ?
N5 Zn2 H9WC 108.7 . . ?
O8W Zn2 H9WC 71.6 . . ?
N2 Zn2 H9WC 108.0 . . ?
O37 Zn2 H9WC 71.7 . . ?
N9 Zn3 N9 180 . 2_567 ?
N9 Zn3 O40 91.7(8) . . ?
N9 Zn3 O40 88.3(8) 2_567 . ?
N9 Zn3 O40 88.3(8) . 2_567 ?
N9 Zn3 O40 91.7(8) 2_567 2_567 ?
O40 Zn3 O40 180 . 2_567 ?
N9 Zn3 N16 87.6(10) . . ?
N9 Zn3 N16 92.4(10) 2_567 . ?
O40 Zn3 N16 91.8(8) . . ?
O40 Zn3 N16 88.2(8) 2_567 . ?
N9 Zn3 N16 92.4(10) . 2_567 ?
N9 Zn3 N16 87.6(10) 2_567 2_567 ?
O40 Zn3 N16 88.2(8) . 2_567 ?
O40 Zn3 N16 91.8(8) 2_567 2_567 ?
N16 Zn3 N16 180 . 2_567 ?
C1 N1 N2 105(2) . . ?
C1 N1 Zn1 127(2) . . ?
N2 N1 Zn1 127.6(16) . . ?
C2 N2 N1 108(2) . . ?
C2 N2 Zn2 131.8(19) . . ?
N1 N2 Zn2 117.2(16) . . ?
C2 N3 C1 104(2) . . ?
C2 N3 H3 128.1 . . ?
C1 N3 H3 128.1 . . ?
C3 N7 N8 105(2) . . ?
C3 N7 Zn1 130(2) . . ?
N8 N7 Zn1 125.0(17) . . ?
C4 N8 N7 107(2) . . ?
C4 N8 Zn2 130(2) . . ?
N7 N8 Zn2 122.9(16) . . ?
C4 N9 C3 105(3) . . ?
C4 N9 Zn3 127(2) . . ?
C3 N9 Zn3 127(2) . . ?
C7 N10 N11 102(2) . . ?
C7 N10 Zn1 128.2(19) . . ?
N11 N10 Zn1 129.8(16) . . ?
C8 N11 N10 112(2) . . ?
C8 N12 C7 110(2) . . ?
C8 N12 H12 124.8 . . ?
C7 N12 H12 124.8 . . ?
N1 C1 N3 113(3) . . ?
N1 C1 H1 123.4 . . ?
N3 C1 H1 123.4 . . ?
N3 C2 N2 109(3) . . ?
N3 C2 H2 125.3 . . ?
N2 C2 H2 125.3 . . ?
N7 C3 N9 111(3) . . ?
N7 C3 H3A 124.4 . . ?
N9 C3 H3A 124.4 . . ?
N8 C4 N9 111(3) . . ?
N8 C4 H4 124.3 . . ?
N9 C4 H4 124.3 . . ?
N12 C7 N10 109(3) . . ?
N12 C7 H7 125.4 . . ?
N10 C7 H7 125.4 . . ?
N11 C8 N12 107(2) . . ?
N11 C8 H8 126.6 . . ?
N12 C8 H8 126.6 . . ?
N16 N13 C10 110.2(18) . . ?
N16 N13 H13 124.9 . . ?
C10 N13 H13 124.9 . . ?
C9 N15 C10 103.0(17) . . ?
N13 C10 N15 110.5(18) . . ?
N13 C10 H10 124.8 . . ?
N15 C10 H10 124.8 . . ?
N15 C9 N16 112.4(18) . . ?
N15 C9 H9 123.8 . . ?
N16 C9 H9 123.8 . . ?
N13 N16 C9 103.4(17) . . ?
N13 N16 Zn3 130.6(18) . . ?
C9 N16 Zn3 124.4(18) . . ?
C5 N4 N5 105(2) . . ?
C5 N4 Zn1 132(2) . . ?
N5 N4 Zn1 122.1(15) . . ?
N6 C5 N4 113(3) . . ?
N6 C5 H5 123.4 . . ?
N4 C5 H5 123.4 . . ?
C5 N6 C6 105(2) . . ?
C5 N6 H6 127.3 . . ?
C6 N6 H6 127.3 . . ?
C6 N5 N4 109(2) . . ?
C6 N5 Zn2 125(2) . . ?
N4 N5 Zn2 125.3(16) . . ?
N5 C6 N6 107(3) . . ?
N5 C6 H6A 126.7 . . ?
N6 C6 H6A 126.7 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
W8 O22 Si1 O25 -60.2(12) . . . . ?
W2 O22 Si1 O25 179.8(9) . . . . ?
W9 O22 Si1 O25 58.6(12) . . . . ?
W8 O22 Si1 O21 60.2(12) . . . . ?
W2 O22 Si1 O21 -59.8(12) . . . . ?
W9 O22 Si1 O21 178.9(9) . . . . ?
W8 O22 Si1 O16 -178.8(9) . . . . ?
W2 O22 Si1 O16 61.2(12) . . . . ?
W9 O22 Si1 O16 -60.0(12) . . . . ?
W12 O25 Si1 O22 -179.8(9) . . . . ?
W11 O25 Si1 O22 -57.9(12) . . . . ?
W10 O25 Si1 O22 61.3(12) . . . . ?
W12 O25 Si1 O21 59.3(12) . . . . ?
W11 O25 Si1 O21 -178.8(8) . . . . ?
W10 O25 Si1 O21 -59.7(11) . . . . ?
W12 O25 Si1 O16 -61.1(12) . . . . ?
W11 O25 Si1 O16 60.8(11) . . . . ?
W10 O25 Si1 O16 179.9(8) . . . . ?
W6 O21 Si1 O22 178.4(9) . . . . ?
W7 O21 Si1 O22 -59.4(11) . . . . ?
W3 O21 Si1 O22 58.2(12) . . . . ?
W6 O21 Si1 O25 -60.2(12) . . . . ?
W7 O21 Si1 O25 62.0(11) . . . . ?
W3 O21 Si1 O25 179.5(8) . . . . ?
W6 O21 Si1 O16 58.8(11) . . . . ?
W7 O21 Si1 O16 -179.0(8) . . . . ?
W3 O21 Si1 O16 -61.5(11) . . . . ?
W4 O16 Si1 O22 60.0(11) . . . . ?
W1 O16 Si1 O22 -61.1(11) . . . . ?
W5 O16 Si1 O22 -179.0(9) . . . . ?
W4 O16 Si1 O25 -60.0(11) . . . . ?
W1 O16 Si1 O25 178.9(8) . . . . ?
W5 O16 Si1 O25 61.0(11) . . . . ?
W4 O16 Si1 O21 -179.4(8) . . . . ?
W1 O16 Si1 O21 59.5(11) . . . . ?
W5 O16 Si1 O21 -58.4(11) . . . . ?
W2 O4 W1 O1 127(2) . . . . ?
W2 O4 W1 O3 26(2) . . . . ?
W2 O4 W1 O8 -51(3) . . . . ?
W2 O4 W1 O10 -131(2) . . . . ?
W2 O4 W1 O16 -59(2) . . . . ?
W3 O3 W1 O1 -124.7(19) . . . . ?
W3 O3 W1 O4 -21.5(19) . . . . ?
W3 O3 W1 O8 137.4(19) . . . . ?
W3 O3 W1 O10 58(3) . . . . ?
W3 O3 W1 O16 63.9(19) . . . . ?
W5 O8 W1 O1 172.6(10) . . . . ?
W5 O8 W1 O4 -9(2) . . . . ?
W5 O8 W1 O3 -85.9(10) . . . . ?
W5 O8 W1 O10 71.4(10) . . . . ?
W5 O8 W1 O16 -0.8(8) . . . . ?
W4 O10 W1 O1 -170.7(10) . . . . ?
W4 O10 W1 O4 85.6(10) . . . . ?
W4 O10 W1 O3 6(2) . . . . ?
W4 O10 W1 O8 -73.0(10) . . . . ?
W4 O10 W1 O16 0.4(8) . . . . ?
Si1 O16 W1 O1 -170(4) . . . . ?
W4 O16 W1 O1 55(4) . . . . ?
W5 O16 W1 O1 -37(4) . . . . ?
Si1 O16 W1 O4 44.8(10) . . . . ?
W4 O16 W1 O4 -90.7(6) . . . . ?
W5 O16 W1 O4 177.4(6) . . . . ?
Si1 O16 W1 O3 -42.4(10) . . . . ?
W4 O16 W1 O3 -177.9(6) . . . . ?
W5 O16 W1 O3 90.2(6) . . . . ?
Si1 O16 W1 O8 -132.0(11) . . . . ?
W4 O16 W1 O8 92.5(6) . . . . ?
W5 O16 W1 O8 0.6(5) . . . . ?
Si1 O16 W1 O10 135.2(11) . . . . ?
W4 O16 W1 O10 -0.3(6) . . . . ?
W5 O16 W1 O10 -92.2(6) . . . . ?
W8 O7 W2 O35 -173.0(10) . . . . ?
W8 O7 W2 O6 -72.2(9) . . . . ?
W8 O7 W2 O4 12(2) . . . . ?
W8 O7 W2 O5 84.7(9) . . . . ?
W8 O7 W2 O22 1.1(8) . . . . ?
W9 O6 W2 O35 172.0(10) . . . . ?
W9 O6 W2 O7 71.0(10) . . . . ?
W9 O6 W2 O4 -85.8(10) . . . . ?
W9 O6 W2 O5 -17(2) . . . . ?
W9 O6 W2 O22 -2.4(9) . . . . ?
W1 O4 W2 O35 -128(2) . . . . ?
W1 O4 W2 O7 47(3) . . . . ?
W1 O4 W2 O6 131(2) . . . . ?
W1 O4 W2 O5 -27.0(19) . . . . ?
W1 O4 W2 O22 58(2) . . . . ?
W3 O5 W2 O35 132(2) . . . . ?
W3 O5 W2 O7 -126(2) . . . . ?
W3 O5 W2 O6 -39(3) . . . . ?
W3 O5 W2 O4 31(2) . . . . ?
W3 O5 W2 O22 -53(2) . . . . ?
Si1 O22 W2 O35 -179(100) . . . . ?
W8 O22 W2 O35 47(6) . . . . ?
W9 O22 W2 O35 -44(6) . . . . ?
Si1 O22 W2 O7 132.7(12) . . . . ?
W8 O22 W2 O7 -0.8(6) . . . . ?
W9 O22 W2 O7 -92.1(6) . . . . ?
Si1 O22 W2 O6 -133.6(12) . . . . ?
W8 O22 W2 O6 92.9(7) . . . . ?
W9 O22 W2 O6 1.6(6) . . . . ?
Si1 O22 W2 O4 -43.1(11) . . . . ?
W8 O22 W2 O4 -176.6(7) . . . . ?
W9 O22 W2 O4 92.1(6) . . . . ?
Si1 O22 W2 O5 40.8(11) . . . . ?
W8 O22 W2 O5 -92.7(6) . . . . ?
W9 O22 W2 O5 176.0(6) . . . . ?
W2 O5 W3 O2 -130(2) . . . . ?
W2 O5 W3 O9 127(2) . . . . ?
W2 O5 W3 O3 -30(2) . . . . ?
W2 O5 W3 O39 40(3) . . . . ?
W2 O5 W3 O21 53(2) . . . . ?
W7 O9 W3 O2 172.1(9) . . . . ?
W7 O9 W3 O5 -84.8(10) . . . . ?
W7 O9 W3 O3 -3(2) . . . . ?
W7 O9 W3 O39 72.9(10) . . . . ?
W7 O9 W3 O21 0.4(8) . . . . ?
W1 O3 W3 O2 123.5(19) . . . . ?
W1 O3 W3 O5 21.8(19) . . . . ?
W1 O3 W3 O9 -62(3) . . . . ?
W1 O3 W3 O39 -137.2(19) . . . . ?
W1 O3 W3 O21 -64.6(19) . . . . ?
W6 O39 W3 O2 -175.7(9) . . . . ?
W6 O39 W3 O5 14(2) . . . . ?
W6 O39 W3 O9 -73.8(9) . . . . ?
W6 O39 W3 O3 83.8(9) . . . . ?
W6 O39 W3 O21 0.1(8) . . . . ?
Si1 O21 W3 O2 162(4) . . . . ?
W6 O21 W3 O2 28(4) . . . . ?
W7 O21 W3 O2 -64(4) . . . . ?
Si1 O21 W3 O5 -40.5(10) . . . . ?
W6 O21 W3 O5 -174.9(6) . . . . ?
W7 O21 W3 O5 92.9(6) . . . . ?
Si1 O21 W3 O9 -133.6(11) . . . . ?
W6 O21 W3 O9 91.9(7) . . . . ?
W7 O21 W3 O9 -0.3(6) . . . . ?
Si1 O21 W3 O3 45.2(10) . . . . ?
W6 O21 W3 O3 -89.2(6) . . . . ?
W7 O21 W3 O3 178.6(6) . . . . ?
Si1 O21 W3 O39 134.4(11) . . . . ?
W6 O21 W3 O39 0.0(5) . . . . ?
W7 O21 W3 O39 -92.2(6) . . . . ?
W11 O23 W4 O12 129(2) . . . . ?
W11 O23 W4 O13 27(2) . . . . ?
W11 O23 W4 O10 -49(3) . . . . ?
W11 O23 W4 O15 -132(2) . . . . ?
W11 O23 W4 O16 -59(2) . . . . ?
W9 O13 W4 O12 -130.3(19) . . . . ?
W9 O13 W4 O23 -27.2(19) . . . . ?
W9 O13 W4 O10 131(2) . . . . ?
W9 O13 W4 O15 52(3) . . . . ?
W9 O13 W4 O16 57.5(19) . . . . ?
W1 O10 W4 O12 171.8(9) . . . . ?
W1 O10 W4 O23 -10(2) . . . . ?
W1 O10 W4 O13 -85.4(10) . . . . ?
W1 O10 W4 O15 73.3(10) . . . . ?
W1 O10 W4 O16 -0.4(8) . . . . ?
W5 O15 W4 O12 -172.2(10) . . . . ?
W5 O15 W4 O23 83.8(10) . . . . ?
W5 O15 W4 O13 5(2) . . . . ?
W5 O15 W4 O10 -73.9(10) . . . . ?
W5 O15 W4 O16 -0.3(8) . . . . ?
Si1 O16 W4 O12 -179(3) . . . . ?
W1 O16 W4 O12 -45(3) . . . . ?
W5 O16 W4 O12 47(3) . . . . ?
Si1 O16 W4 O23 42.6(10) . . . . ?
W1 O16 W4 O23 176.5(6) . . . . ?
W5 O16 W4 O23 -91.9(6) . . . . ?
Si1 O16 W4 O13 -43.2(10) . . . . ?
W1 O16 W4 O13 90.7(6) . . . . ?
W5 O16 W4 O13 -177.7(6) . . . . ?
Si1 O16 W4 O10 -133.6(11) . . . . ?
W1 O16 W4 O10 0.3(6) . . . . ?
W5 O16 W4 O10 91.9(6) . . . . ?
Si1 O16 W4 O15 134.7(11) . . . . ?
W1 O16 W4 O15 -91.4(7) . . . . ?
W5 O16 W4 O15 0.2(6) . . . . ?
W12 O26 W5 O34 -128(2) . . . . ?
W12 O26 W5 O15 130(2) . . . . ?
W12 O26 W5 O20 -28.4(19) . . . . ?
W12 O26 W5 O8 45(3) . . . . ?
W12 O26 W5 O16 56.9(19) . . . . ?
W4 O15 W5 O34 174.3(10) . . . . ?
W4 O15 W5 O26 -83.1(10) . . . . ?
W4 O15 W5 O20 -5(2) . . . . ?
W4 O15 W5 O8 73.1(10) . . . . ?
W4 O15 W5 O16 0.3(8) . . . . ?
W6 O20 W5 O34 128.5(17) . . . . ?
W6 O20 W5 O26 26.9(16) . . . . ?
W6 O20 W5 O15 -52(3) . . . . ?
W6 O20 W5 O8 -130.3(17) . . . . ?
W6 O20 W5 O16 -57.3(16) . . . . ?
W1 O8 W5 O34 -173.4(10) . . . . ?
W1 O8 W5 O26 13(2) . . . . ?
W1 O8 W5 O15 -71.9(10) . . . . ?
W1 O8 W5 O20 86.1(10) . . . . ?
W1 O8 W5 O16 0.8(8) . . . . ?
Si1 O16 W5 O34 177(4) . . . . ?
W4 O16 W5 O34 -48(5) . . . . ?
W1 O16 W5 O34 45(5) . . . . ?
Si1 O16 W5 O26 -43.5(10) . . . . ?
W4 O16 W5 O26 92.0(6) . . . . ?
W1 O16 W5 O26 -175.4(6) . . . . ?
Si1 O16 W5 O15 -135.7(11) . . . . ?
W4 O16 W5 O15 -0.2(6) . . . . ?
W1 O16 W5 O15 92.4(7) . . . . ?
Si1 O16 W5 O20 42.2(10) . . . . ?
W4 O16 W5 O20 177.7(6) . . . . ?
W1 O16 W5 O20 -89.8(6) . . . . ?
Si1 O16 W5 O8 131.4(11) . . . . ?
W4 O16 W5 O8 -93.1(6) . . . . ?
W1 O16 W5 O8 -0.6(5) . . . . ?
Zn3 O40 W6 O28 -87(2) . . . . ?
Zn3 O40 W6 O20 0(2) . . . . ?
Zn3 O40 W6 O39 91(2) . . . . ?
Zn3 O40 W6 O38 179.6(19) . . . . ?
Zn3 O40 W6 O21 134(4) . . . . ?
W12 O28 W6 O40 127(2) . . . . ?
W12 O28 W6 O20 28(2) . . . . ?
W12 O28 W6 O39 -50(3) . . . . ?
W12 O28 W6 O38 -132(2) . . . . ?
W12 O28 W6 O21 -59(2) . . . . ?
W5 O20 W6 O40 -128.6(16) . . . . ?
W5 O20 W6 O28 -26.5(16) . . . . ?
W5 O20 W6 O39 131.9(16) . . . . ?
W5 O20 W6 O38 52(3) . . . . ?
W5 O20 W6 O21 57.4(16) . . . . ?
W3 O39 W6 O40 174.0(9) . . . . ?
W3 O39 W6 O28 -9(2) . . . . ?
W3 O39 W6 O20 -85.9(9) . . . . ?
W3 O39 W6 O38 73.6(9) . . . . ?
W3 O39 W6 O21 -0.1(8) . . . . ?
W7 O38 W6 O40 -172.9(9) . . . . ?
W7 O38 W6 O28 84.0(10) . . . . ?
W7 O38 W6 O20 6(2) . . . . ?
W7 O38 W6 O39 -74.0(10) . . . . ?
W7 O38 W6 O21 0.8(8) . . . . ?
Si1 O21 W6 O40 -178(4) . . . . ?
W7 O21 W6 O40 46(5) . . . . ?
W3 O21 W6 O40 -44(5) . . . . ?
Si1 O21 W6 O28 43.1(10) . . . . ?
W7 O21 W6 O28 -93.0(6) . . . . ?
W3 O21 W6 O28 176.6(7) . . . . ?
Si1 O21 W6 O20 -42.5(10) . . . . ?
W7 O21 W6 O20 -178.6(6) . . . . ?
W3 O21 W6 O20 90.9(6) . . . . ?
Si1 O21 W6 O39 -133.4(11) . . . . ?
W7 O21 W6 O39 90.5(6) . . . . ?
W3 O21 W6 O39 0.0(5) . . . . ?
Si1 O21 W6 O38 135.5(11) . . . . ?
W7 O21 W6 O38 -0.6(6) . . . . ?
W3 O21 W6 O38 -91.1(6) . . . . ?
W10 O27 W7 O18 -125(2) . . . . ?
W10 O27 W7 O38 135(2) . . . . ?
W10 O27 W7 O17 -23(2) . . . . ?
W10 O27 W7 O9 54(3) . . . . ?
W10 O27 W7 O21 62(2) . . . . ?
W6 O38 W7 O18 173.9(10) . . . . ?
W6 O38 W7 O27 -83.8(10) . . . . ?
W6 O38 W7 O17 -12(2) . . . . ?
W6 O38 W7 O9 72.6(10) . . . . ?
W6 O38 W7 O21 -0.8(8) . . . . ?
W8 O17 W7 O18 130(2) . . . . ?
W8 O17 W7 O27 29(2) . . . . ?
W8 O17 W7 O38 -44(3) . . . . ?
W8 O17 W7 O9 -128(2) . . . . ?
W8 O17 W7 O21 -54(2) . . . . ?
W3 O9 W7 O18 -173.2(10) . . . . ?
W3 O9 W7 O27 8(2) . . . . ?
W3 O9 W7 O38 -72.9(10) . . . . ?
W3 O9 W7 O17 83.9(10) . . . . ?
W3 O9 W7 O21 -0.4(8) . . . . ?
Si1 O21 W7 O18 -172(4) . . . . ?
W6 O21 W7 O18 -37(5) . . . . ?
W3 O21 W7 O18 56(4) . . . . ?
Si1 O21 W7 O27 -44.5(10) . . . . ?
W6 O21 W7 O27 91.1(6) . . . . ?
W3 O21 W7 O27 -176.4(6) . . . . ?
Si1 O21 W7 O38 -135.0(11) . . . . ?
W6 O21 W7 O38 0.6(6) . . . . ?
W3 O21 W7 O38 93.1(6) . . . . ?
Si1 O21 W7 O17 40.5(10) . . . . ?
W6 O21 W7 O17 176.2(6) . . . . ?
W3 O21 W7 O17 -91.3(6) . . . . ?
Si1 O21 W7 O9 132.1(11) . . . . ?
W6 O21 W7 O9 -92.2(7) . . . . ?
W3 O21 W7 O9 0.2(6) . . . . ?
W7 O17 W8 O19 -131(2) . . . . ?
W7 O17 W8 O29 -29(2) . . . . ?
W7 O17 W8 O14 46(3) . . . . ?
W7 O17 W8 O7 128(2) . . . . ?
W7 O17 W8 O22 56(2) . . . . ?
W10 O29 W8 O19 124(2) . . . . ?
W10 O29 W8 O17 22(2) . . . . ?
W10 O29 W8 O14 -137(2) . . . . ?
W10 O29 W8 O7 -56(3) . . . . ?
W10 O29 W8 O22 -64(2) . . . . ?
W9 O14 W8 O19 -171.6(9) . . . . ?
W9 O14 W8 O17 11(2) . . . . ?
W9 O14 W8 O29 84.8(10) . . . . ?
W9 O14 W8 O7 -71.9(9) . . . . ?
W9 O14 W8 O22 1.0(8) . . . . ?
W2 O7 W8 O19 170.8(9) . . . . ?
W2 O7 W8 O17 -86.3(9) . . . . ?
W2 O7 W8 O29 -9(2) . . . . ?
W2 O7 W8 O14 72.0(9) . . . . ?
W2 O7 W8 O22 -1.1(8) . . . . ?
Si1 O22 W8 O19 176(3) . . . . ?
W2 O22 W8 O19 -48(4) . . . . ?
W9 O22 W8 O19 43(4) . . . . ?
Si1 O22 W8 O17 -43.2(10) . . . . ?
W2 O22 W8 O17 92.1(6) . . . . ?
W9 O22 W8 O17 -177.0(6) . . . . ?
Si1 O22 W8 O29 42.1(10) . . . . ?
W2 O22 W8 O29 177.5(7) . . . . ?
W9 O22 W8 O29 -91.6(6) . . . . ?
Si1 O22 W8 O14 133.1(11) . . . . ?
W2 O22 W8 O14 -91.5(6) . . . . ?
W9 O22 W8 O14 -0.7(6) . . . . ?
Si1 O22 W8 O7 -134.6(11) . . . . ?
W2 O22 W8 O7 0.8(5) . . . . ?
W9 O22 W8 O7 91.6(6) . . . . ?
W8 O14 W9 O11 170.5(9) . . . . ?
W8 O14 W9 O13 -12(2) . . . . ?
W8 O14 W9 O6 72.0(10) . . . . ?
W8 O14 W9 O24 -86.2(10) . . . . ?
W8 O14 W9 O22 -1.0(8) . . . . ?
W4 O13 W9 O11 130.6(19) . . . . ?
W4 O13 W9 O14 -47(3) . . . . ?
W4 O13 W9 O6 -131(2) . . . . ?
W4 O13 W9 O24 28(2) . . . . ?
W4 O13 W9 O22 -57.5(19) . . . . ?
W2 O6 W9 O11 -169.7(11) . . . . ?
W2 O6 W9 O14 -70.3(10) . . . . ?
W2 O6 W9 O13 86.4(10) . . . . ?
W2 O6 W9 O24 12(3) . . . . ?
W2 O6 W9 O22 2.4(9) . . . . ?
W11 O24 W9 O11 -133(2) . . . . ?
W11 O24 W9 O14 128(2) . . . . ?
W11 O24 W9 O13 -30(2) . . . . ?
W11 O24 W9 O6 45(3) . . . . ?
W11 O24 W9 O22 55(2) . . . . ?
Si1 O22 W9 O11 179(3) . . . . ?
W8 O22 W9 O11 -48(4) . . . . ?
W2 O22 W9 O11 43(4) . . . . ?
Si1 O22 W9 O14 -132.0(12) . . . . ?
W8 O22 W9 O14 0.7(6) . . . . ?
W2 O22 W9 O14 91.9(6) . . . . ?
Si1 O22 W9 O13 43.7(11) . . . . ?
W8 O22 W9 O13 176.4(6) . . . . ?
W2 O22 W9 O13 -92.4(6) . . . . ?
Si1 O22 W9 O6 134.5(12) . . . . ?
W8 O22 W9 O6 -92.8(7) . . . . ?
W2 O22 W9 O6 -1.6(6) . . . . ?
Si1 O22 W9 O24 -41.8(11) . . . . ?
W8 O22 W9 O24 90.9(6) . . . . ?
W2 O22 W9 O24 -177.9(7) . . . . ?
W8 O29 W10 O36 -125(2) . . . . ?
W8 O29 W10 O27 -21(2) . . . . ?
W8 O29 W10 O33 60(3) . . . . ?
W8 O29 W10 O31 137(2) . . . . ?
W8 O29 W10 O25 64(2) . . . . ?
W7 O27 W10 O36 124(2) . . . . ?
W7 O27 W10 O29 22(2) . . . . ?
W7 O27 W10 O33 -135(2) . . . . ?
W7 O27 W10 O31 -52(3) . . . . ?
W7 O27 W10 O25 -62(2) . . . . ?
W12 O33 W10 O36 -170.8(9) . . . . ?
W12 O33 W10 O29 4(2) . . . . ?
W12 O33 W10 O27 84.2(9) . . . . ?
W12 O33 W10 O31 -72.6(9) . . . . ?
W12 O33 W10 O25 0.1(7) . . . . ?
W11 O31 W10 O36 173.8(9) . . . . ?
W11 O31 W10 O29 -83.7(9) . . . . ?
W11 O31 W10 O27 -10(2) . . . . ?
W11 O31 W10 O33 73.2(9) . . . . ?
W11 O31 W10 O25 -0.3(7) . . . . ?
Si1 O25 W10 O36 -167(4) . . . . ?
W12 O25 W10 O36 58(4) . . . . ?
W11 O25 W10 O36 -33(4) . . . . ?
Si1 O25 W10 O29 -43.8(10) . . . . ?
W12 O25 W10 O29 -178.3(6) . . . . ?
W11 O25 W10 O29 89.8(6) . . . . ?
Si1 O25 W10 O27 42.7(10) . . . . ?
W12 O25 W10 O27 -91.8(6) . . . . ?
W11 O25 W10 O27 176.4(6) . . . . ?
Si1 O25 W10 O33 134.5(11) . . . . ?
W12 O25 W10 O33 -0.1(5) . . . . ?
W11 O25 W10 O33 -91.9(6) . . . . ?
Si1 O25 W10 O31 -133.4(11) . . . . ?
W12 O25 W10 O31 92.0(6) . . . . ?
W11 O25 W10 O31 0.2(5) . . . . ?
W9 O24 W11 O30 131(2) . . . . ?
W9 O24 W11 O23 29(2) . . . . ?
W9 O24 W11 O32 -43(3) . . . . ?
W9 O24 W11 O31 -128(2) . . . . ?
W9 O24 W11 O25 -54(2) . . . . ?
W4 O23 W11 O30 -129(2) . . . . ?
W4 O23 W11 O24 -28(2) . . . . ?
W4 O23 W11 O32 132(2) . . . . ?
W4 O23 W11 O31 52(3) . . . . ?
W4 O23 W11 O25 59(2) . . . . ?
W12 O32 W11 O30 170.9(10) . . . . ?
W12 O32 W11 O24 -15(2) . . . . ?
W12 O32 W11 O23 -86.8(10) . . . . ?
W12 O32 W11 O31 70.3(10) . . . . ?
W12 O32 W11 O25 -2.8(8) . . . . ?
W10 O31 W11 O30 -171.2(9) . . . . ?
W10 O31 W11 O24 86.2(9) . . . . ?
W10 O31 W11 O23 8(2) . . . . ?
W10 O31 W11 O32 -72.0(9) . . . . ?
W10 O31 W11 O25 0.3(7) . . . . ?
Si1 O25 W11 O30 -173(4) . . . . ?
W12 O25 W11 O30 -36(4) . . . . ?
W10 O25 W11 O30 55(4) . . . . ?
Si1 O25 W11 O24 41.2(11) . . . . ?
W12 O25 W11 O24 177.4(7) . . . . ?
W10 O25 W11 O24 -91.6(7) . . . . ?
Si1 O25 W11 O23 -44.3(10) . . . . ?
W12 O25 W11 O23 91.9(6) . . . . ?
W10 O25 W11 O23 -177.1(6) . . . . ?
Si1 O25 W11 O32 -134.3(12) . . . . ?
W12 O25 W11 O32 1.9(6) . . . . ?
W10 O25 W11 O32 92.9(6) . . . . ?
Si1 O25 W11 O31 132.6(11) . . . . ?
W12 O25 W11 O31 -91.2(6) . . . . ?
W10 O25 W11 O31 -0.2(5) . . . . ?
Zn2 O37 W12 O32 -72.0(17) . . . . ?
Zn2 O37 W12 O33 -163.4(16) . . . . ?
Zn2 O37 W12 O28 104.6(17) . . . . ?
Zn2 O37 W12 O26 19.2(18) . . . . ?
Zn2 O37 W12 O25 -115(5) . . . . ?
W11 O32 W12 O37 -171.6(10) . . . . ?
W11 O32 W12 O33 -71.6(10) . . . . ?
W11 O32 W12 O28 17(2) . . . . ?
W11 O32 W12 O26 87.1(10) . . . . ?
W11 O32 W12 O25 2.8(8) . . . . ?
W10 O33 W12 O37 173.9(9) . . . . ?
W10 O33 W12 O32 73.1(9) . . . . ?
W10 O33 W12 O28 -83.2(9) . . . . ?
W10 O33 W12 O26 -13(2) . . . . ?
W10 O33 W12 O25 -0.1(8) . . . . ?
W6 O28 W12 O37 -127(2) . . . . ?
W6 O28 W12 O32 45(3) . . . . ?
W6 O28 W12 O33 133(2) . . . . ?
W6 O28 W12 O26 -27(2) . . . . ?
W6 O28 W12 O25 58(2) . . . . ?
W5 O26 W12 O37 129(2) . . . . ?
W5 O26 W12 O32 -130(2) . . . . ?
W5 O26 W12 O33 -44(3) . . . . ?
W5 O26 W12 O28 27.5(19) . . . . ?
W5 O26 W12 O25 -56.4(19) . . . . ?
Si1 O25 W12 O37 178(5) . . . . ?
W11 O25 W12 O37 43(5) . . . . ?
W10 O25 W12 O37 -49(5) . . . . ?
Si1 O25 W12 O32 133.4(12) . . . . ?
W11 O25 W12 O32 -2.0(6) . . . . ?
W10 O25 W12 O32 -93.9(7) . . . . ?
Si1 O25 W12 O33 -132.6(11) . . . . ?
W11 O25 W12 O33 92.0(6) . . . . ?
W10 O25 W12 O33 0.1(5) . . . . ?
Si1 O25 W12 O28 -41.0(11) . . . . ?
W11 O25 W12 O28 -176.4(7) . . . . ?
W10 O25 W12 O28 91.6(6) . . . . ?
Si1 O25 W12 O26 42.7(11) . . . . ?
W11 O25 W12 O26 -92.7(6) . . . . ?
W10 O25 W12 O26 175.3(6) . . . . ?
W12 O37 Zn2 N8 -73.2(18) . . . . ?
W12 O37 Zn2 O9W 109.8(18) . . . . ?
W12 O37 Zn2 N5 -136(9) . . . . ?
W12 O37 Zn2 O8W -160.2(18) . . . . ?
W12 O37 Zn2 N2 19.0(18) . . . . ?
W6 O40 Zn3 N9 55(2) . . . . ?
W6 O40 Zn3 N9 -125(2) . . . 2_567 ?
W6 O40 Zn3 O40 -59(30) . . . 2_567 ?
W6 O40 Zn3 N16 143(2) . . . . ?
W6 O40 Zn3 N16 -37(2) . . . 2_567 ?
N7 Zn1 N1 C1 -121(2) . . . . ?
N10 Zn1 N1 C1 56(2) . . . . ?
O6W Zn1 N1 C1 -71(7) . . . . ?
N4 Zn1 N1 C1 145(2) . . . . ?
O7W Zn1 N1 C1 -34(2) . . . . ?
N7 Zn1 N1 N2 57(2) . . . . ?
N10 Zn1 N1 N2 -125.7(19) . . . . ?
O6W Zn1 N1 N2 107(6) . . . . ?
N4 Zn1 N1 N2 -37(2) . . . . ?
O7W Zn1 N1 N2 144(2) . . . . ?
C1 N1 N2 C2 1(3) . . . . ?
Zn1 N1 N2 C2 -177.4(18) . . . . ?
C1 N1 N2 Zn2 164.8(17) . . . . ?
Zn1 N1 N2 Zn2 -14(2) . . . . ?
N8 Zn2 N2 C2 118(2) . . . . ?
O9W Zn2 N2 C2 -53(2) . . . . ?
N5 Zn2 N2 C2 -147(2) . . . . ?
O8W Zn2 N2 C2 47(13) . . . . ?
O37 Zn2 N2 C2 35(2) . . . . ?
N8 Zn2 N2 N1 -40.8(17) . . . . ?
O9W Zn2 N2 N1 148.6(16) . . . . ?
N5 Zn2 N2 N1 54.2(17) . . . . ?
O8W Zn2 N2 N1 -112(12) . . . . ?
O37 Zn2 N2 N1 -123.9(16) . . . . ?
N10 Zn1 N7 C3 -17(9) . . . . ?
O6W Zn1 N7 C3 -39(2) . . . . ?
N1 Zn1 N7 C3 135(2) . . . . ?
N4 Zn1 N7 C3 -133(2) . . . . ?
O7W Zn1 N7 C3 47(2) . . . . ?
N10 Zn1 N7 N8 162(7) . . . . ?
O6W Zn1 N7 N8 139.9(19) . . . . ?
N1 Zn1 N7 N8 -45.6(19) . . . . ?
N4 Zn1 N7 N8 46.2(19) . . . . ?
O7W Zn1 N7 N8 -134.1(19) . . . . ?
C3 N7 N8 C4 -7(3) . . . . ?
Zn1 N7 N8 C4 173.7(19) . . . . ?
C3 N7 N8 Zn2 173.5(17) . . . . ?
Zn1 N7 N8 Zn2 -6(3) . . . . ?
O9W Zn2 N8 C4 -18(6) . . . . ?
N5 Zn2 N8 C4 140(3) . . . . ?
O8W Zn2 N8 C4 49(3) . . . . ?
N2 Zn2 N8 C4 -127(3) . . . . ?
O37 Zn2 N8 C4 -36(3) . . . . ?
O9W Zn2 N8 N7 161(4) . . . . ?
N5 Zn2 N8 N7 -40.5(19) . . . . ?
O8W Zn2 N8 N7 -131.3(19) . . . . ?
N2 Zn2 N8 N7 52.3(19) . . . . ?
O37 Zn2 N8 N7 143.4(19) . . . . ?
N9 Zn3 N9 C4 117(100) 2_567 . . . ?
O40 Zn3 N9 C4 37(3) . . . . ?
O40 Zn3 N9 C4 -143(3) 2_567 . . . ?
N16 Zn3 N9 C4 -55(3) . . . . ?
N16 Zn3 N9 C4 125(3) 2_567 . . . ?
N9 Zn3 N9 C3 -58(100) 2_567 . . . ?
O40 Zn3 N9 C3 -138(2) . . . . ?
O40 Zn3 N9 C3 42(2) 2_567 . . . ?
N16 Zn3 N9 C3 130(3) . . . . ?
N16 Zn3 N9 C3 -50(3) 2_567 . . . ?
N7 Zn1 N10 C7 -18(9) . . . . ?
O6W Zn1 N10 C7 5(2) . . . . ?
N1 Zn1 N10 C7 -170(2) . . . . ?
N4 Zn1 N10 C7 98(2) . . . . ?
O7W Zn1 N10 C7 -81(2) . . . . ?
N7 Zn1 N10 N11 167(7) . . . . ?
O6W Zn1 N10 N11 -171(2) . . . . ?
N1 Zn1 N10 N11 15(2) . . . . ?
N4 Zn1 N10 N11 -77(2) . . . . ?
O7W Zn1 N10 N11 103(2) . . . . ?
C7 N10 N11 C8 0(3) . . . . ?
Zn1 N10 N11 C8 175.6(18) . . . . ?
N2 N1 C1 N3 1(3) . . . . ?
Zn1 N1 C1 N3 179.8(16) . . . . ?
C2 N3 C1 N1 -3(3) . . . . ?
C1 N3 C2 N2 4(3) . . . . ?
N1 N2 C2 N3 -3(3) . . . . ?
Zn2 N2 C2 N3 -163.5(17) . . . . ?
N8 N7 C3 N9 6(3) . . . . ?
Zn1 N7 C3 N9 -175.3(18) . . . . ?
C4 N9 C3 N7 -2(3) . . . . ?
Zn3 N9 C3 N7 174.0(18) . . . . ?
N7 N8 C4 N9 6(3) . . . . ?
Zn2 N8 C4 N9 -174.4(18) . . . . ?
C3 N9 C4 N8 -3(3) . . . . ?
Zn3 N9 C4 N8 -178.8(18) . . . . ?
C8 N12 C7 N10 0(3) . . . . ?
N11 N10 C7 N12 0(3) . . . . ?
Zn1 N10 C7 N12 -175.9(17) . . . . ?
N10 N11 C8 N12 0(3) . . . . ?
C7 N12 C8 N11 0(3) . . . . ?
N16 N13 C10 N15 -5(5) . . . . ?
C9 N15 C10 N13 1(5) . . . . ?
C10 N15 C9 N16 4(5) . . . . ?
C10 N13 N16 C9 6(4) . . . . ?
C10 N13 N16 Zn3 173(3) . . . . ?
N15 C9 N16 N13 -6(5) . . . . ?
N15 C9 N16 Zn3 -174(3) . . . . ?
N9 Zn3 N16 N13 143(3) . . . . ?
N9 Zn3 N16 N13 -37(3) 2_567 . . . ?
O40 Zn3 N16 N13 51(3) . . . . ?
O40 Zn3 N16 N13 -129(3) 2_567 . . . ?
N16 Zn3 N16 N13 -39(100) 2_567 . . . ?
N9 Zn3 N16 C9 -53(3) . . . . ?
N9 Zn3 N16 C9 127(3) 2_567 . . . ?
O40 Zn3 N16 C9 -145(3) . . . . ?
O40 Zn3 N16 C9 35(3) 2_567 . . . ?
N16 Zn3 N16 C9 125(100) 2_567 . . . ?
N7 Zn1 N4 C5 130(3) . . . . ?
N10 Zn1 N4 C5 -45(3) . . . . ?
O6W Zn1 N4 C5 42(3) . . . . ?
N1 Zn1 N4 C5 -142(3) . . . . ?
O7W Zn1 N4 C5 -29(60) . . . . ?
N7 Zn1 N4 N5 -38(2) . . . . ?
N10 Zn1 N4 N5 148(2) . . . . ?
O6W Zn1 N4 N5 -125.7(19) . . . . ?
N1 Zn1 N4 N5 50(2) . . . . ?
O7W Zn1 N4 N5 164(58) . . . . ?
N5 N4 C5 N6 0(3) . . . . ?
Zn1 N4 C5 N6 -168.9(19) . . . . ?
N4 C5 N6 C6 -2(3) . . . . ?
C5 N4 N5 C6 3(3) . . . . ?
Zn1 N4 N5 C6 172.9(18) . . . . ?
C5 N4 N5 Zn2 -178.9(19) . . . . ?
Zn1 N4 N5 Zn2 -9(3) . . . . ?
N8 Zn2 N5 C6 -132(2) . . . . ?
O9W Zn2 N5 C6 44(2) . . . . ?
O8W Zn2 N5 C6 -46(2) . . . . ?
N2 Zn2 N5 C6 135(2) . . . . ?
O37 Zn2 N5 C6 -70(10) . . . . ?
N8 Zn2 N5 N4 49(2) . . . . ?
O9W Zn2 N5 N4 -134(2) . . . . ?
O8W Zn2 N5 N4 136(2) . . . . ?
N2 Zn2 N5 N4 -43(2) . . . . ?
O37 Zn2 N5 N4 111(9) . . . . ?
N4 N5 C6 N6 -4(3) . . . . ?
Zn2 N5 C6 N6 177.5(17) . . . . ?
C5 N6 C6 N5 4(3) . . . . ?

_diffrn_measured_fraction_theta_max 0.989
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.989
_refine_diff_density_max         3.366
_refine_diff_density_min         -2.529
_refine_diff_density_rms         0.504
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3
_audit_block_doi                 10.5517/cc13894t
_database_code_depnum_ccdc_archive 'CCDC 1020865'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C16 H50 Cl2 Cu6 Ge N24 O55 W12'
_chemical_formula_sum            'C16 H50 Cl2 Cu6 Ge N24 O55 W12'
_chemical_formula_weight         4189.73

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.5510(5)
_cell_length_b                   12.1300(5)
_cell_length_c                   14.2860(5)
_cell_angle_alpha                94.156(5)
_cell_angle_beta                 105.714(5)
_cell_angle_gamma                106.035(5)
_cell_volume                     1828.27(5)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.5
_cell_measurement_theta_max      25.0

_exptl_crystal_description       Block
_exptl_crystal_colour            'dark green'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    3.805
_exptl_crystal_F_000             1882
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.15
_exptl_absorpt_coefficient_mu    21.085
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.035
_exptl_absorpt_correction_T_max  0.04
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            10121
_diffrn_reflns_av_unetI/netI     0.0973
_diffrn_reflns_av_R_equivalents  0.0504
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_theta_min         1.500
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_full        24.998
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measured_fraction_theta_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_point_group_measured_fraction_full 0.995
_reflns_number_total             6403
_reflns_number_gt                4086
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
The restraint command 'DELU' was refined the atoms n9 and c1.
And the restraint command 'ISOR' was used to refine n1,n5,n8,n9,n10,n12,c2,c5,c6,c7,o2w atoms.
The restraint order 'SIMU' was refined the atoms o3, o5, o7,o14,o20,o22,Ge1,W1,W2,W3,W4 and W5.
The 'OMIT' order was used to confirm the data completeless.
 Due to high levels of disorder about the solvent, we removed the 
 electronic contribution of the unidentified solvent with SQUEEZE. 
 In this P-1 space group with Z = 1 this implies that the 216 removed electrons would 
 all be associated with the disordered water of the formula unit and thus 
 implies that the contributions of 216/10 = 22 additional water molecules 
 should be associated with the Formula unit. When the electron density, TGA, 
 and elemental analysis are taken into account, 15 water molecules are determined.

 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.010 0.500 0.500 283 216 ' '
_platon_squeeze_details          
;
;

_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0904P)²+80.3782P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         6403
_refine_ls_number_parameters     511
_refine_ls_number_restraints     751
_refine_ls_R_factor_all          0.1178
_refine_ls_R_factor_gt           0.0685
_refine_ls_wR_factor_ref         0.2041
_refine_ls_wR_factor_gt          0.1697
_refine_ls_goodness_of_fit_ref   1.034
_refine_ls_restrained_S_all      1.003
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.130(2) 0.701(2) 0.7183(18) 0.073(5) Uani 1 1 d . U . . .
O2 O 0.099(2) 0.812(2) 1.0298(16) 0.055(3) Uani 1 1 d . U . . .
O3 O 0.042(4) 0.627(4) 0.955(3) 0.052(2) Uani 0.5 1 d . U P . .
O4 O -0.104(2) 0.878(2) 0.9254(18) 0.069(6) Uani 1 1 d . U . . .
O5 O 0.297(4) 0.640(4) 1.052(3) 0.053(2) Uani 0.5 1 d . U P . .
O5A O 0.370(4) 0.680(4) 1.098(3) 0.054(3) Uani 0.5 1 d . U P . .
O6 O 0.281(2) 0.566(2) 1.2205(17) 0.060(3) Uani 1 1 d . U . . .
O7 O 0.102(4) 0.421(4) 0.994(3) 0.054(3) Uani 0.5 1 d . U P . .
O8 O 0.236(2) 0.322(2) 0.7952(19) 0.066(5) Uani 1 1 d . U . . .
O9 O -0.062(2) 0.524(2) 0.7379(17) 0.062(3) Uani 1 1 d . U . . .
O10 O -0.233(2) 0.315(2) 0.6354(17) 0.065(6) Uani 1 1 d . U . . .
O11 O 0.3622(19) 0.893(2) 1.0856(15) 0.049(3) Uani 1 1 d . U . . .
O12A O 0.190(4) 0.724(4) 1.156(3) 0.052(3) Uani 0.5 1 d . U P . .
O12B O 0.258(4) 0.772(4) 1.206(3) 0.051(3) Uani 0.5 1 d . U P . .
O13 O -0.011(2) 0.328(2) 0.7794(17) 0.061(3) Uani 1 1 d . U . . .
O14 O 0.027(4) 0.480(4) 0.896(3) 0.053(3) Uani 0.5 1 d . U P . .
O15 O 0.170(2) 0.521(2) 0.8235(17) 0.061(3) Uani 1 1 d . U . . .
O16 O 0.4675(19) 0.520(2) 1.1600(17) 0.056(4) Uani 1 1 d . U . . .
O17 O -0.017(2) 0.721(2) 0.8438(17) 0.062(3) Uani 1 1 d . U . . .
O18 O 0.217(2) 0.732(2) 0.9204(16) 0.056(2) Uani 1 1 d . U . . .
O19 O 0.147(4) 0.589(4) 1.086(3) 0.053(3) Uani 0.5 1 d . U P . .
O20 O 0.108(2) 0.259(2) 0.9325(17) 0.062(3) Uani 1 1 d . U . . .
O21 O 0.293(2) 0.456(2) 0.9732(17) 0.061(2) Uani 1 1 d . U . . .
O22 O 0.232(2) 0.349(2) 1.1162(17) 0.061(3) Uani 1 1 d . U . . .
Ge1 Ge 0.0000 0.5000 1.0000 0.0206(8) Uani 1 2 d S U P . .
W1 W 0.15779(11) 0.37864(12) 0.85868(9) 0.0391(3) Uani 1 1 d . U . . .
W2 W 0.31558(12) 0.50807(14) 1.10637(12) 0.0545(4) Uani 1 1 d . U . . .
W3 W -0.07234(10) 0.76055(10) 0.94955(9) 0.0343(3) Uani 1 1 d . . . . .
W4 W 0.08812(10) 0.63923(10) 0.80952(7) 0.0321(3) Uani 1 1 d . U . . .
W5 W 0.24344(11) 0.76689(10) 1.05960(10) 0.0403(4) Uani 1 1 d . U . . .
W6 W -0.15783(14) 0.37306(12) 0.75043(8) 0.0470(4) Uani 1 1 d . . . . .
Cu1 Cu 0.5000 1.0000 1.0000 0.0198(9) Uani 1 2 d S . P . .
Cu2 Cu 0.5323(3) 1.0151(3) 1.2611(2) 0.0305(8) Uani 1 1 d . . . . .
Cu3 Cu 0.5000 1.0000 1.5000 0.0407(14) Uani 1 2 d S . P . .
N1 N 0.6501(17) 0.9816(17) 1.1047(13) 0.018(4) Uani 1 1 d . U . . .
N2 N 0.6604(18) 0.999(2) 1.2006(14) 0.028(5) Uani 1 1 d . . . . .
N3 N 0.5023(18) 1.145(2) 1.0845(13) 0.028(5) Uani 1 1 d . . . . .
N4 N 0.520(2) 1.144(2) 1.1856(14) 0.033(6) Uani 1 1 d . . . . .
N9 N 0.531(2) 1.319(2) 1.1479(18) 0.044(6) Uani 1 1 d . U . . .
H9 H 0.5366 1.3916 1.1545 0.053 Uiso 1 1 calc R U . . .
N11 N 0.8430(17) 0.9865(19) 1.1838(13) 0.025(5) Uani 1 1 d . . . . .
C1 C 0.544(4) 1.253(3) 1.221(2) 0.060(9) Uani 1 1 d . U . . .
H1 H 0.5662 1.2813 1.2882 0.072 Uiso 1 1 calc R U . . .
C2 C 0.507(2) 1.247(2) 1.0620(19) 0.029(6) Uani 1 1 d . U . . .
H2 H 0.4962 1.2676 0.9995 0.035 Uiso 1 1 calc R U . . .
C3 C 0.775(2) 0.998(3) 1.2461(18) 0.039(8) Uani 1 1 d . . . . .
H3 H 0.8073 1.0044 1.3141 0.047 Uiso 1 1 calc R U . . .
C4 C 0.757(3) 0.978(2) 1.0947(17) 0.030(6) Uani 1 1 d . . . . .
H4 H 0.7733 0.9714 1.0346 0.036 Uiso 1 1 calc R U . . .
Cl1 Cl 0.6703(8) 1.1489(9) 1.4216(5) 0.060(2) Uani 1 1 d . . . . .
N8 N 0.3598(17) 0.9978(19) 1.3817(13) 0.024(4) Uani 1 1 d . U . . .
Cu4 Cu 1.0107(3) 0.9907(4) 1.2244(2) 0.0401(9) Uani 1 1 d . . . . .
N10 N 0.1785(18) 0.9960(18) 1.2802(13) 0.022(4) Uani 1 1 d . U . . .
N7 N 0.3799(18) 1.020(2) 1.2959(15) 0.036(6) Uani 1 1 d . . . . .
C6 C 0.242(2) 0.985(3) 1.3720(19) 0.035(6) Uani 1 1 d . U . . .
H6 H 0.2048 0.9695 1.4219 0.042 Uiso 1 1 calc R U . . .
C7 C 0.268(2) 1.015(3) 1.2350(18) 0.030(6) Uani 1 1 d . U . . .
H7 H 0.2531 1.0246 1.1692 0.036 Uiso 1 1 calc R U . . .
O1W O 0.695(9) 0.655(8) 1.644(6) 0.32(4) Uani 1 1 d . U . . .
O2W O 1.0000 1.0000 1.5000 0.17(3) Uani 1 2 d S U P . .
N5 N 0.5321(18) 0.8745(18) 1.4207(13) 0.022(4) Uani 1 1 d . U . . .
N6 N 0.540(2) 0.874(3) 1.3286(16) 0.044(7) Uani 1 1 d . . . . .
C8 C 0.566(4) 0.785(3) 1.301(2) 0.056(10) Uani 1 1 d . . . . .
H8 H 0.5763 0.7669 1.2399 0.067 Uiso 1 1 calc R U . . .
N12 N 0.576(3) 0.718(3) 1.375(2) 0.075(9) Uani 1 1 d . U . . .
H12 H 0.5930 0.6537 1.3774 0.090 Uiso 1 1 calc R U . . .
C5 C 0.550(3) 0.783(3) 1.445(2) 0.052(8) Uani 1 1 d . U . . .
H5 H 0.5467 0.7604 1.5053 0.063 Uiso 1 1 calc R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 W4 1.67(2) . ?
O2 W5 1.85(2) . ?
O2 W3 1.90(2) . ?
O3 Ge1 1.71(4) . ?
O3 W4 2.28(4) . ?
O3 W3 2.35(5) . ?
O3 W5 2.47(4) . ?
O4 W3 1.61(3) . ?
O5 O5A 0.90(5) . ?
O5 W5 1.81(5) . ?
O5 W2 1.88(5) . ?
O5A W5 2.01(5) . ?
O5A W2 2.03(5) . ?
O6 W6 1.90(3) 2_567 ?
O6 W2 1.91(2) . ?
O7 Ge1 1.73(5) . ?
O7 O14 1.75(6) . ?
O7 W1 2.27(5) . ?
O7 W3 2.37(5) 2_567 ?
O7 W2 2.44(4) . ?
O8 W1 1.67(2) . ?
O9 W4 1.87(2) . ?
O9 W6 1.91(2) . ?
O10 W6 1.63(2) . ?
O11 W5 1.68(2) . ?
O11 Cu1 2.42(2) . ?
O12A O12B 0.92(5) . ?
O12A W5 1.72(4) . ?
O12A O19 1.73(6) . ?
O12A W6 1.88(4) 2_567 ?
O12B W5 2.04(4) . ?
O12B W6 2.06(4) 2_567 ?
O13 W1 1.87(2) . ?
O13 W6 1.88(3) . ?
O14 Ge1 1.61(4) . ?
O14 W1 2.34(5) . ?
O14 W4 2.41(4) . ?
O14 W6 2.50(4) . ?
O15 W1 1.81(3) . ?
O15 W4 1.92(3) . ?
O16 W2 1.68(2) . ?
O17 W3 1.87(2) . ?
O17 W4 1.91(3) . ?
O18 W4 1.88(2) . ?
O18 W5 1.92(2) . ?
O19 Ge1 1.80(4) . ?
O19 W5 2.25(4) . ?
O19 W6 2.31(4) 2_567 ?
O19 W2 2.37(5) . ?
O20 W3 1.85(2) 2_567 ?
O20 W1 1.91(2) . ?
O21 W2 1.88(2) . ?
O21 W1 1.89(2) . ?
O22 W3 1.89(2) 2_567 ?
O22 W2 1.94(2) . ?
Ge1 O14 1.61(4) 2_567 ?
Ge1 O3 1.71(4) 2_567 ?
Ge1 O7 1.73(5) 2_567 ?
Ge1 O19 1.80(4) 2_567 ?
W3 O20 1.85(2) 2_567 ?
W3 O22 1.89(2) 2_567 ?
W3 O7 2.37(5) 2_567 ?
W6 O12A 1.88(4) 2_567 ?
W6 O6 1.90(3) 2_567 ?
W6 O12B 2.06(4) 2_567 ?
W6 O19 2.31(4) 2_567 ?
Cu1 N1 2.037(18) . ?
Cu1 N1 2.037(18) 2_677 ?
Cu1 N3 2.05(2) . ?
Cu1 N3 2.05(2) 2_677 ?
Cu1 O11 2.42(2) 2_677 ?
Cu2 N2 1.951(19) . ?
Cu2 N7 1.97(2) . ?
Cu2 N4 1.98(2) . ?
Cu2 N6 2.03(3) . ?
Cu2 Cl1 2.547(9) . ?
Cu3 N8 1.992(17) . ?
Cu3 N8 1.992(17) 2_678 ?
Cu3 N5 2.01(2) 2_678 ?
Cu3 N5 2.01(2) . ?
N1 C4 1.29(3) . ?
N1 N2 1.34(3) . ?
N2 C3 1.31(3) . ?
N3 C2 1.29(3) . ?
N3 N4 1.41(3) . ?
N4 C1 1.30(4) . ?
N9 C2 1.37(3) . ?
N9 C1 1.37(4) . ?
N9 H9 0.8600 . ?
N11 C3 1.35(3) . ?
N11 C4 1.36(3) . ?
N11 Cu4 1.850(19) . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 H4 0.9300 . ?
N8 C6 1.30(3) . ?
N8 N7 1.34(3) . ?
Cu4 N10 1.867(19) 1_655 ?
N10 C7 1.33(3) . ?
N10 C6 1.35(3) . ?
N10 Cu4 1.867(18) 1_455 ?
N7 C7 1.34(3) . ?
C6 H6 0.9300 . ?
C7 H7 0.9300 . ?
N5 C5 1.24(4) . ?
N5 N6 1.34(3) . ?
N6 C8 1.27(4) . ?
C8 N12 1.38(4) . ?
C8 H8 0.9300 . ?
N12 C5 1.37(5) . ?
N12 H12 0.8600 . ?
C5 H5 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W5 O2 W3 141.1(13) . . ?
Ge1 O3 W4 124(2) . . ?
Ge1 O3 W3 122(2) . . ?
W4 O3 W3 100.7(17) . . ?
Ge1 O3 W5 113(2) . . ?
W4 O3 W5 96.4(15) . . ?
W3 O3 W5 94.4(16) . . ?
O5A O5 W5 89(5) . . ?
O5A O5 W2 87(5) . . ?
W5 O5 W2 146(3) . . ?
O5 O5A W5 64(4) . . ?
O5 O5A W2 67(4) . . ?
W5 O5A W2 122(2) . . ?
W6 O6 W2 137.8(13) 2_567 . ?
Ge1 O7 O14 55(2) . . ?
Ge1 O7 W1 125(2) . . ?
O14 O7 W1 70(2) . . ?
Ge1 O7 W3 120(2) . 2_567 ?
O14 O7 W3 138(3) . 2_567 ?
W1 O7 W3 99.6(19) . 2_567 ?
Ge1 O7 W2 114(2) . . ?
O14 O7 W2 127(3) . . ?
W1 O7 W2 97.1(16) . . ?
W3 O7 W2 94.7(16) 2_567 . ?
W4 O9 W6 138.0(14) . . ?
W5 O11 Cu1 136.3(11) . . ?
O12B O12A W5 97(4) . . ?
O12B O12A O19 138(6) . . ?
W5 O12A O19 81(2) . . ?
O12B O12A W6 88(4) . 2_567 ?
W5 O12A W6 156(3) . 2_567 ?
O19 O12A W6 79(2) . 2_567 ?
O12A O12B W5 57(4) . . ?
O12A O12B W6 66(4) . 2_567 ?
W5 O12B W6 118(2) . 2_567 ?
W1 O13 W6 141.0(14) . . ?
Ge1 O14 O7 62(2) . . ?
Ge1 O14 W1 127(3) . . ?
O7 O14 W1 66(2) . . ?
Ge1 O14 W4 122(2) . . ?
O7 O14 W4 136(3) . . ?
W1 O14 W4 96.5(15) . . ?
Ge1 O14 W6 117(2) . . ?
O7 O14 W6 127(3) . . ?
W1 O14 W6 93.9(16) . . ?
W4 O14 W6 91.9(15) . . ?
W1 O15 W4 143.6(13) . . ?
W3 O17 W4 141.1(15) . . ?
W4 O18 W5 137.6(12) . . ?
O12A O19 Ge1 132(3) . . ?
O12A O19 W5 49.1(18) . . ?
Ge1 O19 W5 120(2) . . ?
O12A O19 W6 53.2(19) . 2_567 ?
Ge1 O19 W6 119(2) . 2_567 ?
W5 O19 W6 101.1(17) . 2_567 ?
O12A O19 W2 114(3) . . ?
Ge1 O19 W2 115(2) . . ?
W5 O19 W2 99.6(15) . . ?
W6 O19 W2 98.9(17) 2_567 . ?
W3 O20 W1 140.7(15) 2_567 . ?
W2 O21 W1 138.1(13) . . ?
W3 O22 W2 134.6(13) 2_567 . ?
O14 Ge1 O14 180.00(2) . 2_567 ?
O14 Ge1 O3 112(2) . 2_567 ?
O14 Ge1 O3 68(2) 2_567 2_567 ?
O14 Ge1 O3 68(2) . . ?
O14 Ge1 O3 112(2) 2_567 . ?
O3 Ge1 O3 179.999(13) 2_567 . ?
O14 Ge1 O7 63(2) . . ?
O14 Ge1 O7 117(2) 2_567 . ?
O3 Ge1 O7 69(2) 2_567 . ?
O3 Ge1 O7 111(2) . . ?
O14 Ge1 O7 117(2) . 2_567 ?
O14 Ge1 O7 63(2) 2_567 2_567 ?
O3 Ge1 O7 111(2) 2_567 2_567 ?
O3 Ge1 O7 69(2) . 2_567 ?
O7 Ge1 O7 180(3) . 2_567 ?
O14 Ge1 O19 74(2) . 2_567 ?
O14 Ge1 O19 106(2) 2_567 2_567 ?
O3 Ge1 O19 74(2) 2_567 2_567 ?
O3 Ge1 O19 106(2) . 2_567 ?
O7 Ge1 O19 103(2) . 2_567 ?
O7 Ge1 O19 77(2) 2_567 2_567 ?
O14 Ge1 O19 106(2) . . ?
O14 Ge1 O19 74(2) 2_567 . ?
O3 Ge1 O19 106(2) 2_567 . ?
O3 Ge1 O19 74(2) . . ?
O7 Ge1 O19 77(2) . . ?
O7 Ge1 O19 103(2) 2_567 . ?
O19 Ge1 O19 180.0 2_567 . ?
O8 W1 O15 104.5(12) . . ?
O8 W1 O13 105.1(12) . . ?
O15 W1 O13 88.6(10) . . ?
O8 W1 O21 99.7(12) . . ?
O15 W1 O21 86.5(10) . . ?
O13 W1 O21 155.2(11) . . ?
O8 W1 O20 102.3(12) . . ?
O15 W1 O20 153.1(11) . . ?
O13 W1 O20 85.9(10) . . ?
O21 W1 O20 87.6(10) . . ?
O8 W1 O7 155.1(15) . . ?
O15 W1 O7 93.7(14) . . ?
O13 W1 O7 92.0(13) . . ?
O21 W1 O7 64.1(13) . . ?
O20 W1 O7 60.3(14) . . ?
O8 W1 O14 160.2(15) . . ?
O15 W1 O14 60.7(13) . . ?
O13 W1 O14 63.9(13) . . ?
O21 W1 O14 92.7(13) . . ?
O20 W1 O14 93.5(14) . . ?
O7 W1 O14 44.6(16) . . ?
O16 W2 O5 112.2(16) . . ?
O16 W2 O21 102.4(11) . . ?
O5 W2 O21 79.9(16) . . ?
O16 W2 O6 97.6(11) . . ?
O5 W2 O6 89.6(16) . . ?
O21 W2 O6 159.7(10) . . ?
O16 W2 O22 101.4(11) . . ?
O5 W2 O22 145.9(16) . . ?
O21 W2 O22 87.6(10) . . ?
O6 W2 O22 91.7(10) . . ?
O16 W2 O5A 88.8(16) . . ?
O5 W2 O5A 26.1(15) . . ?
O21 W2 O5A 96.0(15) . . ?
O6 W2 O5A 81.0(15) . . ?
O22 W2 O5A 168.3(15) . . ?
O16 W2 O19 149.2(13) . . ?
O5 W2 O19 51.0(17) . . ?
O21 W2 O19 99.4(13) . . ?
O6 W2 O19 60.9(13) . . ?
O22 W2 O19 101.1(13) . . ?
O5A W2 O19 67.4(17) . . ?
O16 W2 O7 156.7(14) . . ?
O5 W2 O7 82.0(18) . . ?
O21 W2 O7 60.5(13) . . ?
O6 W2 O7 101.1(13) . . ?
O22 W2 O7 64.3(13) . . ?
O5A W2 O7 107.8(18) . . ?
O19 W2 O7 54.1(16) . . ?
O4 W3 O20 103.4(13) . 2_567 ?
O4 W3 O17 102.1(12) . . ?
O20 W3 O17 154.4(12) 2_567 . ?
O4 W3 O22 99.5(12) . 2_567 ?
O20 W3 O22 88.4(10) 2_567 2_567 ?
O17 W3 O22 88.4(10) . 2_567 ?
O4 W3 O2 104.1(11) . . ?
O20 W3 O2 84.4(10) 2_567 . ?
O17 W3 O2 88.4(10) . . ?
O22 W3 O2 156.3(11) 2_567 . ?
O4 W3 O3 155.0(14) . . ?
O20 W3 O3 96.8(14) 2_567 . ?
O17 W3 O3 58.3(13) . . ?
O22 W3 O3 95.5(13) 2_567 . ?
O2 W3 O3 63.1(12) . . ?
O4 W3 O7 155.9(15) . 2_567 ?
O20 W3 O7 58.7(14) 2_567 2_567 ?
O17 W3 O7 97.0(14) . 2_567 ?
O22 W3 O7 66.4(13) 2_567 2_567 ?
O2 W3 O7 90.8(13) . 2_567 ?
O3 W3 O7 49.0(15) . 2_567 ?
O1 W4 O9 100.4(11) . . ?
O1 W4 O18 101.4(11) . . ?
O9 W4 O18 158.1(10) . . ?
O1 W4 O17 104.5(13) . . ?
O9 W4 O17 86.2(11) . . ?
O18 W4 O17 86.4(10) . . ?
O1 W4 O15 102.9(13) . . ?
O9 W4 O15 88.1(10) . . ?
O18 W4 O15 89.0(10) . . ?
O17 W4 O15 152.6(10) . . ?
O1 W4 O3 158.2(16) . . ?
O9 W4 O3 93.2(13) . . ?
O18 W4 O3 65.3(12) . . ?
O17 W4 O3 59.2(14) . . ?
O15 W4 O3 94.4(14) . . ?
O1 W4 O14 155.3(15) . . ?
O9 W4 O14 66.1(13) . . ?
O18 W4 O14 94.2(12) . . ?
O17 W4 O14 95.4(14) . . ?
O15 W4 O14 58.0(13) . . ?
O3 W4 O14 46.5(16) . . ?
O11 W5 O12A 115.9(17) . . ?
O11 W5 O5 112.8(16) . . ?
O12A W5 O5 90(2) . . ?
O11 W5 O2 103.9(11) . . ?
O12A W5 O2 81.1(17) . . ?
O5 W5 O2 142.3(16) . . ?
O11 W5 O18 99.1(10) . . ?
O12A W5 O18 144.9(17) . . ?
O5 W5 O18 78.0(16) . . ?
O2 W5 O18 88.2(10) . . ?
O11 W5 O5A 90.0(15) . . ?
O12A W5 O5A 88(2) . . ?
O5 W5 O5A 26.5(16) . . ?
O2 W5 O5A 165.2(15) . . ?
O18 W5 O5A 94.7(15) . . ?
O11 W5 O12B 90.3(14) . . ?
O12A W5 O12B 26.5(16) . . ?
O5 W5 O12B 94(2) . . ?
O2 W5 O12B 93.6(15) . . ?
O18 W5 O12B 169.7(15) . . ?
O5A W5 O12B 81.0(19) . . ?
O11 W5 O19 154.0(13) . . ?
O12A W5 O19 49.4(19) . . ?
O5 W5 O19 53.8(18) . . ?
O2 W5 O19 95.1(14) . . ?
O18 W5 O19 99.0(13) . . ?
O5A W5 O19 70.1(17) . . ?
O12B W5 O19 70.7(17) . . ?
O11 W5 O3 153.1(13) . . ?
O12A W5 O3 85.1(19) . . ?
O5 W5 O3 81.9(19) . . ?
O2 W5 O3 60.9(13) . . ?
O18 W5 O3 60.7(12) . . ?
O5A W5 O3 108.0(18) . . ?
O12B W5 O3 111.6(16) . . ?
O19 W5 O3 52.7(16) . . ?
O10 W6 O13 104.1(12) . . ?
O10 W6 O12A 115.4(17) . 2_567 ?
O13 W6 O12A 80.5(16) . 2_567 ?
O10 W6 O6 99.3(12) . 2_567 ?
O13 W6 O6 155.9(10) . 2_567 ?
O12A W6 O6 84.5(16) 2_567 2_567 ?
O10 W6 O9 101.8(11) . . ?
O13 W6 O9 89.8(11) . . ?
O12A W6 O9 142.8(16) 2_567 . ?
O6 W6 O9 90.9(11) 2_567 . ?
O10 W6 O12B 89.7(16) . 2_567 ?
O13 W6 O12B 92.3(15) . 2_567 ?
O12A W6 O12B 26.4(15) 2_567 2_567 ?
O6 W6 O12B 82.1(15) 2_567 2_567 ?
O9 W6 O12B 167.4(15) . 2_567 ?
O10 W6 O19 152.9(14) . 2_567 ?
O13 W6 O19 93.9(14) . 2_567 ?
O12A W6 O19 47.4(18) 2_567 2_567 ?
O6 W6 O19 62.2(13) 2_567 2_567 ?
O9 W6 O19 98.3(13) . 2_567 ?
O12B W6 O19 69.2(17) 2_567 2_567 ?
O10 W6 O14 156.9(14) . . ?
O13 W6 O14 60.2(13) . . ?
O12A W6 O14 80.5(17) 2_567 . ?
O6 W6 O14 98.9(13) 2_567 . ?
O9 W6 O14 63.7(12) . . ?
O12B W6 O14 106.9(16) 2_567 . ?
O19 W6 O14 50.2(14) 2_567 . ?
N1 Cu1 N1 180.0 . 2_677 ?
N1 Cu1 N3 91.8(8) . . ?
N1 Cu1 N3 88.2(8) 2_677 . ?
N1 Cu1 N3 88.2(8) . 2_677 ?
N1 Cu1 N3 91.8(8) 2_677 2_677 ?
N3 Cu1 N3 180.0 . 2_677 ?
N1 Cu1 O11 91.3(7) . 2_677 ?
N1 Cu1 O11 88.7(7) 2_677 2_677 ?
N3 Cu1 O11 94.6(8) . 2_677 ?
N3 Cu1 O11 85.4(8) 2_677 2_677 ?
N1 Cu1 O11 88.7(7) . . ?
N1 Cu1 O11 91.3(7) 2_677 . ?
N3 Cu1 O11 85.4(8) . . ?
N3 Cu1 O11 94.6(8) 2_677 . ?
O11 Cu1 O11 180.0(8) 2_677 . ?
N2 Cu2 N7 168.8(8) . . ?
N2 Cu2 N4 86.5(10) . . ?
N7 Cu2 N4 89.4(10) . . ?
N2 Cu2 N6 91.8(9) . . ?
N7 Cu2 N6 91.5(10) . . ?
N4 Cu2 N6 175.6(9) . . ?
N2 Cu2 Cl1 100.8(6) . . ?
N7 Cu2 Cl1 89.9(7) . . ?
N4 Cu2 Cl1 94.2(7) . . ?
N6 Cu2 Cl1 90.1(7) . . ?
N8 Cu3 N8 180.0(11) . 2_678 ?
N8 Cu3 N5 92.3(8) . 2_678 ?
N8 Cu3 N5 87.7(8) 2_678 2_678 ?
N8 Cu3 N5 87.7(8) . . ?
N8 Cu3 N5 92.3(8) 2_678 . ?
N5 Cu3 N5 180.000(11) 2_678 . ?
C4 N1 N2 109.3(19) . . ?
C4 N1 Cu1 127.5(16) . . ?
N2 N1 Cu1 121.6(15) . . ?
C3 N2 N1 104.8(19) . . ?
C3 N2 Cu2 127.0(17) . . ?
N1 N2 Cu2 128.2(15) . . ?
C2 N3 N4 112(2) . . ?
C2 N3 Cu1 129.2(17) . . ?
N4 N3 Cu1 118.5(18) . . ?
C1 N4 N3 104(2) . . ?
C1 N4 Cu2 127(2) . . ?
N3 N4 Cu2 128.8(18) . . ?
C2 N9 C1 106(3) . . ?
C2 N9 H9 126.8 . . ?
C1 N9 H9 126.8 . . ?
C3 N11 C4 101.4(19) . . ?
C3 N11 Cu4 124.0(16) . . ?
C4 N11 Cu4 134.5(16) . . ?
N4 C1 N9 111(3) . . ?
N4 C1 H1 124.4 . . ?
N9 C1 H1 124.4 . . ?
N3 C2 N9 107(2) . . ?
N3 C2 H2 126.6 . . ?
N9 C2 H2 126.6 . . ?
N2 C3 N11 113(2) . . ?
N2 C3 H3 123.4 . . ?
N11 C3 H3 123.4 . . ?
N1 C4 N11 111(2) . . ?
N1 C4 H4 124.4 . . ?
N11 C4 H4 124.4 . . ?
C6 N8 N7 107.8(19) . . ?
C6 N8 Cu3 130.1(17) . . ?
N7 N8 Cu3 121.9(14) . . ?
N11 Cu4 N10 173.3(8) . 1_655 ?
C7 N10 C6 103(2) . . ?
C7 N10 Cu4 125.8(16) . 1_455 ?
C6 N10 Cu4 131.3(18) . 1_455 ?
C7 N7 N8 105.7(19) . . ?
C7 N7 Cu2 127.7(17) . . ?
N8 N7 Cu2 124.4(16) . . ?
N8 C6 N10 112(2) . . ?
N8 C6 H6 124.1 . . ?
N10 C6 H6 124.1 . . ?
N10 C7 N7 112(2) . . ?
N10 C7 H7 124.1 . . ?
N7 C7 H7 124.1 . . ?
C5 N5 N6 106(3) . . ?
C5 N5 Cu3 129(2) . . ?
N6 N5 Cu3 125.9(19) . . ?
C8 N6 N5 110(3) . . ?
C8 N6 Cu2 129.0(19) . . ?
N5 N6 Cu2 120(2) . . ?
N6 C8 N12 109(3) . . ?
N6 C8 H8 125.4 . . ?
N12 C8 H8 125.4 . . ?
C5 N12 C8 101(3) . . ?
C5 N12 H12 129.6 . . ?
C8 N12 H12 129.6 . . ?
N5 C5 N12 114(3) . . ?
N5 C5 H5 122.9 . . ?
N12 C5 H5 122.9 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
W2 O5 O5A W5 -146(2) . . . . ?
W5 O5 O5A W2 146(2) . . . . ?
O19 O12A O12B W5 85(7) . . . . ?
W6 O12A O12B W5 156(3) 2_567 . . . ?
W5 O12A O12B W6 -156(3) . . . 2_567 ?
O19 O12A O12B W6 -71(7) . . . 2_567 ?
W1 O7 O14 Ge1 179.8(19) . . . . ?
W3 O7 O14 Ge1 98(4) 2_567 . . . ?
W2 O7 O14 Ge1 -96(3) . . . . ?
Ge1 O7 O14 W1 -180(2) . . . . ?
W3 O7 O14 W1 -82(4) 2_567 . . . ?
W2 O7 O14 W1 84(3) . . . . ?
Ge1 O7 O14 W4 107(4) . . . . ?
W1 O7 O14 W4 -73(4) . . . . ?
W3 O7 O14 W4 -155(3) 2_567 . . . ?
W2 O7 O14 W4 11(6) . . . . ?
Ge1 O7 O14 W6 -104(3) . . . . ?
W1 O7 O14 W6 75(3) . . . . ?
W3 O7 O14 W6 -6(6) 2_567 . . . ?
W2 O7 O14 W6 159(2) . . . . ?
O12B O12A O19 Ge1 172(7) . . . . ?
W5 O12A O19 Ge1 -97(4) . . . . ?
W6 O12A O19 Ge1 98(4) 2_567 . . . ?
O12B O12A O19 W5 -91(8) . . . . ?
W6 O12A O19 W5 -165(2) 2_567 . . . ?
O12B O12A O19 W6 75(8) . . . 2_567 ?
W5 O12A O19 W6 165(2) . . . 2_567 ?
O12B O12A O19 W2 -9(9) . . . . ?
W5 O12A O19 W2 82(2) . . . . ?
W6 O12A O19 W2 -83(2) 2_567 . . . ?
O7 O14 Ge1 O3 -51(3) . . . 2_567 ?
W1 O14 Ge1 O3 -50(3) . . . 2_567 ?
W4 O14 Ge1 O3 -180(2) . . . 2_567 ?
W6 O14 Ge1 O3 69(3) . . . 2_567 ?
O7 O14 Ge1 O3 129(3) . . . . ?
W1 O14 Ge1 O3 130(3) . . . . ?
W4 O14 Ge1 O3 0(2) . . . . ?
W6 O14 Ge1 O3 -111(3) . . . . ?
W1 O14 Ge1 O7 0(2) . . . . ?
W4 O14 Ge1 O7 -129(3) . . . . ?
W6 O14 Ge1 O7 119(3) . . . . ?
O7 O14 Ge1 O7 180.00(5) . . . 2_567 ?
W1 O14 Ge1 O7 -180(2) . . . 2_567 ?
W4 O14 Ge1 O7 51(3) . . . 2_567 ?
W6 O14 Ge1 O7 -61(3) . . . 2_567 ?
O7 O14 Ge1 O19 -115(3) . . . 2_567 ?
W1 O14 Ge1 O19 -115(3) . . . 2_567 ?
W4 O14 Ge1 O19 116(3) . . . 2_567 ?
W6 O14 Ge1 O19 5(2) . . . 2_567 ?
O7 O14 Ge1 O19 65(3) . . . . ?
W1 O14 Ge1 O19 65(3) . . . . ?
W4 O14 Ge1 O19 -64(3) . . . . ?
W6 O14 Ge1 O19 -175(2) . . . . ?
W4 O3 Ge1 O14 0(2) . . . . ?
W3 O3 Ge1 O14 133(3) . . . . ?
W5 O3 Ge1 O14 -116(3) . . . . ?
W4 O3 Ge1 O14 180(2) . . . 2_567 ?
W3 O3 Ge1 O14 -47(3) . . . 2_567 ?
W5 O3 Ge1 O14 64(3) . . . 2_567 ?
W4 O3 Ge1 O7 47(3) . . . . ?
W3 O3 Ge1 O7 -180(2) . . . . ?
W5 O3 Ge1 O7 -68(3) . . . . ?
W4 O3 Ge1 O7 -133(3) . . . 2_567 ?
W3 O3 Ge1 O7 0(2) . . . 2_567 ?
W5 O3 Ge1 O7 112(3) . . . 2_567 ?
W4 O3 Ge1 O19 -64(3) . . . 2_567 ?
W3 O3 Ge1 O19 69(3) . . . 2_567 ?
W5 O3 Ge1 O19 -180(2) . . . 2_567 ?
W4 O3 Ge1 O19 116(3) . . . . ?
W3 O3 Ge1 O19 -111(3) . . . . ?
W5 O3 Ge1 O19 0(2) . . . . ?
W1 O7 Ge1 O14 0(2) . . . . ?
W3 O7 Ge1 O14 -130(3) 2_567 . . . ?
W2 O7 Ge1 O14 119(3) . . . . ?
O14 O7 Ge1 O14 180.00(5) . . . 2_567 ?
W1 O7 Ge1 O14 180(2) . . . 2_567 ?
W3 O7 Ge1 O14 50(3) 2_567 . . 2_567 ?
W2 O7 Ge1 O14 -61(3) . . . 2_567 ?
O14 O7 Ge1 O3 130(3) . . . 2_567 ?
W1 O7 Ge1 O3 130(3) . . . 2_567 ?
W3 O7 Ge1 O3 0(2) 2_567 . . 2_567 ?
W2 O7 Ge1 O3 -111(3) . . . 2_567 ?
O14 O7 Ge1 O3 -50(3) . . . . ?
W1 O7 Ge1 O3 -50(3) . . . . ?
W3 O7 Ge1 O3 -180(2) 2_567 . . . ?
W2 O7 Ge1 O3 69(3) . . . . ?
O14 O7 Ge1 O19 63(2) . . . 2_567 ?
W1 O7 Ge1 O19 63(3) . . . 2_567 ?
W3 O7 Ge1 O19 -66(3) 2_567 . . 2_567 ?
W2 O7 Ge1 O19 -178(2) . . . 2_567 ?
O14 O7 Ge1 O19 -117(2) . . . . ?
W1 O7 Ge1 O19 -117(3) . . . . ?
W3 O7 Ge1 O19 114(3) 2_567 . . . ?
W2 O7 Ge1 O19 2(2) . . . . ?
O12A O19 Ge1 O14 120(4) . . . . ?
W5 O19 Ge1 O14 60(3) . . . . ?
W6 O19 Ge1 O14 -175(2) 2_567 . . . ?
W2 O19 Ge1 O14 -59(3) . . . . ?
O12A O19 Ge1 O14 -60(4) . . . 2_567 ?
W5 O19 Ge1 O14 -120(3) . . . 2_567 ?
W6 O19 Ge1 O14 5(3) 2_567 . . 2_567 ?
W2 O19 Ge1 O14 121(3) . . . 2_567 ?
O12A O19 Ge1 O3 -120(4) . . . 2_567 ?
W5 O19 Ge1 O3 180(2) . . . 2_567 ?
W6 O19 Ge1 O3 -55(3) 2_567 . . 2_567 ?
W2 O19 Ge1 O3 61(3) . . . 2_567 ?
O12A O19 Ge1 O3 60(4) . . . . ?
W5 O19 Ge1 O3 0(2) . . . . ?
W6 O19 Ge1 O3 125(3) 2_567 . . . ?
W2 O19 Ge1 O3 -119(3) . . . . ?
O12A O19 Ge1 O7 177(4) . . . . ?
W5 O19 Ge1 O7 116(3) . . . . ?
W6 O19 Ge1 O7 -119(3) 2_567 . . . ?
W2 O19 Ge1 O7 -2(2) . . . . ?
O12A O19 Ge1 O7 -3(4) . . . 2_567 ?
W5 O19 Ge1 O7 -64(3) . . . 2_567 ?
W6 O19 Ge1 O7 61(3) 2_567 . . 2_567 ?
W2 O19 Ge1 O7 178(2) . . . 2_567 ?
W4 O15 W1 O8 153(2) . . . . ?
W4 O15 W1 O13 48(2) . . . . ?
W4 O15 W1 O21 -108(2) . . . . ?
W4 O15 W1 O20 -30(4) . . . . ?
W4 O15 W1 O7 -44(2) . . . . ?
W4 O15 W1 O14 -13(2) . . . . ?
W6 O13 W1 O8 -150(2) . . . . ?
W6 O13 W1 O15 -45(2) . . . . ?
W6 O13 W1 O21 33(4) . . . . ?
W6 O13 W1 O20 108(2) . . . . ?
W6 O13 W1 O7 48(2) . . . . ?
W6 O13 W1 O14 12(2) . . . . ?
W2 O21 W1 O8 -156(2) . . . . ?
W2 O21 W1 O15 100(2) . . . . ?
W2 O21 W1 O13 21(4) . . . . ?
W2 O21 W1 O20 -54(2) . . . . ?
W2 O21 W1 O7 4(2) . . . . ?
W2 O21 W1 O14 39(2) . . . . ?
O5A O5 W2 O16 -28(5) . . . . ?
W5 O5 W2 O16 -111(5) . . . . ?
O5A O5 W2 O21 -127(4) . . . . ?
W5 O5 W2 O21 150(5) . . . . ?
O5A O5 W2 O6 70(4) . . . . ?
W5 O5 W2 O6 -13(5) . . . . ?
O5A O5 W2 O22 163(3) . . . . ?
W5 O5 W2 O22 79(6) . . . . ?
W5 O5 W2 O5A -83(6) . . . . ?
O5A O5 W2 O19 122(5) . . . . ?
W5 O5 W2 O19 39(4) . . . . ?
O5A O5 W2 O7 171(5) . . . . ?
W5 O5 W2 O7 88(5) . . . . ?
W1 O21 W2 O16 159(2) . . . . ?
W1 O21 W2 O5 -90(2) . . . . ?
W1 O21 W2 O6 -30(4) . . . . ?
W1 O21 W2 O22 58(2) . . . . ?
W1 O21 W2 O5A -111(2) . . . . ?
W1 O21 W2 O19 -43(2) . . . . ?
W1 O21 W2 O7 -4(2) . . . . ?
W4 O17 W3 O4 154(2) . . . . ?
W4 O17 W3 O20 -24(4) . . . 2_567 ?
W4 O17 W3 O22 -107(2) . . . 2_567 ?
W4 O17 W3 O2 50(2) . . . . ?
W4 O17 W3 O3 -9.4(19) . . . . ?
W4 O17 W3 O7 -41(2) . . . 2_567 ?
W6 O9 W4 O1 151(2) . . . . ?
W6 O9 W4 O18 -34(4) . . . . ?
W6 O9 W4 O17 -105(2) . . . . ?
W6 O9 W4 O15 49(2) . . . . ?
W6 O9 W4 O3 -46(2) . . . . ?
W6 O9 W4 O14 -7(2) . . . . ?
W5 O18 W4 O1 161(2) . . . . ?
W5 O18 W4 O9 -14(4) . . . . ?
W5 O18 W4 O17 57(2) . . . . ?
W5 O18 W4 O15 -96(2) . . . . ?
W5 O18 W4 O3 -1(2) . . . . ?
W5 O18 W4 O14 -39(2) . . . . ?
Cu1 O11 W5 O12A 173(2) . . . . ?
Cu1 O11 W5 O5 70(2) . . . . ?
Cu1 O11 W5 O2 -100.8(17) . . . . ?
Cu1 O11 W5 O18 -10.4(19) . . . . ?
Cu1 O11 W5 O5A 84(2) . . . . ?
Cu1 O11 W5 O12B 165(2) . . . . ?
Cu1 O11 W5 O19 123(3) . . . . ?
Cu1 O11 W5 O3 -49(4) . . . . ?
O12B O12A W5 O11 -16(5) . . . . ?
O19 O12A W5 O11 -154.2(19) . . . . ?
W6 O12A W5 O11 -116(7) 2_567 . . . ?
O12B O12A W5 O5 100(5) . . . . ?
O19 O12A W5 O5 -39(3) . . . . ?
W6 O12A W5 O5 -1(7) 2_567 . . . ?
O12B O12A W5 O2 -117(5) . . . . ?
O19 O12A W5 O2 105(2) . . . . ?
W6 O12A W5 O2 143(7) 2_567 . . . ?
O12B O12A W5 O18 169(4) . . . . ?
O19 O12A W5 O18 31(4) . . . . ?
W6 O12A W5 O18 69(8) 2_567 . . . ?
O12B O12A W5 O5A 73(5) . . . . ?
O19 O12A W5 O5A -65(2) . . . . ?
W6 O12A W5 O5A -27(7) 2_567 . . . ?
O19 O12A W5 O12B -138(6) . . . . ?
W6 O12A W5 O12B -100(9) 2_567 . . . ?
O12B O12A W5 O19 138(6) . . . . ?
W6 O12A W5 O19 38(6) 2_567 . . . ?
O12B O12A W5 O3 -179(5) . . . . ?
O19 O12A W5 O3 43(2) . . . . ?
W6 O12A W5 O3 81(7) 2_567 . . . ?
O5A O5 W5 O11 33(5) . . . . ?
W2 O5 W5 O11 115(5) . . . . ?
O5A O5 W5 O12A -86(4) . . . . ?
W2 O5 W5 O12A -3(5) . . . . ?
O5A O5 W5 O2 -161(3) . . . . ?
W2 O5 W5 O2 -79(6) . . . . ?
O5A O5 W5 O18 128(4) . . . . ?
W2 O5 W5 O18 -150(5) . . . . ?
W2 O5 W5 O5A 82(6) . . . . ?
O5A O5 W5 O12B -59(4) . . . . ?
W2 O5 W5 O12B 23(5) . . . . ?
O5A O5 W5 O19 -122(5) . . . . ?
W2 O5 W5 O19 -39(4) . . . . ?
O5A O5 W5 O3 -171(4) . . . . ?
W2 O5 W5 O3 -88(5) . . . . ?
W3 O2 W5 O11 148(2) . . . . ?
W3 O2 W5 O12A -97(3) . . . . ?
W3 O2 W5 O5 -18(4) . . . . ?
W3 O2 W5 O18 49(2) . . . . ?
W3 O2 W5 O5A -52(7) . . . . ?
W3 O2 W5 O12B -120(2) . . . . ?
W3 O2 W5 O19 -49(2) . . . . ?
W3 O2 W5 O3 -7.6(19) . . . . ?
W1 O13 W6 O10 150(2) . . . . ?
W1 O13 W6 O12A -96(3) . . . 2_567 ?
W1 O13 W6 O6 -44(4) . . . 2_567 ?
W1 O13 W6 O9 48(2) . . . . ?
W1 O13 W6 O12B -120(2) . . . 2_567 ?
W1 O13 W6 O19 -51(2) . . . 2_567 ?
W1 O13 W6 O14 -12(2) . . . . ?
C4 N1 N2 C3 -4(3) . . . . ?
Cu1 N1 N2 C3 -170(2) . . . . ?
C4 N1 N2 Cu2 178(2) . . . . ?
Cu1 N1 N2 Cu2 12(3) . . . . ?
C2 N3 N4 C1 -4(3) . . . . ?
Cu1 N3 N4 C1 167(2) . . . . ?
C2 N3 N4 Cu2 -175.6(18) . . . . ?
Cu1 N3 N4 Cu2 -4(3) . . . . ?
N3 N4 C1 N9 6(3) . . . . ?
Cu2 N4 C1 N9 177.0(19) . . . . ?
C2 N9 C1 N4 -5(4) . . . . ?
N4 N3 C2 N9 1(3) . . . . ?
Cu1 N3 C2 N9 -168.7(16) . . . . ?
C1 N9 C2 N3 2(3) . . . . ?
N1 N2 C3 N11 3(3) . . . . ?
Cu2 N2 C3 N11 -179.1(19) . . . . ?
C4 N11 C3 N2 -1(3) . . . . ?
Cu4 N11 C3 N2 176(2) . . . . ?
N2 N1 C4 N11 3(3) . . . . ?
Cu1 N1 C4 N11 168.9(17) . . . . ?
C3 N11 C4 N1 -2(3) . . . . ?
Cu4 N11 C4 N1 -178(2) . . . . ?
C6 N8 N7 C7 -2(3) . . . . ?
Cu3 N8 N7 C7 -177.8(19) . . . . ?
C6 N8 N7 Cu2 -167(2) . . . . ?
Cu3 N8 N7 Cu2 18(3) . . . . ?
N7 N8 C6 N10 1(3) . . . . ?
Cu3 N8 C6 N10 176.0(18) . . . . ?
C7 N10 C6 N8 1(3) . . . . ?
Cu4 N10 C6 N8 -177.9(19) 1_455 . . . ?
C6 N10 C7 N7 -2(3) . . . . ?
Cu4 N10 C7 N7 176.6(19) 1_455 . . . ?
N8 N7 C7 N10 3(3) . . . . ?
Cu2 N7 C7 N10 166.5(19) . . . . ?
C5 N5 N6 C8 -2(3) . . . . ?
Cu3 N5 N6 C8 177(2) . . . . ?
C5 N5 N6 Cu2 -174(2) . . . . ?
Cu3 N5 N6 Cu2 5(3) . . . . ?
N5 N6 C8 N12 1(4) . . . . ?
Cu2 N6 C8 N12 172(2) . . . . ?
N6 C8 N12 C5 1(4) . . . . ?
N6 N5 C5 N12 2(4) . . . . ?
Cu3 N5 C5 N12 -177(2) . . . . ?
C8 N12 C5 N5 -2(4) . . . . ?

_refine_diff_density_max         5.409
_refine_diff_density_min         -3.209
_refine_diff_density_rms         0.449

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_4
_audit_block_doi                 10.5517/cc13895v
_database_code_depnum_ccdc_archive 'CCDC 1020866'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C16 H50 Cl2 Cu6 N24 O55 Si W12'
_chemical_formula_sum            'C16 H50 Cl2 Cu6 N24 O55 Si W12'
_chemical_formula_weight         4145.23

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.5350(5)
_cell_length_b                   12.0910(5)
_cell_length_c                   14.3130(5)
_cell_angle_alpha                94.051(5)
_cell_angle_beta                 105.611(5)
_cell_angle_gamma                105.770(5)
_cell_volume                     1827.83(14)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.800
_cell_measurement_theta_max      25.000

_exptl_crystal_description       block
_exptl_crystal_colour            'dark green'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    3.766
_exptl_crystal_F_000             1864
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.16
_exptl_absorpt_coefficient_mu    20.703
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.032
_exptl_absorpt_correction_T_max  0.035
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            10539
_diffrn_reflns_av_unetI/netI     0.0694
_diffrn_reflns_av_R_equivalents  0.0371
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_theta_min         1.771
_diffrn_reflns_theta_max         24.997
_diffrn_reflns_theta_full        24.997
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 0.996
_reflns_number_total             6404
_reflns_number_gt                4948
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
The restraint command 'DELU' was refined the atoms Si1,W1,W2,W3,W4,W5,W6,
 O3,O8,O9,O12,O15,N4 and N7. And the restraint command 'ISOR' was used to refine 
 O3,O8,O12,N1,N4,N9,N11,C3,C7 and C8 atoms.The restraint order 'SIMU' was refined
 the atoms o1,o5,o8,W1,W2,W5 and W6.   
 The 'OMIT' order was used to confirm the data completeless. 
 Due to high levels of disorder about the solvent, we removed the 
 electronic contribution of the unidentified solvent with SQUEEZE. 
 In this P-1 space group with Z = 1 this implies that the 156 removed electrons would 
 all be associated with the disordered water of the formula unit and thus 
 implies that the contributions of 156/10 = 16 additional water molecules 
 should be associated with the Formula unit. When the electron density, TGA, 
 and elemental analysis are taken into account, 15 water molecules are determined.
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.000 0.000 340 156 ' '
_platon_squeeze_details          
;
;
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0887P)²+94.5388P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         6404
_refine_ls_number_parameters     505
_refine_ls_number_restraints     730
_refine_ls_R_factor_all          0.0904
_refine_ls_R_factor_gt           0.0688
_refine_ls_wR_factor_ref         0.1862
_refine_ls_wR_factor_gt          0.1701
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_restrained_S_all      1.019
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O -0.0184(16) 0.2243(15) 0.3404(14) 0.046(2) Uani 1 1 d . U . . .
O2 O 0.2173(16) 0.2322(15) 0.4173(13) 0.043(2) Uani 1 1 d . U . . .
O3 O 0.1402(13) 0.0798(12) 0.5813(10) 0.0227(7) Uani 1 1 d . U . . .
O4A O 0.301(3) 0.135(3) 0.549(3) 0.038(2) Uani 0.5 1 d . U P . .
O4B O 0.370(3) 0.179(3) 0.594(3) 0.037(2) Uani 0.5 1 d . U P . .
O5 O 0.2626(17) 0.0516(15) 0.7109(14) 0.046(2) Uani 1 1 d . U . . .
O6 O 0.4686(18) 0.0168(16) 0.6566(16) 0.055(4) Uani 1 1 d . U . . .
O7 O 0.2295(17) -0.1472(16) 0.6171(14) 0.051(2) Uani 1 1 d . U . . .
O8 O 0.1007(15) -0.0730(14) 0.4986(12) 0.0344(13) Uani 1 1 d . U . . .
O9 O 0.2911(18) -0.0394(16) 0.4700(16) 0.0564(18) Uani 1 1 d . U . . .
O10 O 0.1047(18) -0.2456(17) 0.4297(15) 0.055(3) Uani 1 1 d . U . . .
O11 O 0.2348(19) -0.1750(16) 0.2942(16) 0.058(4) Uani 1 1 d . U . . .
O12 O 0.0204(15) -0.0169(13) 0.3952(12) 0.0315(10) Uani 1 1 d . U . . .
O15 O 0.0478(14) 0.1240(12) 0.4643(11) 0.0256(7) Uani 1 1 d . U . . .
O16 O 0.0984(16) 0.3218(15) 0.5273(13) 0.041(2) Uani 1 1 d . U . . .
O17 O 0.3619(15) 0.3913(14) 0.5832(12) 0.035(2) Uani 1 1 d . U . . .
O18 O -0.108(2) 0.3836(15) 0.4241(15) 0.054(4) Uani 1 1 d . U . . .
O19 O 0.1278(19) 0.2081(19) 0.2223(16) 0.063(5) Uani 1 1 d . U . . .
O20 O 0.1746(17) 0.0289(15) 0.3169(14) 0.047(2) Uani 1 1 d . U . . .
O21A O 0.192(3) 0.232(3) 0.660(3) 0.036(2) Uani 0.5 1 d . U P . .
O21B O 0.249(3) 0.271(3) 0.704(3) 0.033(3) Uani 0.5 1 d . U P . .
O22 O 0.2337(19) 0.1840(17) 0.8638(14) 0.057(4) Uani 1 1 d . U . . .
O23 O 0.0641(17) -0.0260(15) 0.7629(14) 0.046(3) Uani 1 1 d . U . . .
O24 O -0.0070(17) -0.1729(16) 0.2780(15) 0.051(3) Uani 1 1 d . U . . .
Si1 Si 0.0000 0.0000 0.5000 0.0280(13) Uani 1 2 d S U P . .
Cu1 Cu 0.5000 0.5000 0.5000 0.0187(7) Uani 1 2 d S . P . .
Cu2 Cu 0.5310(2) 0.5122(3) 0.76132(19) 0.0263(6) Uani 1 1 d . . . . .
Cu3 Cu 0.5000 0.5000 1.0000 0.0316(9) Uani 1 2 d S . P . .
W1 W 0.15632(11) 0.12538(9) 0.74777(7) 0.0399(3) Uani 1 1 d . U . . .
W2 W 0.31421(9) 0.00704(10) 0.60525(10) 0.0463(3) Uani 1 1 d . U . . .
W3 W 0.15818(9) -0.12084(9) 0.35890(8) 0.0361(3) Uani 1 1 d . U . . .
W4 W 0.24191(9) 0.26557(7) 0.55830(8) 0.0338(3) Uani 1 1 d . U . . .
W5 W 0.08776(9) 0.13962(8) 0.31011(7) 0.0306(3) Uani 1 1 d . U . . .
W6 W -0.07232(9) 0.26029(7) 0.44999(8) 0.0319(3) Uani 1 1 d . U . . .
N1 N 0.5299(16) 0.3703(16) 0.9230(13) 0.026(4) Uani 1 1 d . U . . .
N2 N 0.5384(17) 0.3696(18) 0.8291(13) 0.032(5) Uani 1 1 d . . . . .
N3 N 0.6557(17) 0.4885(18) 0.7012(13) 0.031(4) Uani 1 1 d . . . . .
N4 N 0.6476(15) 0.4849(14) 0.6015(11) 0.018(3) Uani 1 1 d . U . . .
N5 N 0.5230(18) 0.6445(17) 0.6849(14) 0.031(4) Uani 1 1 d . . . . .
N6 N 0.5026(15) 0.6397(16) 0.5860(11) 0.021(4) Uani 1 1 d . . . . .
N7 N 0.531(2) 0.819(2) 0.6452(18) 0.052(6) Uani 1 1 d . U . . .
H10 H 0.5418 0.8927 0.6506 0.063 Uiso 1 1 calc R U . . .
N9 N 0.559(2) 0.2090(19) 0.8736(16) 0.045(5) Uani 1 1 d . U . . .
H9 H 0.5702 0.1413 0.8739 0.053 Uiso 1 1 calc R U . . .
N10 N 0.8390(15) 0.4834(16) 0.6833(13) 0.024(4) Uani 1 1 d . . . . .
Cl1 Cl 0.6683(6) 0.6439(6) 0.9217(4) 0.0471(16) Uani 1 1 d . . . . .
C1 C 0.559(3) 0.275(3) 0.802(2) 0.058(8) Uani 1 1 d . . . . .
H1 H 0.5711 0.2556 0.7424 0.070 Uiso 1 1 calc R U . . .
C2 C 0.7590(19) 0.4795(19) 0.5940(15) 0.024(5) Uani 1 1 d . . . . .
H2 H 0.7787 0.4739 0.5354 0.029 Uiso 1 1 calc R U . . .
C3 C 0.773(2) 0.492(2) 0.7466(17) 0.029(5) Uani 1 1 d . U . . .
H3 H 0.8063 0.5001 0.8144 0.035 Uiso 1 1 calc R U . . .
C4 C 0.532(3) 0.751(2) 0.718(2) 0.054(7) Uani 1 1 d . U . . .
H4 H 0.5385 0.7767 0.7820 0.064 Uiso 1 1 calc R U . . .
C5 C 0.509(2) 0.7472(19) 0.567(2) 0.040(6) Uani 1 1 d . . . . .
H5 H 0.4986 0.7680 0.5049 0.048 Uiso 1 1 calc R U . . .
C6 C 0.540(3) 0.271(3) 0.942(2) 0.056(8) Uani 1 1 d . . . . .
H6 H 0.5344 0.2456 1.0007 0.067 Uiso 1 1 calc R U . . .
Cu4 Cu 1.0103(2) 0.4904(3) 0.7254(2) 0.0379(7) Uani 1 1 d . . . . .
N8 N 1.1792(16) 0.5003(18) 0.7800(13) 0.032(5) Uani 1 1 d . . . . .
C7 C 1.270(2) 0.516(2) 0.7365(17) 0.030(5) Uani 1 1 d . U . . .
H7 H 1.2569 0.5255 0.6710 0.037 Uiso 1 1 calc R U . . .
C8 C 1.242(2) 0.491(2) 0.8736(17) 0.033(5) Uani 1 1 d . U . . .
H8 H 1.2042 0.4799 0.9237 0.040 Uiso 1 1 calc R U . . .
O1W O 0.538(4) -0.019(3) 0.895(3) 0.140(10) Uani 1 1 d . U . . .
N11 N 1.3759(16) 0.5168(15) 0.7932(12) 0.023(4) Uani 1 1 d . U . . .
N12 N 1.3605(18) 0.501(2) 0.8840(14) 0.037(5) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 W6 1.901(19) . ?
O1 W5 1.908(18) . ?
O2 W5 1.858(18) . ?
O2 W4 1.957(18) . ?
O3 Si1 1.697(15) . ?
O3 W4 2.326(13) . ?
O3 W1 2.352(14) . ?
O3 W2 2.357(14) . ?
O4A O4B 0.88(4) . ?
O4A W2 1.82(3) . ?
O4A W4 1.89(3) . ?
O4B W4 2.01(3) . ?
O4B W2 2.03(3) . ?
O5 W1 1.858(19) . ?
O5 W2 1.865(19) . ?
O6 W2 1.701(19) . ?
O7 W2 1.899(18) . ?
O7 W6 1.899(18) 2_556 ?
O8 Si1 1.642(15) . ?
O8 O12 1.80(2) . ?
O8 W3 2.351(15) . ?
O8 W6 2.396(16) 2_556 ?
O8 W2 2.409(16) . ?
O9 W3 1.870(19) . ?
O9 W2 1.90(2) . ?
O10 W6 1.87(2) 2_556 ?
O10 W3 1.932(19) . ?
O11 W3 1.654(19) . ?
O12 Si1 1.587(15) . ?
O12 O15 1.81(2) . ?
O12 W5 2.389(14) . ?
O12 W3 2.411(15) . ?
O12 W1 2.447(17) 2_556 ?
O15 Si1 1.620(14) . ?
O15 W5 2.383(14) . ?
O15 W4 2.392(15) . ?
O15 W6 2.411(14) . ?
O16 W6 1.889(17) . ?
O16 W4 1.913(17) . ?
O17 W4 1.693(16) . ?
O17 Cu1 2.406(16) . ?
O18 W6 1.689(16) . ?
O19 W5 1.652(19) . ?
O20 W5 1.871(19) . ?
O20 W3 1.925(18) . ?
O21A O21B 0.79(4) . ?
O21A W4 1.74(3) . ?
O21A W1 1.91(3) . ?
O21B W1 2.03(3) . ?
O21B W4 2.06(3) . ?
O22 W1 1.658(19) . ?
O23 W5 1.885(17) 2_556 ?
O23 W1 1.910(17) . ?
O24 W3 1.850(19) . ?
O24 W1 1.91(2) 2_556 ?
Si1 O12 1.587(15) 2_556 ?
Si1 O15 1.620(14) 2_556 ?
Si1 O8 1.642(15) 2_556 ?
Si1 O3 1.697(15) 2_556 ?
Cu1 N4 1.980(16) . ?
Cu1 N4 1.980(16) 2_666 ?
Cu1 N6 2.007(17) . ?
Cu1 N6 2.007(17) 2_666 ?
Cu1 O17 2.406(16) 2_666 ?
Cu2 N3 1.936(19) . ?
Cu2 N11 1.975(17) 1_455 ?
Cu2 N5 2.009(19) . ?
Cu2 N2 2.05(2) . ?
Cu2 Cl1 2.543(7) . ?
Cu3 N12 1.982(19) 2_767 ?
Cu3 N12 1.982(19) 1_455 ?
Cu3 N1 2.012(18) 2_667 ?
Cu3 N1 2.012(18) . ?
Cu3 Cl1 2.769(7) 2_667 ?
Cu3 Cl1 2.769(7) . ?
W1 O24 1.91(2) 2_556 ?
W1 O12 2.447(17) 2_556 ?
W5 O23 1.885(17) 2_556 ?
W6 O10 1.87(2) 2_556 ?
W6 O7 1.899(18) 2_556 ?
W6 O8 2.396(16) 2_556 ?
N1 C6 1.28(3) . ?
N1 N2 1.37(2) . ?
N2 C1 1.28(3) . ?
N3 C3 1.32(3) . ?
N3 N4 1.40(2) . ?
N4 C2 1.34(3) . ?
N5 C4 1.30(3) . ?
N5 N6 1.37(2) . ?
N6 C5 1.33(3) . ?
N7 C5 1.29(3) . ?
N7 C4 1.37(4) . ?
N7 H10 0.8600 . ?
N9 C6 1.29(4) . ?
N9 C1 1.34(4) . ?
N9 H9 0.8600 . ?
N10 C3 1.35(3) . ?
N10 C2 1.35(3) . ?
N10 Cu4 1.880(16) . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 H4 0.9300 . ?
C5 H5 0.9300 . ?
C6 H6 0.9300 . ?
Cu4 N8 1.861(17) . ?
N8 C7 1.33(3) . ?
N8 C8 1.37(3) . ?
C7 N11 1.27(3) . ?
C7 H7 0.9300 . ?
C8 N12 1.31(3) . ?
C8 H8 0.9300 . ?
N11 N12 1.38(2) . ?
N11 Cu2 1.975(17) 1_655 ?
N12 Cu3 1.982(18) 1_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W6 O1 W5 137.3(11) . . ?
W5 O2 W4 135.4(10) . . ?
Si1 O3 W4 120.4(7) . . ?
Si1 O3 W1 120.3(6) . . ?
W4 O3 W1 97.6(5) . . ?
Si1 O3 W2 118.8(7) . . ?
W4 O3 W2 97.1(5) . . ?
W1 O3 W2 97.5(5) . . ?
O4B O4A W2 91(3) . . ?
O4B O4A W4 85(3) . . ?
W2 O4A W4 142(2) . . ?
O4A O4B W4 69(3) . . ?
O4A O4B W2 64(3) . . ?
W4 O4B W2 120.4(17) . . ?
W1 O5 W2 143.9(11) . . ?
W2 O7 W6 136.1(11) . 2_556 ?
Si1 O8 O12 54.6(7) . . ?
Si1 O8 W3 124.1(9) . . ?
O12 O8 W3 69.5(7) . . ?
Si1 O8 W6 121.4(8) . 2_556 ?
O12 O8 W6 134.9(10) . 2_556 ?
W3 O8 W6 96.3(6) . 2_556 ?
Si1 O8 W2 118.6(8) . . ?
O12 O8 W2 128.5(9) . . ?
W3 O8 W2 95.2(5) . . ?
W6 O8 W2 94.3(6) 2_556 . ?
W3 O9 W2 137.5(11) . . ?
W6 O10 W3 137.1(12) 2_556 . ?
Si1 O12 O8 57.5(7) . . ?
Si1 O12 O15 56.5(7) . . ?
O8 O12 O15 94.8(10) . . ?
Si1 O12 W5 124.0(8) . . ?
O8 O12 W5 133.4(10) . . ?
O15 O12 W5 67.5(6) . . ?
Si1 O12 W3 123.5(8) . . ?
O8 O12 W3 66.0(7) . . ?
O15 O12 W3 133.6(9) . . ?
W5 O12 W3 94.7(5) . . ?
Si1 O12 W1 120.4(8) . 2_556 ?
O8 O12 W1 127.9(9) . 2_556 ?
O15 O12 W1 129.0(9) . 2_556 ?
W5 O12 W1 93.2(5) . 2_556 ?
W3 O12 W1 92.9(5) . 2_556 ?
Si1 O15 O12 54.7(6) . . ?
Si1 O15 W5 122.6(8) . . ?
O12 O15 W5 67.8(6) . . ?
Si1 O15 W4 120.6(8) . . ?
O12 O15 W4 129.9(9) . . ?
W5 O15 W4 95.4(5) . . ?
Si1 O15 W6 121.7(7) . . ?
O12 O15 W6 132.7(9) . . ?
W5 O15 W6 95.5(5) . . ?
W4 O15 W6 94.2(5) . . ?
W6 O16 W4 135.5(9) . . ?
W4 O17 Cu1 137.7(9) . . ?
W5 O20 W3 136.9(10) . . ?
O21B O21A W4 103(4) . . ?
O21B O21A W1 88(4) . . ?
W4 O21A W1 150(2) . . ?
O21A O21B W1 69(4) . . ?
O21A O21B W4 55(3) . . ?
W1 O21B W4 118.4(17) . . ?
W5 O23 W1 135.6(10) 2_556 . ?
W3 O24 W1 138.6(11) . 2_556 ?
O12 Si1 O12 180.0 2_556 . ?
O12 Si1 O15 111.2(7) 2_556 . ?
O12 Si1 O15 68.8(7) . . ?
O12 Si1 O15 68.8(7) 2_556 2_556 ?
O12 Si1 O15 111.2(7) . 2_556 ?
O15 Si1 O15 180.0 . 2_556 ?
O12 Si1 O8 67.8(8) 2_556 2_556 ?
O12 Si1 O8 112.2(8) . 2_556 ?
O15 Si1 O8 70.7(7) . 2_556 ?
O15 Si1 O8 109.3(7) 2_556 2_556 ?
O12 Si1 O8 112.2(8) 2_556 . ?
O12 Si1 O8 67.8(8) . . ?
O15 Si1 O8 109.3(7) . . ?
O15 Si1 O8 70.7(7) 2_556 . ?
O8 Si1 O8 180.0(8) 2_556 . ?
O12 Si1 O3 108.1(7) 2_556 2_556 ?
O12 Si1 O3 71.9(7) . 2_556 ?
O15 Si1 O3 109.1(7) . 2_556 ?
O15 Si1 O3 70.9(7) 2_556 2_556 ?
O8 Si1 O3 73.2(7) 2_556 2_556 ?
O8 Si1 O3 106.8(7) . 2_556 ?
O12 Si1 O3 71.9(7) 2_556 . ?
O12 Si1 O3 108.1(7) . . ?
O15 Si1 O3 70.9(7) . . ?
O15 Si1 O3 109.1(7) 2_556 . ?
O8 Si1 O3 106.8(7) 2_556 . ?
O8 Si1 O3 73.2(7) . . ?
O3 Si1 O3 180.0(9) 2_556 . ?
N4 Cu1 N4 180.0 . 2_666 ?
N4 Cu1 N6 89.8(7) . . ?
N4 Cu1 N6 90.2(7) 2_666 . ?
N4 Cu1 N6 90.2(7) . 2_666 ?
N4 Cu1 N6 89.8(7) 2_666 2_666 ?
N6 Cu1 N6 180.0 . 2_666 ?
N4 Cu1 O17 90.2(6) . 2_666 ?
N4 Cu1 O17 89.8(6) 2_666 2_666 ?
N6 Cu1 O17 95.1(6) . 2_666 ?
N6 Cu1 O17 84.9(6) 2_666 2_666 ?
N4 Cu1 O17 89.8(6) . . ?
N4 Cu1 O17 90.2(6) 2_666 . ?
N6 Cu1 O17 84.9(6) . . ?
N6 Cu1 O17 95.1(6) 2_666 . ?
O17 Cu1 O17 180.0 2_666 . ?
N3 Cu2 N11 166.7(7) . 1_455 ?
N3 Cu2 N5 87.1(8) . . ?
N11 Cu2 N5 90.4(7) 1_455 . ?
N3 Cu2 N2 89.7(8) . . ?
N11 Cu2 N2 91.9(7) 1_455 . ?
N5 Cu2 N2 175.4(8) . . ?
N3 Cu2 Cl1 102.1(6) . . ?
N11 Cu2 Cl1 91.1(5) 1_455 . ?
N5 Cu2 Cl1 94.1(6) . . ?
N2 Cu2 Cl1 89.7(6) . . ?
N12 Cu3 N12 180.0 2_767 1_455 ?
N12 Cu3 N1 89.2(8) 2_767 2_667 ?
N12 Cu3 N1 90.8(8) 1_455 2_667 ?
N12 Cu3 N1 90.8(8) 2_767 . ?
N12 Cu3 N1 89.2(8) 1_455 . ?
N1 Cu3 N1 180.0 2_667 . ?
N12 Cu3 Cl1 88.9(6) 2_767 2_667 ?
N12 Cu3 Cl1 91.1(6) 1_455 2_667 ?
N1 Cu3 Cl1 84.5(5) 2_667 2_667 ?
N1 Cu3 Cl1 95.5(5) . 2_667 ?
N12 Cu3 Cl1 91.1(6) 2_767 . ?
N12 Cu3 Cl1 88.9(6) 1_455 . ?
N1 Cu3 Cl1 95.5(5) 2_667 . ?
N1 Cu3 Cl1 84.5(5) . . ?
Cl1 Cu3 Cl1 180.0(2) 2_667 . ?
O22 W1 O5 103.6(10) . . ?
O22 W1 O21A 111.7(13) . . ?
O5 W1 O21A 87.9(11) . . ?
O22 W1 O23 101.1(9) . . ?
O5 W1 O23 85.3(8) . . ?
O21A W1 O23 147.2(13) . . ?
O22 W1 O24 103.5(10) . 2_556 ?
O5 W1 O24 152.9(8) . 2_556 ?
O21A W1 O24 80.9(12) . 2_556 ?
O23 W1 O24 90.8(8) . 2_556 ?
O22 W1 O21B 89.5(12) . . ?
O5 W1 O21B 88.2(10) . . ?
O21A W1 O21B 22.8(12) . . ?
O23 W1 O21B 168.6(11) . . ?
O24 W1 O21B 90.7(11) 2_556 . ?
O22 W1 O3 154.0(8) . . ?
O5 W1 O3 59.1(7) . . ?
O21A W1 O3 52.9(11) . . ?
O23 W1 O3 96.8(7) . . ?
O24 W1 O3 94.9(7) 2_556 . ?
O21B W1 O3 71.9(10) . . ?
O22 W1 O12 158.6(8) . 2_556 ?
O5 W1 O12 91.2(7) . 2_556 ?
O21A W1 O12 83.8(12) . 2_556 ?
O23 W1 O12 64.4(6) . 2_556 ?
O24 W1 O12 63.1(7) 2_556 2_556 ?
O21B W1 O12 106.5(11) . 2_556 ?
O3 W1 O12 47.4(5) . 2_556 ?
O6 W2 O4A 110.4(13) . . ?
O6 W2 O5 104.1(9) . . ?
O4A W2 O5 93.8(12) . . ?
O6 W2 O7 102.4(9) . . ?
O4A W2 O7 146.3(13) . . ?
O5 W2 O7 85.3(8) . . ?
O6 W2 O9 101.7(10) . . ?
O4A W2 O9 75.5(13) . . ?
O5 W2 O9 154.1(8) . . ?
O7 W2 O9 90.8(8) . . ?
O6 W2 O4B 88.6(12) . . ?
O4A W2 O4B 25.5(12) . . ?
O5 W2 O4B 86.6(11) . . ?
O7 W2 O4B 167.7(11) . . ?
O9 W2 O4B 92.5(11) . . ?
O6 W2 O3 152.8(8) . . ?
O4A W2 O3 55.0(11) . . ?
O5 W2 O3 58.9(7) . . ?
O7 W2 O3 97.4(7) . . ?
O9 W2 O3 96.4(7) . . ?
O4B W2 O3 70.4(10) . . ?
O6 W2 O8 157.7(8) . . ?
O4A W2 O8 81.9(12) . . ?
O5 W2 O8 93.1(7) . . ?
O7 W2 O8 64.5(7) . . ?
O9 W2 O8 62.4(7) . . ?
O4B W2 O8 106.8(11) . . ?
O3 W2 O8 49.4(5) . . ?
O11 W3 O24 102.8(10) . . ?
O11 W3 O9 100.9(10) . . ?
O24 W3 O9 156.2(9) . . ?
O11 W3 O20 100.5(9) . . ?
O24 W3 O20 89.4(8) . . ?
O9 W3 O20 85.0(8) . . ?
O11 W3 O10 102.5(10) . . ?
O24 W3 O10 84.9(8) . . ?
O9 W3 O10 91.3(8) . . ?
O20 W3 O10 157.0(9) . . ?
O11 W3 O8 157.1(9) . . ?
O24 W3 O8 93.6(8) . . ?
O9 W3 O8 64.1(8) . . ?
O20 W3 O8 95.4(7) . . ?
O10 W3 O8 62.9(8) . . ?
O11 W3 O12 158.3(9) . . ?
O24 W3 O12 64.6(7) . . ?
O9 W3 O12 92.3(8) . . ?
O20 W3 O12 63.4(7) . . ?
O10 W3 O12 94.2(7) . . ?
O8 W3 O12 44.5(6) . . ?
O17 W4 O21A 112.7(13) . . ?
O17 W4 O4A 111.0(12) . . ?
O21A W4 O4A 94.4(15) . . ?
O17 W4 O16 101.3(7) . . ?
O21A W4 O16 82.2(12) . . ?
O4A W4 O16 146.0(12) . . ?
O17 W4 O2 97.8(7) . . ?
O21A W4 O2 149.2(13) . . ?
O4A W4 O2 77.4(12) . . ?
O16 W4 O2 88.3(7) . . ?
O17 W4 O4B 89.0(11) . . ?
O21A W4 O4B 91.1(15) . . ?
O4A W4 O4B 25.8(12) . . ?
O16 W4 O4B 169.3(11) . . ?
O2 W4 O4B 93.3(11) . . ?
O17 W4 O21B 91.7(11) . . ?
O21A W4 O21B 21.8(12) . . ?
O4A W4 O21B 96.9(14) . . ?
O16 W4 O21B 92.2(10) . . ?
O2 W4 O21B 170.1(11) . . ?
O4B W4 O21B 84.4(13) . . ?
O17 W4 O3 155.3(7) . . ?
O21A W4 O3 54.7(12) . . ?
O4A W4 O3 55.1(11) . . ?
O16 W4 O3 97.8(6) . . ?
O2 W4 O3 98.2(6) . . ?
O4B W4 O3 71.5(10) . . ?
O21B W4 O3 71.9(10) . . ?
O17 W4 O15 156.3(7) . . ?
O21A W4 O15 85.7(13) . . ?
O4A W4 O15 81.0(12) . . ?
O16 W4 O15 65.1(6) . . ?
O2 W4 O15 63.9(6) . . ?
O4B W4 O15 106.2(11) . . ?
O21B W4 O15 107.5(10) . . ?
O3 W4 O15 48.1(5) . . ?
O19 W5 O2 98.7(9) . . ?
O19 W5 O20 101.6(10) . . ?
O2 W5 O20 88.8(8) . . ?
O19 W5 O23 100.9(9) . 2_556 ?
O2 W5 O23 160.0(8) . 2_556 ?
O20 W5 O23 90.7(8) . 2_556 ?
O19 W5 O1 99.5(10) . . ?
O2 W5 O1 88.0(8) . . ?
O20 W5 O1 158.9(8) . . ?
O23 W5 O1 85.3(8) 2_556 . ?
O19 W5 O15 155.8(9) . . ?
O2 W5 O15 65.3(7) . . ?
O20 W5 O15 96.3(7) . . ?
O23 W5 O15 95.0(7) 2_556 . ?
O1 W5 O15 63.6(7) . . ?
O19 W5 O12 159.5(9) . . ?
O2 W5 O12 96.0(7) . . ?
O20 W5 O12 64.5(7) . . ?
O23 W5 O12 66.0(7) 2_556 . ?
O1 W5 O12 95.2(7) . . ?
O15 W5 O12 44.6(5) . . ?
O18 W6 O10 102.0(10) . 2_556 ?
O18 W6 O16 100.8(9) . . ?
O10 W6 O16 84.6(8) 2_556 . ?
O18 W6 O7 100.4(9) . 2_556 ?
O10 W6 O7 91.0(8) 2_556 2_556 ?
O16 W6 O7 158.7(8) . 2_556 ?
O18 W6 O1 100.3(9) . . ?
O10 W6 O1 157.6(9) 2_556 . ?
O16 W6 O1 89.4(8) . . ?
O7 W6 O1 86.7(8) 2_556 . ?
O18 W6 O8 156.9(8) . 2_556 ?
O10 W6 O8 62.6(7) 2_556 2_556 ?
O16 W6 O8 95.0(7) . 2_556 ?
O7 W6 O8 64.8(7) 2_556 2_556 ?
O1 W6 O8 96.6(7) . 2_556 ?
O18 W6 O15 156.9(8) . . ?
O10 W6 O15 95.0(7) 2_556 . ?
O16 W6 O15 64.9(6) . . ?
O7 W6 O15 94.9(7) 2_556 . ?
O1 W6 O15 63.1(7) . . ?
O8 W6 O15 46.2(5) 2_556 . ?
C6 N1 N2 103(2) . . ?
C6 N1 Cu3 132.4(19) . . ?
N2 N1 Cu3 124.8(14) . . ?
C1 N2 N1 109(2) . . ?
C1 N2 Cu2 131.3(19) . . ?
N1 N2 Cu2 119.7(15) . . ?
C3 N3 N4 105.5(17) . . ?
C3 N3 Cu2 127.1(15) . . ?
N4 N3 Cu2 126.6(13) . . ?
C2 N4 N3 106.5(15) . . ?
C2 N4 Cu1 129.8(13) . . ?
N3 N4 Cu1 123.5(12) . . ?
C4 N5 N6 106(2) . . ?
C4 N5 Cu2 127.9(19) . . ?
N6 N5 Cu2 126.4(14) . . ?
C5 N6 N5 106.3(19) . . ?
C5 N6 Cu1 130.0(16) . . ?
N5 N6 Cu1 122.6(13) . . ?
C5 N7 C4 104(2) . . ?
C5 N7 H10 128.1 . . ?
C4 N7 H10 128.1 . . ?
C6 N9 C1 103(2) . . ?
C6 N9 H9 128.3 . . ?
C1 N9 H9 128.3 . . ?
C3 N10 C2 104.9(17) . . ?
C3 N10 Cu4 122.4(15) . . ?
C2 N10 Cu4 132.5(14) . . ?
Cu2 Cl1 Cu3 83.4(2) . . ?
N2 C1 N9 110(3) . . ?
N2 C1 H1 125.2 . . ?
N9 C1 H1 125.2 . . ?
N4 C2 N10 110.7(17) . . ?
N4 C2 H2 124.6 . . ?
N10 C2 H2 124.6 . . ?
N3 C3 N10 112.2(19) . . ?
N3 C3 H3 123.9 . . ?
N10 C3 H3 123.9 . . ?
N5 C4 N7 112(2) . . ?
N5 C4 H4 124.2 . . ?
N7 C4 H4 124.2 . . ?
N7 C5 N6 112(3) . . ?
N7 C5 H5 123.8 . . ?
N6 C5 H5 123.8 . . ?
N1 C6 N9 115(3) . . ?
N1 C6 H6 122.3 . . ?
N9 C6 H6 122.3 . . ?
N8 Cu4 N10 174.2(8) . . ?
C7 N8 C8 102.3(18) . . ?
C7 N8 Cu4 128.4(15) . . ?
C8 N8 Cu4 129.3(16) . . ?
N11 C7 N8 114(2) . . ?
N11 C7 H7 123.2 . . ?
N8 C7 H7 123.2 . . ?
N12 C8 N8 111(2) . . ?
N12 C8 H8 124.3 . . ?
N8 C8 H8 124.3 . . ?
C7 N11 N12 107.3(18) . . ?
C7 N11 Cu2 129.4(15) . 1_655 ?
N12 N11 Cu2 122.5(13) . 1_655 ?
C8 N12 N11 105.4(18) . . ?
C8 N12 Cu3 131.3(16) . 1_655 ?
N11 N12 Cu3 123.2(14) . 1_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
W2 O4A O4B W4 -142.4(18) . . . . ?
W4 O4A O4B W2 142.4(18) . . . . ?
W3 O8 O12 Si1 179.3(7) . . . . ?
W6 O8 O12 Si1 101.2(12) 2_556 . . . ?
W2 O8 O12 Si1 -100.7(11) . . . . ?
Si1 O8 O12 O15 44.7(7) . . . . ?
W3 O8 O12 O15 -136.0(8) . . . . ?
W6 O8 O12 O15 145.9(11) 2_556 . . . ?
W2 O8 O12 O15 -56.0(12) . . . . ?
Si1 O8 O12 W5 108.0(12) . . . . ?
W3 O8 O12 W5 -72.7(11) . . . . ?
W6 O8 O12 W5 -150.8(9) 2_556 . . . ?
W2 O8 O12 W5 7.4(19) . . . . ?
Si1 O8 O12 W3 -179.3(7) . . . . ?
W6 O8 O12 W3 -78.1(11) 2_556 . . . ?
W2 O8 O12 W3 80.0(9) . . . . ?
Si1 O8 O12 W1 -105.4(10) . . . 2_556 ?
W3 O8 O12 W1 73.9(9) . . . 2_556 ?
W6 O8 O12 W1 -4.1(18) 2_556 . . 2_556 ?
W2 O8 O12 W1 154.0(7) . . . 2_556 ?
O8 O12 O15 Si1 -45.4(7) . . . . ?
W5 O12 O15 Si1 179.2(7) . . . . ?
W3 O12 O15 Si1 -106.5(12) . . . . ?
W1 O12 O15 Si1 104.2(10) 2_556 . . . ?
Si1 O12 O15 W5 -179.2(7) . . . . ?
O8 O12 O15 W5 135.4(8) . . . . ?
W3 O12 O15 W5 74.3(10) . . . . ?
W1 O12 O15 W5 -75.1(9) 2_556 . . . ?
Si1 O12 O15 W4 102.8(10) . . . . ?
O8 O12 O15 W4 57.4(12) . . . . ?
W5 O12 O15 W4 -78.0(9) . . . . ?
W3 O12 O15 W4 -3.7(18) . . . . ?
W1 O12 O15 W4 -153.0(7) 2_556 . . . ?
Si1 O12 O15 W6 -102.9(11) . . . . ?
O8 O12 O15 W6 -148.2(10) . . . . ?
W5 O12 O15 W6 76.4(9) . . . . ?
W3 O12 O15 W6 150.6(8) . . . . ?
W1 O12 O15 W6 1.3(17) 2_556 . . . ?
W4 O21A O21B W1 -152(3) . . . . ?
W1 O21A O21B W4 152(3) . . . . ?
O8 O12 Si1 O15 122.8(9) . . . . ?
W5 O12 Si1 O15 -0.9(8) . . . . ?
W3 O12 Si1 O15 123.5(11) . . . . ?
W1 O12 Si1 O15 -119.1(10) 2_556 . . . ?
O8 O12 Si1 O15 -57.2(9) . . . 2_556 ?
O15 O12 Si1 O15 180.000(4) . . . 2_556 ?
W5 O12 Si1 O15 179.1(8) . . . 2_556 ?
W3 O12 Si1 O15 -56.5(11) . . . 2_556 ?
W1 O12 Si1 O15 60.9(10) 2_556 . . 2_556 ?
O8 O12 Si1 O8 180.001(6) . . . 2_556 ?
O15 O12 Si1 O8 57.2(9) . . . 2_556 ?
W5 O12 Si1 O8 56.4(12) . . . 2_556 ?
W3 O12 Si1 O8 -179.2(8) . . . 2_556 ?
W1 O12 Si1 O8 -61.9(10) 2_556 . . 2_556 ?
O15 O12 Si1 O8 -122.8(9) . . . . ?
W5 O12 Si1 O8 -123.6(12) . . . . ?
W3 O12 Si1 O8 0.8(8) . . . . ?
W1 O12 Si1 O8 118.1(10) 2_556 . . . ?
O8 O12 Si1 O3 -117.4(9) . . . 2_556 ?
O15 O12 Si1 O3 119.8(8) . . . 2_556 ?
W5 O12 Si1 O3 118.9(11) . . . 2_556 ?
W3 O12 Si1 O3 -116.7(10) . . . 2_556 ?
W1 O12 Si1 O3 0.7(7) 2_556 . . 2_556 ?
O8 O12 Si1 O3 62.6(9) . . . . ?
O15 O12 Si1 O3 -60.2(8) . . . . ?
W5 O12 Si1 O3 -61.1(11) . . . . ?
W3 O12 Si1 O3 63.3(10) . . . . ?
W1 O12 Si1 O3 -179.3(7) 2_556 . . . ?
O12 O15 Si1 O12 179.999(3) . . . 2_556 ?
W5 O15 Si1 O12 -179.2(8) . . . 2_556 ?
W4 O15 Si1 O12 60.4(10) . . . 2_556 ?
W6 O15 Si1 O12 -57.3(11) . . . 2_556 ?
W5 O15 Si1 O12 0.8(8) . . . . ?
W4 O15 Si1 O12 -119.6(10) . . . . ?
W6 O15 Si1 O12 122.7(11) . . . . ?
O12 O15 Si1 O8 -124.4(9) . . . 2_556 ?
W5 O15 Si1 O8 -123.5(11) . . . 2_556 ?
W4 O15 Si1 O8 116.0(10) . . . 2_556 ?
W6 O15 Si1 O8 -1.7(8) . . . 2_556 ?
O12 O15 Si1 O8 55.6(9) . . . . ?
W5 O15 Si1 O8 56.5(11) . . . . ?
W4 O15 Si1 O8 -64.0(10) . . . . ?
W6 O15 Si1 O8 178.3(8) . . . . ?
O12 O15 Si1 O3 -60.9(8) . . . 2_556 ?
W5 O15 Si1 O3 -60.0(10) . . . 2_556 ?
W4 O15 Si1 O3 179.6(7) . . . 2_556 ?
W6 O15 Si1 O3 61.8(10) . . . 2_556 ?
O12 O15 Si1 O3 119.1(8) . . . . ?
W5 O15 Si1 O3 120.0(10) . . . . ?
W4 O15 Si1 O3 -0.4(7) . . . . ?
W6 O15 Si1 O3 -118.2(10) . . . . ?
O12 O8 Si1 O12 180.000(7) . . . 2_556 ?
W3 O8 Si1 O12 179.2(8) . . . 2_556 ?
W6 O8 Si1 O12 54.5(12) 2_556 . . 2_556 ?
W2 O8 Si1 O12 -61.1(11) . . . 2_556 ?
W3 O8 Si1 O12 -0.8(8) . . . . ?
W6 O8 Si1 O12 -125.5(12) 2_556 . . . ?
W2 O8 Si1 O12 118.9(11) . . . . ?
O12 O8 Si1 O15 -56.2(9) . . . . ?
W3 O8 Si1 O15 -57.0(11) . . . . ?
W6 O8 Si1 O15 178.3(8) 2_556 . . . ?
W2 O8 Si1 O15 62.7(10) . . . . ?
O12 O8 Si1 O15 123.8(9) . . . 2_556 ?
W3 O8 Si1 O15 123.0(11) . . . 2_556 ?
W6 O8 Si1 O15 -1.7(8) 2_556 . . 2_556 ?
W2 O8 Si1 O15 -117.3(10) . . . 2_556 ?
O12 O8 Si1 O3 61.8(8) . . . 2_556 ?
W3 O8 Si1 O3 61.0(10) . . . 2_556 ?
W6 O8 Si1 O3 -63.7(10) 2_556 . . 2_556 ?
W2 O8 Si1 O3 -179.4(7) . . . 2_556 ?
O12 O8 Si1 O3 -118.2(8) . . . . ?
W3 O8 Si1 O3 -119.0(10) . . . . ?
W6 O8 Si1 O3 116.3(10) 2_556 . . . ?
W2 O8 Si1 O3 0.6(7) . . . . ?
W4 O3 Si1 O12 -120.6(9) . . . 2_556 ?
W1 O3 Si1 O12 0.7(8) . . . 2_556 ?
W2 O3 Si1 O12 120.2(9) . . . 2_556 ?
W4 O3 Si1 O12 59.4(9) . . . . ?
W1 O3 Si1 O12 -179.3(8) . . . . ?
W2 O3 Si1 O12 -59.8(9) . . . . ?
W4 O3 Si1 O15 0.4(7) . . . . ?
W1 O3 Si1 O15 121.7(9) . . . . ?
W2 O3 Si1 O15 -118.7(9) . . . . ?
W4 O3 Si1 O15 -179.6(7) . . . 2_556 ?
W1 O3 Si1 O15 -58.3(9) . . . 2_556 ?
W2 O3 Si1 O15 61.3(9) . . . 2_556 ?
W4 O3 Si1 O8 -61.5(9) . . . 2_556 ?
W1 O3 Si1 O8 59.8(9) . . . 2_556 ?
W2 O3 Si1 O8 179.4(7) . . . 2_556 ?
W4 O3 Si1 O8 118.5(9) . . . . ?
W1 O3 Si1 O8 -120.2(9) . . . . ?
W2 O3 Si1 O8 -0.6(7) . . . . ?
W2 O5 W1 O22 -149.4(17) . . . . ?
W2 O5 W1 O21A -38(2) . . . . ?
W2 O5 W1 O23 110.3(18) . . . . ?
W2 O5 W1 O24 28(3) . . . 2_556 ?
W2 O5 W1 O21B -60.4(19) . . . . ?
W2 O5 W1 O3 9.5(14) . . . . ?
W2 O5 W1 O12 46.1(17) . . . 2_556 ?
O4B O4A W2 O6 -33(4) . . . . ?
W4 O4A W2 O6 -116(3) . . . . ?
O4B O4A W2 O5 74(3) . . . . ?
W4 O4A W2 O5 -9(3) . . . . ?
O4B O4A W2 O7 161(3) . . . . ?
W4 O4A W2 O7 78(4) . . . . ?
O4B O4A W2 O9 -130(4) . . . . ?
W4 O4A W2 O9 147(4) . . . . ?
W4 O4A W2 O4B -83(5) . . . . ?
O4B O4A W2 O3 121(4) . . . . ?
W4 O4A W2 O3 38(3) . . . . ?
O4B O4A W2 O8 167(4) . . . . ?
W4 O4A W2 O8 84(3) . . . . ?
W1 O5 W2 O6 147.3(17) . . . . ?
W1 O5 W2 O4A 35(2) . . . . ?
W1 O5 W2 O7 -111.1(18) . . . . ?
W1 O5 W2 O9 -29(3) . . . . ?
W1 O5 W2 O4B 59.7(19) . . . . ?
W1 O5 W2 O3 -9.5(14) . . . . ?
W1 O5 W2 O8 -47.0(17) . . . . ?
W6 O7 W2 O6 -154.5(16) 2_556 . . . ?
W6 O7 W2 O4A 12(3) 2_556 . . . ?
W6 O7 W2 O5 102.0(17) 2_556 . . . ?
W6 O7 W2 O9 -52.4(17) 2_556 . . . ?
W6 O7 W2 O4B 53(6) 2_556 . . . ?
W6 O7 W2 O3 44.2(17) 2_556 . . . ?
W6 O7 W2 O8 6.3(13) 2_556 . . . ?
W1 O24 W3 O11 -151.5(16) 2_556 . . . ?
W1 O24 W3 O9 25(3) 2_556 . . . ?
W1 O24 W3 O20 -50.8(16) 2_556 . . . ?
W1 O24 W3 O10 106.9(17) 2_556 . . . ?
W1 O24 W3 O8 44.5(16) 2_556 . . . ?
W1 O24 W3 O12 9.7(13) 2_556 . . . ?
W2 O9 W3 O11 -152.0(16) . . . . ?
W2 O9 W3 O24 31(3) . . . . ?
W2 O9 W3 O20 108.3(16) . . . . ?
W2 O9 W3 O10 -49.0(17) . . . . ?
W2 O9 W3 O8 9.8(13) . . . . ?
W2 O9 W3 O12 45.3(16) . . . . ?
Cu1 O17 W4 O21A 174.4(15) . . . . ?
Cu1 O17 W4 O4A 70.0(17) . . . . ?
Cu1 O17 W4 O16 -99.3(13) . . . . ?
Cu1 O17 W4 O2 -9.6(14) . . . . ?
Cu1 O17 W4 O4B 83.7(15) . . . . ?
Cu1 O17 W4 O21B 168.0(15) . . . . ?
Cu1 O17 W4 O3 120.6(14) . . . . ?
Cu1 O17 W4 O15 -47(2) . . . . ?
O21B O21A W4 O17 -17(4) . . . . ?
W1 O21A W4 O17 -126(4) . . . . ?
O21B O21A W4 O4A 98(4) . . . . ?
W1 O21A W4 O4A -11(5) . . . . ?
O21B O21A W4 O16 -116(4) . . . . ?
W1 O21A W4 O16 135(4) . . . . ?
O21B O21A W4 O2 170(3) . . . . ?
W1 O21A W4 O2 61(6) . . . . ?
O21B O21A W4 O4B 72(4) . . . . ?
W1 O21A W4 O4B -37(4) . . . . ?
W1 O21A W4 O21B -109(6) . . . . ?
O21B O21A W4 O3 138(4) . . . . ?
W1 O21A W4 O3 29(4) . . . . ?
O21B O21A W4 O15 178(4) . . . . ?
W1 O21A W4 O15 69(4) . . . . ?
O4B O4A W4 O17 33(4) . . . . ?
W2 O4A W4 O17 118(3) . . . . ?
O4B O4A W4 O21A -83(3) . . . . ?
W2 O4A W4 O21A 2(4) . . . . ?
O4B O4A W4 O16 -166(3) . . . . ?
W2 O4A W4 O16 -81(4) . . . . ?
O4B O4A W4 O2 127(3) . . . . ?
W2 O4A W4 O2 -148(4) . . . . ?
W2 O4A W4 O4B 85(5) . . . . ?
O4B O4A W4 O21B -61(3) . . . . ?
W2 O4A W4 O21B 23(4) . . . . ?
O4B O4A W4 O3 -124(4) . . . . ?
W2 O4A W4 O3 -39(3) . . . . ?
O4B O4A W4 O15 -168(3) . . . . ?
W2 O4A W4 O15 -83(3) . . . . ?
W4 O2 W5 O19 157.6(15) . . . . ?
W4 O2 W5 O20 -100.9(14) . . . . ?
W4 O2 W5 O23 -12(3) . . . 2_556 ?
W4 O2 W5 O1 58.3(14) . . . . ?
W4 O2 W5 O15 -3.4(11) . . . . ?
W4 O2 W5 O12 -36.7(14) . . . . ?
W3 O20 W5 O19 -155.7(15) . . . . ?
W3 O20 W5 O2 105.7(15) . . . . ?
W3 O20 W5 O23 -54.4(15) . . . 2_556 ?
W3 O20 W5 O1 24(3) . . . . ?
W3 O20 W5 O15 40.7(15) . . . . ?
W3 O20 W5 O12 8.5(12) . . . . ?
W4 O16 W6 O18 -155.0(14) . . . . ?
W4 O16 W6 O10 103.8(15) . . . 2_556 ?
W4 O16 W6 O7 25(3) . . . 2_556 ?
W4 O16 W6 O1 -54.6(14) . . . . ?
W4 O16 W6 O8 41.9(14) . . . 2_556 ?
W4 O16 W6 O15 5.7(11) . . . . ?
C6 N1 N2 C1 -3(3) . . . . ?
Cu3 N1 N2 C1 179(2) . . . . ?
C6 N1 N2 Cu2 -178.8(18) . . . . ?
Cu3 N1 N2 Cu2 4(2) . . . . ?
C3 N3 N4 C2 4(2) . . . . ?
Cu2 N3 N4 C2 173.4(16) . . . . ?
C3 N3 N4 Cu1 -171.3(15) . . . . ?
Cu2 N3 N4 Cu1 -2(2) . . . . ?
C4 N5 N6 C5 4(3) . . . . ?
Cu2 N5 N6 C5 -178.1(15) . . . . ?
C4 N5 N6 Cu1 173.3(17) . . . . ?
Cu2 N5 N6 Cu1 -9(2) . . . . ?
N1 N2 C1 N9 2(3) . . . . ?
Cu2 N2 C1 N9 177.5(17) . . . . ?
C6 N9 C1 N2 -1(3) . . . . ?
N3 N4 C2 N10 -2(2) . . . . ?
Cu1 N4 C2 N10 172.6(14) . . . . ?
C3 N10 C2 N4 0(2) . . . . ?
Cu4 N10 C2 N4 -174.8(15) . . . . ?
N4 N3 C3 N10 -4(3) . . . . ?
Cu2 N3 C3 N10 -173.9(15) . . . . ?
C2 N10 C3 N3 3(3) . . . . ?
Cu4 N10 C3 N3 178.1(15) . . . . ?
N6 N5 C4 N7 -6(3) . . . . ?
Cu2 N5 C4 N7 176.0(17) . . . . ?
C5 N7 C4 N5 6(3) . . . . ?
C4 N7 C5 N6 -3(3) . . . . ?
N5 N6 C5 N7 0(3) . . . . ?
Cu1 N6 C5 N7 -168.6(16) . . . . ?
N2 N1 C6 N9 3(3) . . . . ?
Cu3 N1 C6 N9 179.9(18) . . . . ?
C1 N9 C6 N1 -1(4) . . . . ?
C8 N8 C7 N11 0(3) . . . . ?
Cu4 N8 C7 N11 -178.8(17) . . . . ?
C7 N8 C8 N12 0(3) . . . . ?
Cu4 N8 C8 N12 179.0(18) . . . . ?
N8 C7 N11 N12 0(3) . . . . ?
N8 C7 N11 Cu2 169.4(16) . . . 1_655 ?
N8 C8 N12 N11 0(3) . . . . ?
N8 C8 N12 Cu3 178.4(18) . . . 1_655 ?
C7 N11 N12 C8 0(3) . . . . ?
Cu2 N11 N12 C8 -170.3(16) 1_655 . . . ?
C7 N11 N12 Cu3 -178.3(17) . . . 1_655 ?
Cu2 N11 N12 Cu3 11(3) 1_655 . . 1_655 ?

_refine_diff_density_max         2.946
_refine_diff_density_min         -5.367
_refine_diff_density_rms         0.443

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_5
_audit_block_doi                 10.5517/cc13896w
_database_code_depnum_ccdc_archive 'CCDC 1020867'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C28 H118 Co11 K2 N42 Na2 O169 P4 W36'
_chemical_formula_sum            'C28 H118 Co11 K2 N42 Na2 O169 P4 W36'
_chemical_formula_weight         11261.99

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   19.1440(5)
_cell_length_b                   23.3880(5)
_cell_length_c                   22.8600(5)
_cell_angle_alpha                90
_cell_angle_beta                 102.838(5)
_cell_angle_gamma                90
_cell_volume                     9979.5(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.8
_cell_measurement_theta_max      25.00

_exptl_crystal_description       needle-like
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    3.631
_exptl_crystal_F_000             9594
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.300
_exptl_crystal_size_mid          0.260
_exptl_crystal_size_min          0.260
_exptl_absorpt_coefficient_mu    21.720
_shelx_estimated_absorpt_T_min   0.059
_shelx_estimated_absorpt_T_max   0.071
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.002
_exptl_absorpt_correction_T_max  0.004
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            50922
_diffrn_reflns_av_unetI/netI     0.0719
_diffrn_reflns_av_R_equivalents  0.0646
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_theta_min         1.796
_diffrn_reflns_theta_max         24.978
_diffrn_reflns_theta_full        24.978
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measured_fraction_theta_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_point_group_measured_fraction_full 0.992
_reflns_number_total             17384
_reflns_number_gt                12958
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
The restraint commands 'DELU', and 'SIMU' were refined the atoms  w17 and o55, 
and the restraint command 'ISOR' was used to refine C3, C6, C7, N3, N4, N5, N10,
 N15, N18, O39, O47, N6, O52, O57, n14, c14, c8, n12,O4, O7, O11, O17, O19, O23,
  O25, O28, O29, O50, O58, o9w, o11w, P2, NA1, K1A, K1B and O26 atoms.
 The restraint order 'SIMU' was refined the atoms n12, c12, c13, co3, n20, n21,
 O11W, K1A and K1B. The restraint command 'DFIX' was used to refine O1W and co2, w18 and o60
 o2w and o4w, CO6 and O12W, W15 and O35, W14 and O35, O59 and W2.
 The restraint command 'DANG' was used to refineN9 and N5, N15 and N9.
 The 'OMIT' order was used to confirm the data completeless.
 Due to high levels of disorder about the solvent, we removed the 
 electronic contribution of the unidentified solvent with SQUEEZE.
In this P21/n space group with Z = 2 this implies that the (745/4 x 2) = 372.5
 removed electrons would be associated with the disordered water 
of the formula unit and thus implies that the contributions of 372.5/10 = 37
 additional water molecules should be associated with the Formula unit.  
 When the electron density, TGA, and elemental analysis are taken into account,
 29 water molecules are determined.
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.000 0.006 597 262 ' '
2 0.073 0.017 0.267 9 2 ' '
3 0.217 0.904 0.425 101 56 ' '
4 0.283 0.404 0.074 101 51 ' '
5 0.500 0.500 0.551 597 256 ' '
6 0.427 0.517 0.233 8 1 ' '
7 0.573 0.483 0.767 9 4 ' '
8 0.717 0.596 0.925 101 57 ' '
9 0.783 0.096 0.574 101 53 ' '
10 0.927 0.983 0.733 8 3 ' '
_platon_squeeze_details          
;
;

_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0509P)²+970.1205P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   mixed
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         17384
_refine_ls_number_parameters     1248
_refine_ls_number_restraints     2089
_refine_ls_R_factor_all          0.0955
_refine_ls_R_factor_gt           0.0681
_refine_ls_wR_factor_ref         0.1700
_refine_ls_wR_factor_gt          0.1558
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_restrained_S_all      1.037
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.6079(14) 0.8745(13) 0.4239(14) 0.040(8) Uani 1 1 d . . . . .
H1A H 0.6121 0.8386 0.4074 0.049 Uiso 1 1 calc R U . . .
C2 C 0.6310(16) 0.9589(14) 0.4610(13) 0.043(8) Uani 1 1 d . . . . .
H2A H 0.6553 0.9922 0.4753 0.052 Uiso 1 1 calc R U . . .
C3 C 0.4366(13) 0.8469(11) 0.5641(11) 0.026(6) Uani 1 1 d . U . . .
H3A H 0.4241 0.8084 0.5607 0.031 Uiso 1 1 calc R U . . .
C4 C 0.4610(13) 0.9276(11) 0.6002(11) 0.023(5) Uani 1 1 d . . . . .
H4 H 0.4696 0.9569 0.6284 0.028 Uiso 1 1 calc R U . . .
C5 C 0.6477(15) 1.1986(11) 0.1455(12) 0.031(6) Uani 1 1 d . . . . .
H5A H 0.6526 1.1893 0.1071 0.037 Uiso 1 1 calc R U . . .
C6 C 0.6442(14) 1.2450(11) 0.2254(12) 0.029(6) Uani 1 1 d . U . . .
H6A H 0.6474 1.2744 0.2533 0.035 Uiso 1 1 calc R U . . .
C7 C 0.4308(18) 1.1095(14) 0.2642(15) 0.050(8) Uani 1 1 d . U . . .
H7A H 0.4139 1.1273 0.2947 0.059 Uiso 1 1 calc R U . . .
C8 C 0.4351(17) 1.0644(13) 0.1879(14) 0.044(7) Uani 1 1 d . U . . .
H8A H 0.4222 1.0422 0.1535 0.053 Uiso 1 1 calc R U . . .
C9 C 0.3836(17) 1.0231(13) 0.3817(14) 0.043(8) Uani 1 1 d . . . . .
H9A H 0.3823 1.0625 0.3866 0.052 Uiso 1 1 calc R U . . .
C10 C 0.6869(12) 1.0552(9) 0.3493(8) 0.067(12) Uani 1 1 d G . . . .
H10A H 0.6983 1.0669 0.3892 0.081 Uiso 1 1 calc R U . . .
C11 C 0.3638(19) 0.9426(12) 0.3430(15) 0.053(9) Uani 1 1 d . . . . .
H11 H 0.3473 0.9131 0.3162 0.064 Uiso 1 1 calc R U . . .
C12 C 0.484(3) 1.256(2) 0.256(2) 0.102(7) Uani 1 1 d . U . . .
H12 H 0.4569 1.2323 0.2278 0.122 Uiso 1 1 calc R U . . .
C13 C 0.547(3) 1.283(2) 0.342(2) 0.102(7) Uani 1 1 d . U . . .
H13 H 0.5753 1.2824 0.3809 0.122 Uiso 1 1 calc R U . . .
C14 C 0.682(2) 1.0097(19) 0.2676(19) 0.077(12) Uani 1 1 d . U . . .
H14A H 0.6922 0.9834 0.2402 0.093 Uiso 1 1 calc R U . . .
N1 N 0.5508(11) 0.8919(9) 0.4437(9) 0.027(5) Uani 1 1 d . . . . .
N2 N 0.4962(11) 1.1202(10) 0.2519(9) 0.031(5) Uani 1 1 d . . . . .
N3 N 0.4956(11) 1.0919(9) 0.2002(9) 0.025(5) Uani 1 1 d . U . . .
N4 N 0.6195(11) 1.1945(8) 0.2322(9) 0.024(5) Uani 1 1 d . U . . .
N5 N 0.4493(11) 0.8792(8) 0.5210(8) 0.023(5) Uani 1 1 d D U . . .
N6 N 0.6450(11) 1.0540(7) 0.2533(7) 0.024(5) Uani 1 1 d G U . . .
N7 N 0.6502(10) 1.0854(6) 0.3030(6) 0.023(5) Uani 1 1 d G . . . .
N8 N 0.6587(11) 0.9154(11) 0.4308(11) 0.041(6) Uani 1 1 d . . . . .
N9 N 0.4441(11) 0.8765(10) 0.6108(8) 0.031(5) Uani 1 1 d D . . . .
N10 N 0.5663(10) 0.9463(9) 0.4663(9) 0.024(5) Uani 1 1 d . U . . .
N11 N 0.4051(12) 0.9342(11) 0.3978(10) 0.037(6) Uani 1 1 d . . . . .
N12 N 0.529(2) 1.2365(16) 0.3085(18) 0.090(7) Uani 1 1 d . U . . .
N13 N 0.3494(13) 0.9949(12) 0.3314(15) 0.064(9) Uani 1 1 d . . . . .
N14 N 0.7044(14) 1.0051(10) 0.3283(10) 0.064(8) Uani 1 1 d G U . . .
N15 N 0.4643(11) 0.9328(9) 0.5451(8) 0.025(5) Uani 1 1 d D U . . .
N16 N 0.6220(10) 1.1625(9) 0.1825(9) 0.025(5) Uani 1 1 d . . . . .
N17 N 0.4197(12) 0.9865(9) 0.4236(9) 0.028(5) Uani 1 1 d . . . . .
N18 N 0.6650(12) 1.2497(10) 0.1722(10) 0.035(5) Uani 1 1 d . U . . .
N19 N 0.3928(18) 1.0691(17) 0.2258(15) 0.080(11) Uani 1 1 d . . . . .
N20 N 0.482(2) 1.3172(18) 0.2506(16) 0.110(7) Uani 1 1 d D U . . .
N21 N 0.516(2) 1.3348(18) 0.3089(16) 0.111(7) Uani 1 1 d D U . . .
O1 O 0.7008(9) 0.8304(8) -0.0687(8) 0.032(3) Uani 1 1 d . U . . .
O2 O 0.7424(9) 0.7601(7) 0.0313(7) 0.025(2) Uani 1 1 d . U . . .
O1W O 0.4825(12) 0.7841(7) 0.4523(10) 0.061(4) Uani 1 1 d D U . . .
H1WC H 0.5227 0.7839 0.4774 0.074 Uiso 1 1 d R U . . .
O3 O 0.7236(9) 0.8704(7) 0.0503(7) 0.028(2) Uani 1 1 d . U . . .
O2W O 0.3449(12) 0.8211(8) 0.4180(10) 0.053(4) Uani 1 1 d D U . . .
O4 O 0.7888(9) 0.9223(8) 0.1581(8) 0.031(3) Uani 1 1 d . U . . .
O3W O 0.6775(10) 1.0577(9) 0.1302(9) 0.041(4) Uani 1 1 d . U . . .
O5 O 0.7838(9) 0.8042(7) 0.1411(7) 0.027(2) Uani 1 1 d . U . . .
O4W O 0.3208(12) 0.7038(8) 0.3702(9) 0.053(3) Uani 1 1 d D U . . .
O6 O 0.7196(9) 0.7170(7) 0.1839(7) 0.0262(18) Uani 1 1 d . U . . .
O5W O 0.2490(14) 1.0598(12) 0.1497(11) 0.074(6) Uani 1 1 d . U . . .
O7 O 0.7003(9) 0.8482(7) 0.2063(7) 0.0276(18) Uani 1 1 d . U . . .
O6W O 0.6329(10) 1.0001(8) 0.0104(8) 0.038(3) Uani 1 1 d . U . . .
O8 O 0.6810(9) 0.6745(7) 0.0777(7) 0.0268(19) Uani 1 1 d . U . . .
O7W O 0.2106(14) 0.9727(12) 0.2398(12) 0.075(5) Uani 1 1 d . U . . .
O9 O 0.6497(9) 0.7936(7) 0.0911(7) 0.0236(18) Uani 1 1 d . U . . .
O8W O 0.8197(15) 0.9134(12) 0.3346(13) 0.082(6) Uani 1 1 d . U . . .
O10 O 0.6372(9) 0.9110(7) 0.1176(7) 0.0259(17) Uani 1 1 d . U . . .
O9W O 0.621(2) 1.2958(18) 0.4861(19) 0.136(14) Uani 1 1 d . U . . .
O11 O 0.5907(9) 0.8609(7) -0.0115(7) 0.0251(19) Uani 1 1 d . U . . .
O10W O 0.4868(18) 1.0325(15) 0.7034(15) 0.105(10) Uani 1 1 d . U . . .
O12 O 0.6078(9) 0.7517(7) -0.0304(7) 0.0265(19) Uani 1 1 d . U . . .
O11W O 1.0132(13) 0.9062(11) 0.1291(12) 0.062(4) Uani 1 1 d . U . . .
O13 O 0.5009(9) 0.7012(8) -0.1125(8) 0.030(3) Uani 1 1 d . U . . .
O12W O 0.7895(15) 0.9640(12) 0.4385(11) 0.104(8) Uani 1 1 d D U . . .
H12C H 0.8159 0.9928 0.4361 0.125 Uiso 1 1 d R U . . .
H12D H 0.8115 0.9423 0.4664 0.125 Uiso 1 1 d R U . . .
O14 O 0.5637(9) 0.6469(7) -0.0060(7) 0.028(2) Uani 1 1 d . U . . .
O13W O 0.6306(11) 0.7292(9) 0.3972(9) 0.049(3) Uani 1 1 d . U . . .
O15 O 0.6268(11) 0.5637(8) 0.0758(9) 0.040(4) Uani 1 1 d . U . . .
O14W O 0.2200(11) 0.6727(10) 0.3373(10) 0.054(3) Uiso 1 1 d . U . . .
H14D H 0.2271 0.6837 0.3037 0.064 Uiso 1 1 d R U . . .
H14E H 0.2297 0.6373 0.3412 0.064 Uiso 1 1 d R U . . .
O16 O 0.6129(9) 0.6465(8) 0.1617(8) 0.0292(19) Uani 1 1 d . U . . .
O17 O 0.7045(10) 0.6432(8) 0.2746(8) 0.033(4) Uani 1 1 d . U . . .
O18 O 0.6721(9) 0.7604(8) 0.2769(8) 0.029(2) Uani 1 1 d . U . . .
O19 O 0.5844(9) 0.7674(7) 0.1723(7) 0.0241(17) Uani 1 1 d . U . . .
O20 O 0.5456(9) 0.7267(7) 0.0688(7) 0.0251(18) Uani 1 1 d . U . . .
O21 O 0.4790(9) 0.7907(7) -0.0349(7) 0.0259(18) Uani 1 1 d . U . . .
O22 O 0.4652(9) 0.9027(7) -0.0800(7) 0.025(3) Uani 1 1 d . U . . .
O23 O 0.5129(9) 0.9319(7) 0.0412(7) 0.0264(19) Uani 1 1 d . U . . .
O24 O 0.5273(9) 0.8307(7) 0.0855(7) 0.0231(18) Uani 1 1 d . U . . .
O25 O 0.5519(9) 0.9934(7) 0.1472(8) 0.030(2) Uani 1 1 d . U . . .
O26 O 0.5709(9) 0.8853(7) 0.2003(7) 0.0252(18) Uani 1 1 d . U . . .
O27 O 0.5663(10) 0.6806(8) 0.2570(8) 0.031(2) Uani 1 1 d . U . . .
O28 O 0.5454(9) 0.8076(8) 0.2746(8) 0.0301(18) Uani 1 1 d . U . . .
O29 O 0.4273(9) 0.6888(8) -0.0242(7) 0.028(2) Uani 1 1 d . U . . .
O30 O 0.3976(9) 0.8659(7) 0.0070(7) 0.027(2) Uani 1 1 d . U . . .
O31 O 0.4997(10) 0.6129(8) 0.0809(8) 0.031(2) Uani 1 1 d . U . . .
O32 O 0.4447(9) 0.9153(8) 0.1306(7) 0.0288(19) Uani 1 1 d . U . . .
O33 O 0.2849(10) 0.6652(9) -0.0777(8) 0.040(4) Uani 1 1 d . U . . .
O34 O 0.2529(10) 0.8663(9) -0.0434(9) 0.041(4) Uani 1 1 d . U . . .
O35 O 0.3569(9) 0.6132(6) 0.0295(6) 0.034(2) Uani 1 1 d D U . . .
O36 O 0.4150(12) 0.5259(9) 0.1094(9) 0.048(4) Uani 1 1 d . U . . .
O37 O 0.4644(10) 0.6207(8) 0.1863(8) 0.035(2) Uani 1 1 d . U . . .
O38 O 0.4901(12) 0.6037(9) 0.3100(9) 0.047(4) Uani 1 1 d . U . . .
O39 O 0.4667(10) 0.7236(8) 0.3110(8) 0.0366(19) Uani 1 1 d . U . . .
O40 O 0.4234(9) 0.8588(8) 0.2246(8) 0.0312(19) Uani 1 1 d . U . . .
O41 O 0.3075(9) 0.8989(8) 0.0774(8) 0.033(2) Uani 1 1 d . U . . .
O42 O 0.3775(9) 0.8061(8) 0.1113(8) 0.0300(18) Uani 1 1 d . U . . .
O43 O 0.4377(9) 0.7417(8) 0.1965(8) 0.0309(18) Uani 1 1 d . U . . .
O44 O 0.3967(9) 0.7003(8) 0.0935(8) 0.0302(19) Uani 1 1 d . U . . .
O45 O 0.4544(10) 0.8324(8) 0.3468(8) 0.035(3) Uani 1 1 d . U . . .
O46 O 0.3679(11) 0.6525(9) 0.2457(8) 0.041(2) Uani 1 1 d . U . . .
O47 O 0.3486(10) 0.7828(9) 0.2667(8) 0.0378(18) Uani 1 1 d . U . . .
O48 O 0.3248(10) 0.6098(9) 0.1378(8) 0.040(2) Uani 1 1 d . U . . .
O49 O 0.3061(10) 0.7300(8) 0.1511(8) 0.0366(19) Uani 1 1 d . U . . .
O50 O 0.2330(10) 0.7976(8) 0.0487(8) 0.037(2) Uani 1 1 d . U . . .
O51 O 0.2520(10) 0.6891(9) 0.0307(8) 0.037(2) Uani 1 1 d . U . . .
O52 O 0.2852(10) 0.8494(9) 0.1798(8) 0.037(2) Uani 1 1 d . U . . .
O53 O 0.1977(11) 0.6630(9) 0.1260(9) 0.044(2) Uani 1 1 d . U . . .
O54 O 0.1792(10) 0.7735(9) 0.1448(8) 0.042(2) Uani 1 1 d . U . . .
O55 O 0.2419(11) 0.7064(10) 0.2355(9) 0.0480(19) Uani 1 1 d . U . . .
O56 O 0.2060(11) 0.8206(10) 0.2611(10) 0.054(4) Uani 1 1 d . U . . .
O57 O 0.2414(11) 0.5879(9) 0.2222(9) 0.047(3) Uani 1 1 d . U . . .
O58 O 0.6678(9) 0.8735(8) 0.3132(8) 0.029(3) Uani 1 1 d . U . . .
O59 O 0.8273(8) 0.6963(7) 0.1259(7) 0.028(3) Uani 1 1 d D U . . .
O60 O 0.1171(8) 0.7271(10) 0.0359(8) 0.050(4) Uani 1 1 d D U . . .
O61 O 0.3293(9) 0.7652(8) -0.0108(8) 0.031(2) Uani 1 1 d . U . . .
O62 O 0.3404(10) 0.9575(9) 0.1876(8) 0.038(3) Uani 1 1 d . U . . .
P1 P 0.5744(3) 0.7788(2) 0.1050(2) 0.0088(11) Uani 1 1 d . . . . .
P2 P 0.3833(3) 0.7452(2) 0.1372(2) 0.0143(12) Uani 1 1 d . U . . .
Co1 Co 0.58778(16) 1.07825(13) 0.16831(13) 0.0166(7) Uani 1 1 d . . . . .
Co2 Co 0.44821(17) 0.85685(13) 0.43237(13) 0.0177(7) Uani 1 1 d D . . . .
Co3 Co 0.58425(17) 1.15762(14) 0.30847(13) 0.0197(7) Uani 1 1 d . . . . .
Co4 Co 0.5000 1.0000 0.5000 0.0164(9) Uani 1 2 d S . P . .
Co5 Co 0.3035(2) 1.0243(2) 0.2380(2) 0.0524(12) Uani 1 1 d . . . . .
Co6 Co 0.7371(3) 0.9249(2) 0.3792(2) 0.0653(14) Uani 1 1 d D U . . .
W1 W 0.66970(5) 0.81376(5) -0.00553(4) 0.0241(2) Uani 1 1 d . . . . .
W2 W 0.74784(5) 0.73007(5) 0.11233(4) 0.0233(2) Uani 1 1 d D . . . .
W3 W 0.72457(5) 0.87134(4) 0.13315(4) 0.0228(2) Uani 1 1 d . . . . .
W4 W 0.65106(6) 0.69138(4) 0.22993(5) 0.0249(2) Uani 1 1 d . . . . .
W5 W 0.62917(5) 0.83144(4) 0.25152(4) 0.0184(2) Uani 1 1 d . . . . .
W6 W 0.53977(5) 0.92355(4) 0.12642(4) 0.0192(2) Uani 1 1 d . . . . .
W7 W 0.48727(5) 0.86861(4) -0.01156(4) 0.0185(2) Uani 1 1 d . . . . .
W8 W 0.51375(5) 0.71545(4) -0.03732(4) 0.0231(2) Uani 1 1 d . . . . .
W9 W 0.59262(6) 0.63183(4) 0.07858(5) 0.0285(3) Uani 1 1 d . . . . .
W10 W 0.47053(7) 0.65816(5) 0.25901(5) 0.0369(3) Uani 1 1 d . . . . .
W11 W 0.44764(5) 0.79749(5) 0.28018(4) 0.0255(2) Uani 1 1 d . . . . .
W12 W 0.35919(6) 0.89259(5) 0.15792(5) 0.0324(3) Uani 1 1 d . . . . .
W13 W 0.30712(6) 0.83779(6) 0.02047(5) 0.0389(3) Uani 1 1 d . . . . .
W14 W 0.33207(6) 0.68534(5) -0.00686(5) 0.0299(3) Uani 1 1 d D . . . .
W15 W 0.41234(8) 0.60056(5) 0.10803(6) 0.0441(3) Uani 1 1 d D . . . .
W16 W 0.27682(7) 0.64466(6) 0.19263(5) 0.0443(4) Uani 1 1 d . . . . .
W17 W 0.25247(6) 0.78668(7) 0.21601(5) 0.0474(4) Uani 1 1 d . U . . .
W18 W 0.19730(6) 0.72982(7) 0.07736(5) 0.0434(3) Uani 1 1 d D . . . .
Na1 Na 0.5434(7) 0.6314(5) -0.1755(5) 0.049(3) Uani 1 1 d . U . . .
K1A K 1.0022(8) 0.9169(6) 0.1637(7) 0.046(3) Uani 0.5 1 d . U P . .
K1B K 0.9193(8) 0.9214(7) 0.1867(7) 0.054(3) Uani 0.5 1 d . U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N1 1.34(3) . ?
C1 N8 1.35(4) . ?
C1 H1A 0.9300 . ?
C2 N10 1.30(3) . ?
C2 N8 1.40(4) . ?
C2 H2A 0.9300 . ?
C3 N9 1.25(3) . ?
C3 N5 1.31(3) . ?
C3 H3A 0.9300 . ?
C4 N9 1.27(3) . ?
C4 N15 1.28(3) . ?
C4 H4 0.9300 . ?
C5 N18 1.35(3) . ?
C5 N16 1.36(3) . ?
C5 H5A 0.9300 . ?
C6 N4 1.30(3) . ?
C6 N18 1.37(3) . ?
C6 H6A 0.9300 . ?
C7 N2 1.37(4) . ?
C7 N19 1.38(4) . ?
C7 H7A 0.9300 . ?
C8 N3 1.30(4) . ?
C8 N19 1.32(4) . ?
C8 H8A 0.9300 . ?
C9 N17 1.35(3) . ?
C9 N13 1.36(4) . ?
C9 H9A 0.9300 . ?
C10 N14 1.336(15) . ?
C10 N7 1.336(15) . ?
C10 H10A 0.9300 . ?
C11 N13 1.27(4) . ?
C11 N11 1.34(4) . ?
C11 H11 0.9300 . ?
C12 N12 1.39(6) . ?
C12 N20 1.43(6) . ?
C12 H12 0.9300 . ?
C13 N12 1.32(5) . ?
C13 N21 1.49(6) . ?
C13 K1A 3.28(5) 2_655 ?
C13 K1B 3.40(5) 2_655 ?
C13 H13 0.9300 . ?
C14 N6 1.26(4) . ?
C14 N14 1.36(4) . ?
C14 H14A 0.9300 . ?
N1 N10 1.38(3) . ?
N1 Co2 2.09(2) . ?
N2 N3 1.35(3) . ?
N2 Co3 2.08(2) . ?
N3 Co1 2.08(2) . ?
N4 N16 1.37(3) . ?
N4 Co3 2.18(2) . ?
N5 N15 1.37(3) . ?
N5 Co2 2.088(18) . ?
N6 N7 1.337(15) . ?
N6 Co1 2.086(16) . ?
N7 Co3 2.128(15) . ?
N8 Co6 2.12(2) . ?
N9 Co3 2.188(18) 3_676 ?
N10 Co4 2.052(19) . ?
N11 N17 1.36(3) . ?
N11 Co2 2.07(2) . ?
N12 Co3 2.12(4) . ?
N13 Co5 2.23(3) . ?
N14 Co6 2.22(2) . ?
N15 Co4 2.077(18) . ?
N16 Co1 2.08(2) . ?
N17 Co4 2.08(2) . ?
N19 Co5 2.08(3) . ?
N20 N21 1.403(10) . ?
N20 Na1 2.06(4) 3_675 ?
N20 K1A 3.02(4) 2_655 ?
N20 K1B 3.21(4) 2_655 ?
N21 K1A 2.07(4) 2_655 ?
N21 K1B 2.37(5) 2_655 ?
O1 W1 1.724(16) . ?
O2 W1 1.924(17) . ?
O2 W2 1.963(16) . ?
O1W Co2 1.844(16) . ?
O1W H1WC 0.8499 . ?
O3 W3 1.891(17) . ?
O3 W1 1.964(17) . ?
O2W Co2 2.11(2) . ?
O4 W3 1.716(17) . ?
O4 K1B 2.44(2) . ?
O3W Co1 2.145(19) . ?
O5 W3 1.922(17) . ?
O5 W2 1.926(17) . ?
O6 W2 1.859(16) . ?
O6 W4 1.950(16) . ?
O5W Co5 2.22(3) . ?
O7 W3 1.911(16) . ?
O7 W5 1.924(17) . ?
O8 W2 1.872(17) . ?
O8 W9 1.967(17) . ?
O7W Co5 2.16(3) . ?
O9 P1 1.581(17) . ?
O9 W2 2.359(16) . ?
O9 W1 2.372(15) . ?
O9 W3 2.383(16) . ?
O8W Co6 2.08(3) . ?
O10 W3 1.876(17) . ?
O10 W6 1.943(16) . ?
O11 W1 1.851(16) . ?
O11 W7 1.988(16) . ?
O12 W1 1.881(17) . ?
O12 W8 1.963(17) . ?
O11W K1A 0.90(3) . ?
O11W K1B 2.48(3) . ?
O13 W8 1.714(17) . ?
O13 Na1 2.43(2) . ?
O12W Co6 1.754(18) . ?
O12W H12C 0.8501 . ?
O12W H12D 0.8499 . ?
O14 W9 1.921(17) . ?
O14 W8 1.923(17) . ?
O15 W9 1.728(19) . ?
O14W H14D 0.8500 . ?
O14W H14E 0.8499 . ?
O16 W9 1.885(17) . ?
O16 W4 1.887(17) . ?
O17 W4 1.701(18) . ?
O18 W5 1.888(18) . ?
O18 W4 1.931(17) . ?
O19 P1 1.530(17) . ?
O19 W5 2.360(16) . ?
O19 W4 2.403(17) . ?
O20 P1 1.507(17) . ?
O20 W8 2.381(16) . ?
O20 W9 2.386(17) . ?
O21 W8 1.887(17) . ?
O21 W7 1.896(17) . ?
O22 W7 1.723(16) . ?
O22 Co1 2.096(17) 3_675 ?
O23 W7 1.905(17) . ?
O23 W6 1.910(17) . ?
O24 P1 1.517(17) . ?
O24 W7 2.354(16) . ?
O24 W6 2.356(16) . ?
O25 W6 1.702(17) . ?
O25 Co1 2.120(18) . ?
O26 W6 1.887(17) . ?
O26 W5 1.902(17) . ?
O27 W4 1.876(17) . ?
O27 W10 1.918(17) . ?
O28 W5 1.881(17) . ?
O28 W11 1.918(17) . ?
O29 W8 1.855(17) . ?
O29 W14 1.951(17) . ?
O30 W7 1.858(16) . ?
O30 W13 1.940(17) . ?
O31 W9 1.846(18) . ?
O31 W15 1.930(17) . ?
O32 W6 1.853(17) . ?
O32 W12 1.951(17) . ?
O33 W14 1.735(18) . ?
O34 W13 1.73(2) . ?
O35 W15 1.894(13) . ?
O35 W14 1.895(13) . ?
O36 W15 1.75(2) . ?
O37 W10 1.860(18) . ?
O37 W15 1.903(18) . ?
O38 W10 1.71(2) . ?
O39 W11 1.87(2) . ?
O39 W10 1.948(19) . ?
O40 W12 1.904(18) . ?
O40 W11 1.904(19) . ?
O41 W12 1.892(18) . ?
O41 W13 1.931(17) . ?
O42 P2 1.539(19) . ?
O42 W13 2.331(18) . ?
O42 W12 2.348(17) . ?
O43 P2 1.516(19) . ?
O43 W11 2.289(17) . ?
O43 W10 2.419(18) . ?
O44 P2 1.508(18) . ?
O44 W15 2.366(18) . ?
O44 W14 2.379(17) . ?
O45 W11 1.707(17) . ?
O45 Co2 2.067(18) . ?
O46 W16 1.90(2) . ?
O46 W10 1.92(2) . ?
O47 W11 1.884(19) . ?
O47 W17 1.946(19) . ?
O48 W16 1.896(19) . ?
O48 W15 1.955(19) . ?
O49 P2 1.619(18) . ?
O49 W16 2.332(19) . ?
O49 W18 2.371(19) . ?
O49 W17 2.385(18) . ?
O50 W18 1.90(2) . ?
O50 W13 1.930(19) . ?
O51 W18 1.907(18) . ?
O51 W14 1.918(18) . ?
O52 W17 1.86(2) . ?
O52 W12 1.895(19) . ?
O53 W18 1.92(2) . ?
O53 W16 1.94(2) . ?
O54 W17 1.923(19) . ?
O54 W18 1.943(19) . ?
O55 W16 1.94(2) . ?
O55 W17 1.95(2) . ?
O56 W17 1.70(2) . ?
O57 W16 1.70(2) . ?
O57 Co5 2.03(2) 2_545 ?
O58 W5 1.744(17) . ?
O58 Co6 2.142(18) . ?
O59 W2 1.680(13) . ?
O59 Co3 2.194(15) 2_645 ?
O60 W18 1.616(15) . ?
O61 W14 1.869(19) . ?
O61 W13 1.926(18) . ?
O62 W12 1.733(19) . ?
O62 Co5 2.152(19) . ?
Co1 O22 2.096(17) 3_675 ?
Co3 N9 2.188(18) 3_676 ?
Co3 O59 2.193(15) 2_655 ?
Co4 N10 2.052(19) 3_676 ?
Co4 N15 2.077(18) 3_676 ?
Co4 N17 2.08(2) 3_676 ?
Co5 O57 2.03(2) 2 ?
W3 K1B 3.839(16) . ?
Na1 N20 2.06(4) 3_675 ?
Na1 K1B 3.71(2) 4_575 ?
Na1 K1A 3.76(2) 4_575 ?
K1A K1B 1.78(2) . ?
K1A N21 2.07(4) 2_645 ?
K1A N20 3.02(4) 2_645 ?
K1A C13 3.28(5) 2_645 ?
K1A Na1 3.76(2) 4_676 ?
K1B N21 2.37(5) 2_645 ?
K1B N20 3.21(4) 2_645 ?
K1B C13 3.40(5) 2_645 ?
K1B Na1 3.71(2) 4_676 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 C1 N8 111(2) . . ?
N1 C1 H1A 124.3 . . ?
N8 C1 H1A 124.3 . . ?
N10 C2 N8 111(3) . . ?
N10 C2 H2A 124.6 . . ?
N8 C2 H2A 124.6 . . ?
N9 C3 N5 108(2) . . ?
N9 C3 H3A 125.8 . . ?
N5 C3 H3A 125.8 . . ?
N9 C4 N15 110(2) . . ?
N9 C4 H4 124.9 . . ?
N15 C4 H4 124.9 . . ?
N18 C5 N16 111(2) . . ?
N18 C5 H5A 124.6 . . ?
N16 C5 H5A 124.6 . . ?
N4 C6 N18 111(2) . . ?
N4 C6 H6A 124.3 . . ?
N18 C6 H6A 124.3 . . ?
N2 C7 N19 112(3) . . ?
N2 C7 H7A 124.1 . . ?
N19 C7 H7A 124.1 . . ?
N3 C8 N19 118(3) . . ?
N3 C8 H8A 121.1 . . ?
N19 C8 H8A 121.1 . . ?
N17 C9 N13 111(3) . . ?
N17 C9 H9A 124.3 . . ?
N13 C9 H9A 124.3 . . ?
N14 C10 N7 108.0 . . ?
N14 C10 H10A 126.0 . . ?
N7 C10 H10A 126.0 . . ?
N13 C11 N11 113(3) . . ?
N13 C11 H11 123.4 . . ?
N11 C11 H11 123.4 . . ?
N12 C12 N20 114(4) . . ?
N12 C12 H12 122.9 . . ?
N20 C12 H12 122.9 . . ?
N12 C13 N21 110(4) . . ?
N12 C13 K1A 136(3) . 2_655 ?
N21 C13 K1A 27.6(18) . 2_655 ?
N12 C13 K1B 134(4) . 2_655 ?
N21 C13 K1B 36(2) . 2_655 ?
K1A C13 K1B 30.9(6) 2_655 2_655 ?
N12 C13 H13 124.8 . . ?
N21 C13 H13 124.8 . . ?
K1A C13 H13 98.2 2_655 . ?
K1B C13 H13 95.4 2_655 . ?
N6 C14 N14 111(4) . . ?
N6 C14 H14A 124.4 . . ?
N14 C14 H14A 124.4 . . ?
C1 N1 N10 107(2) . . ?
C1 N1 Co2 130.9(18) . . ?
N10 N1 Co2 121.7(15) . . ?
N3 N2 C7 105(2) . . ?
N3 N2 Co3 126.9(16) . . ?
C7 N2 Co3 127.1(19) . . ?
C8 N3 N2 105(2) . . ?
C8 N3 Co1 129.2(19) . . ?
N2 N3 Co1 122.5(15) . . ?
C6 N4 N16 108(2) . . ?
C6 N4 Co3 129.9(17) . . ?
N16 N4 Co3 121.5(15) . . ?
C3 N5 N15 106.4(18) . . ?
C3 N5 Co2 128.5(17) . . ?
N15 N5 Co2 125.1(14) . . ?
C14 N6 N7 108(2) . . ?
C14 N6 Co1 128(2) . . ?
N7 N6 Co1 124.5(10) . . ?
C10 N7 N6 108.0 . . ?
C10 N7 Co3 126.0(9) . . ?
N6 N7 Co3 123.6(10) . . ?
C1 N8 C2 103(2) . . ?
C1 N8 Co6 126.2(18) . . ?
C2 N8 Co6 126(2) . . ?
C3 N9 C4 110(2) . . ?
C3 N9 Co3 120.8(18) . 3_676 ?
C4 N9 Co3 128.6(16) . 3_676 ?
C2 N10 N1 107(2) . . ?
C2 N10 Co4 125.2(19) . . ?
N1 N10 Co4 127.2(15) . . ?
C11 N11 N17 107(2) . . ?
C11 N11 Co2 126(2) . . ?
N17 N11 Co2 126.5(17) . . ?
C13 N12 C12 105(4) . . ?
C13 N12 Co3 130(3) . . ?
C12 N12 Co3 120(3) . . ?
C11 N13 C9 104(3) . . ?
C11 N13 Co5 121(3) . . ?
C9 N13 Co5 132(2) . . ?
C10 N14 C14 104(2) . . ?
C10 N14 Co6 128.0(12) . . ?
C14 N14 Co6 126(2) . . ?
C4 N15 N5 104.9(19) . . ?
C4 N15 Co4 130.8(18) . . ?
N5 N15 Co4 123.6(14) . . ?
C5 N16 N4 105(2) . . ?
C5 N16 Co1 129.5(17) . . ?
N4 N16 Co1 125.3(15) . . ?
C9 N17 N11 104(2) . . ?
C9 N17 Co4 131.7(19) . . ?
N11 N17 Co4 122.8(17) . . ?
C5 N18 C6 104(2) . . ?
C8 N19 C7 99(3) . . ?
C8 N19 Co5 134(3) . . ?
C7 N19 Co5 126(2) . . ?
N21 N20 C12 102(4) . . ?
N21 N20 Na1 126(3) . 3_675 ?
C12 N20 Na1 131(3) . 3_675 ?
N21 N20 K1A 37(2) . 2_655 ?
C12 N20 K1A 135(3) . 2_655 ?
Na1 N20 K1A 93.5(15) 3_675 2_655 ?
N21 N20 K1B 42(2) . 2_655 ?
C12 N20 K1B 136(3) . 2_655 ?
Na1 N20 K1B 86.4(15) 3_675 2_655 ?
K1A N20 K1B 33.0(6) 2_655 2_655 ?
N20 N21 C13 107(4) . . ?
N20 N21 K1A 119(3) . 2_655 ?
C13 N21 K1A 133(3) . 2_655 ?
N20 N21 K1B 114(3) . 2_655 ?
C13 N21 K1B 122(3) . 2_655 ?
K1A N21 K1B 46.7(10) 2_655 2_655 ?
W1 O2 W2 121.8(8) . . ?
Co2 O1W H1WC 113.0 . . ?
W3 O3 W1 123.1(9) . . ?
W3 O4 K1B 134.3(10) . . ?
W3 O5 W2 123.0(9) . . ?
W2 O6 W4 152.6(10) . . ?
W3 O7 W5 150.0(10) . . ?
W2 O8 W9 148.9(9) . . ?
P1 O9 W2 122.8(9) . . ?
P1 O9 W1 125.0(9) . . ?
W2 O9 W1 91.8(5) . . ?
P1 O9 W3 125.4(9) . . ?
W2 O9 W3 91.0(6) . . ?
W1 O9 W3 90.9(5) . . ?
W3 O10 W6 153.1(10) . . ?
W1 O11 W7 148.4(10) . . ?
W1 O12 W8 149.6(9) . . ?
K1A O11W K1B 32.0(17) . . ?
W8 O13 Na1 137.0(10) . . ?
Co6 O12W H12C 127.5 . . ?
Co6 O12W H12D 111.8 . . ?
H12C O12W H12D 108.5 . . ?
W9 O14 W8 122.4(9) . . ?
H14D O14W H14E 108.4 . . ?
W9 O16 W4 152.8(10) . . ?
W5 O18 W4 122.8(9) . . ?
P1 O19 W5 127.1(9) . . ?
P1 O19 W4 127.8(9) . . ?
W5 O19 W4 89.5(6) . . ?
P1 O20 W8 128.9(10) . . ?
P1 O20 W9 128.1(10) . . ?
W8 O20 W9 89.9(5) . . ?
W8 O21 W7 153.7(10) . . ?
W7 O22 Co1 160.4(10) . 3_675 ?
W7 O23 W6 122.6(9) . . ?
P1 O24 W7 128.8(9) . . ?
P1 O24 W6 128.2(9) . . ?
W7 O24 W6 90.6(6) . . ?
W6 O25 Co1 168.2(11) . . ?
W6 O26 W5 152.9(9) . . ?
W4 O27 W10 161.1(10) . . ?
W5 O28 W11 163.8(11) . . ?
W8 O29 W14 162.6(10) . . ?
W7 O30 W13 161.9(10) . . ?
W9 O31 W15 162.7(10) . . ?
W6 O32 W12 161.5(10) . . ?
W15 O35 W14 126.0(9) . . ?
W10 O37 W15 150.8(11) . . ?
W11 O39 W10 121.8(9) . . ?
W12 O40 W11 149.9(10) . . ?
W12 O41 W13 121.4(10) . . ?
P2 O42 W13 128.0(10) . . ?
P2 O42 W12 129.0(9) . . ?
W13 O42 W12 90.9(6) . . ?
P2 O43 W11 129.0(11) . . ?
P2 O43 W10 127.5(10) . . ?
W11 O43 W10 90.2(6) . . ?
P2 O44 W15 128.9(10) . . ?
P2 O44 W14 127.8(11) . . ?
W15 O44 W14 90.7(6) . . ?
W11 O45 Co2 165.3(11) . . ?
W16 O46 W10 150.2(11) . . ?
W11 O47 W17 150.8(11) . . ?
W16 O48 W15 148.9(11) . . ?
P2 O49 W16 125.4(11) . . ?
P2 O49 W18 123.9(10) . . ?
W16 O49 W18 92.0(7) . . ?
P2 O49 W17 122.6(10) . . ?
W16 O49 W17 92.7(6) . . ?
W18 O49 W17 90.7(6) . . ?
W18 O50 W13 150.5(11) . . ?
W18 O51 W14 150.1(11) . . ?
W17 O52 W12 152.0(11) . . ?
W18 O53 W16 122.5(10) . . ?
W17 O54 W18 122.1(10) . . ?
W16 O55 W17 122.3(10) . . ?
W16 O57 Co5 175.5(13) . 2_545 ?
W5 O58 Co6 166.2(10) . . ?
W2 O59 Co3 148.2(9) . 2_645 ?
W14 O61 W13 150.4(10) . . ?
W12 O62 Co5 165.2(12) . . ?
O20 P1 O24 111.4(9) . . ?
O20 P1 O19 111.1(9) . . ?
O24 P1 O19 111.7(9) . . ?
O20 P1 O9 107.7(9) . . ?
O24 P1 O9 105.9(9) . . ?
O19 P1 O9 108.9(9) . . ?
O44 P2 O43 111.7(10) . . ?
O44 P2 O42 113.5(10) . . ?
O43 P2 O42 111.8(10) . . ?
O44 P2 O49 105.9(10) . . ?
O43 P2 O49 106.7(10) . . ?
O42 P2 O49 106.6(10) . . ?
N3 Co1 N16 93.6(8) . . ?
N3 Co1 N6 91.5(8) . . ?
N16 Co1 N6 91.7(7) . . ?
N3 Co1 O22 92.2(7) . 3_675 ?
N16 Co1 O22 91.0(7) . 3_675 ?
N6 Co1 O22 175.3(7) . 3_675 ?
N3 Co1 O25 88.1(7) . . ?
N16 Co1 O25 175.9(7) . . ?
N6 Co1 O25 92.0(7) . . ?
O22 Co1 O25 85.3(7) 3_675 . ?
N3 Co1 O3W 174.5(8) . . ?
N16 Co1 O3W 91.2(8) . . ?
N6 Co1 O3W 90.9(8) . . ?
O22 Co1 O3W 85.2(7) 3_675 . ?
O25 Co1 O3W 86.9(7) . . ?
O1W Co2 O45 83.5(9) . . ?
O1W Co2 N11 172.0(10) . . ?
O45 Co2 N11 89.0(8) . . ?
O1W Co2 N5 93.7(9) . . ?
O45 Co2 N5 175.9(8) . . ?
N11 Co2 N5 93.9(8) . . ?
O1W Co2 N1 93.3(10) . . ?
O45 Co2 N1 88.6(7) . . ?
N11 Co2 N1 89.4(9) . . ?
N5 Co2 N1 88.6(8) . . ?
O1W Co2 O2W 86.7(9) . . ?
O45 Co2 O2W 89.6(8) . . ?
N11 Co2 O2W 90.3(9) . . ?
N5 Co2 O2W 93.3(8) . . ?
N1 Co2 O2W 178.1(8) . . ?
N2 Co3 N12 91.9(13) . . ?
N2 Co3 N7 92.2(8) . . ?
N12 Co3 N7 171.6(12) . . ?
N2 Co3 N4 91.2(8) . . ?
N12 Co3 N4 84.1(12) . . ?
N7 Co3 N4 88.5(7) . . ?
N2 Co3 N9 93.0(8) . 3_676 ?
N12 Co3 N9 95.9(13) . 3_676 ?
N7 Co3 N9 91.3(8) . 3_676 ?
N4 Co3 N9 175.8(8) . 3_676 ?
N2 Co3 O59 175.4(7) . 2_655 ?
N12 Co3 O59 87.0(12) . 2_655 ?
N7 Co3 O59 89.4(6) . 2_655 ?
N4 Co3 O59 93.1(7) . 2_655 ?
N9 Co3 O59 82.7(7) 3_676 2_655 ?
N10 Co4 N10 180.0(8) . 3_676 ?
N10 Co4 N15 91.3(8) . . ?
N10 Co4 N15 88.7(8) 3_676 . ?
N10 Co4 N15 88.7(8) . 3_676 ?
N10 Co4 N15 91.3(8) 3_676 3_676 ?
N15 Co4 N15 180.0 . 3_676 ?
N10 Co4 N17 89.8(8) . . ?
N10 Co4 N17 90.2(8) 3_676 . ?
N15 Co4 N17 92.3(8) . . ?
N15 Co4 N17 87.7(8) 3_676 . ?
N10 Co4 N17 90.2(8) . 3_676 ?
N10 Co4 N17 89.8(8) 3_676 3_676 ?
N15 Co4 N17 87.7(8) . 3_676 ?
N15 Co4 N17 92.3(8) 3_676 3_676 ?
N17 Co4 N17 180.0(8) . 3_676 ?
O57 Co5 N19 97.7(12) 2 . ?
O57 Co5 O62 173.4(8) 2 . ?
N19 Co5 O62 85.2(11) . . ?
O57 Co5 O7W 88.2(10) 2 . ?
N19 Co5 O7W 172.7(12) . . ?
O62 Co5 O7W 88.5(9) . . ?
O57 Co5 O5W 88.4(9) 2 . ?
N19 Co5 O5W 85.6(13) . . ?
O62 Co5 O5W 85.9(9) . . ?
O7W Co5 O5W 90.2(10) . . ?
O57 Co5 N13 85.0(10) 2 . ?
N19 Co5 N13 97.1(12) . . ?
O62 Co5 N13 100.6(10) . . ?
O7W Co5 N13 87.7(10) . . ?
O5W Co5 N13 173.2(11) . . ?
O12W Co6 O8W 94.5(14) . . ?
O12W Co6 N8 88.8(13) . . ?
O8W Co6 N8 165.9(11) . . ?
O12W Co6 O58 174.3(12) . . ?
O8W Co6 O58 90.1(10) . . ?
N8 Co6 O58 85.9(8) . . ?
O12W Co6 N14 90.6(12) . . ?
O8W Co6 N14 90.4(10) . . ?
N8 Co6 N14 103.2(10) . . ?
O58 Co6 N14 92.7(8) . . ?
O1 W1 O11 103.4(8) . . ?
O1 W1 O12 103.5(8) . . ?
O11 W1 O12 89.3(7) . . ?
O1 W1 O2 99.4(8) . . ?
O11 W1 O2 157.0(7) . . ?
O12 W1 O2 88.6(7) . . ?
O1 W1 O3 99.3(8) . . ?
O11 W1 O3 87.1(7) . . ?
O12 W1 O3 157.1(7) . . ?
O2 W1 O3 86.1(7) . . ?
O1 W1 O9 169.2(7) . . ?
O11 W1 O9 83.6(6) . . ?
O12 W1 O9 84.6(6) . . ?
O2 W1 O9 73.4(6) . . ?
O3 W1 O9 72.5(6) . . ?
O59 W2 O6 100.9(8) . . ?
O59 W2 O8 105.0(8) . . ?
O6 W2 O8 87.3(7) . . ?
O59 W2 O5 96.8(8) . . ?
O6 W2 O5 90.0(7) . . ?
O8 W2 O5 158.2(7) . . ?
O59 W2 O2 101.4(7) . . ?
O6 W2 O2 157.7(7) . . ?
O8 W2 O2 87.8(7) . . ?
O5 W2 O2 86.6(7) . . ?
O59 W2 O9 168.7(7) . . ?
O6 W2 O9 84.9(6) . . ?
O8 W2 O9 84.9(7) . . ?
O5 W2 O9 73.3(6) . . ?
O2 W2 O9 73.0(6) . . ?
O4 W3 O10 105.2(8) . . ?
O4 W3 O3 100.9(8) . . ?
O10 W3 O3 90.4(7) . . ?
O4 W3 O7 101.6(8) . . ?
O10 W3 O7 85.7(7) . . ?
O3 W3 O7 157.5(7) . . ?
O4 W3 O5 99.9(8) . . ?
O10 W3 O5 154.7(7) . . ?
O3 W3 O5 87.7(7) . . ?
O7 W3 O5 86.5(7) . . ?
O4 W3 O9 170.7(7) . . ?
O10 W3 O9 82.5(6) . . ?
O3 W3 O9 73.5(6) . . ?
O7 W3 O9 84.0(6) . . ?
O5 W3 O9 72.8(6) . . ?
O4 W3 K1B 27.0(6) . . ?
O10 W3 K1B 132.1(6) . . ?
O3 W3 K1B 96.7(6) . . ?
O7 W3 K1B 102.4(6) . . ?
O5 W3 K1B 73.1(6) . . ?
O9 W3 K1B 144.7(5) . . ?
O17 W4 O27 99.3(8) . . ?
O17 W4 O16 101.5(8) . . ?
O27 W4 O16 89.6(7) . . ?
O17 W4 O18 101.3(8) . . ?
O27 W4 O18 91.0(7) . . ?
O16 W4 O18 156.8(8) . . ?
O17 W4 O6 98.0(8) . . ?
O27 W4 O6 162.5(7) . . ?
O16 W4 O6 84.7(7) . . ?
O18 W4 O6 87.8(7) . . ?
O17 W4 O19 173.7(7) . . ?
O27 W4 O19 83.6(7) . . ?
O16 W4 O19 84.1(7) . . ?
O18 W4 O19 73.0(6) . . ?
O6 W4 O19 79.4(6) . . ?
O58 W5 O28 100.1(8) . . ?
O58 W5 O18 99.8(8) . . ?
O28 W5 O18 89.6(8) . . ?
O58 W5 O26 102.1(8) . . ?
O28 W5 O26 87.1(7) . . ?
O18 W5 O26 158.1(7) . . ?
O58 W5 O7 95.5(8) . . ?
O28 W5 O7 163.9(7) . . ?
O18 W5 O7 91.9(7) . . ?
O26 W5 O7 85.5(7) . . ?
O58 W5 O19 174.5(7) . . ?
O28 W5 O19 80.8(6) . . ?
O18 W5 O19 74.7(7) . . ?
O26 W5 O19 83.4(6) . . ?
O7 W5 O19 84.1(6) . . ?
O25 W6 O32 99.3(8) . . ?
O25 W6 O26 102.1(8) . . ?
O32 W6 O26 91.3(7) . . ?
O25 W6 O23 100.1(8) . . ?
O32 W6 O23 91.1(7) . . ?
O26 W6 O23 157.0(7) . . ?
O25 W6 O10 95.7(8) . . ?
O32 W6 O10 165.0(7) . . ?
O26 W6 O10 84.3(7) . . ?
O23 W6 O10 87.6(7) . . ?
O25 W6 O24 172.2(7) . . ?
O32 W6 O24 84.9(7) . . ?
O26 W6 O24 84.4(6) . . ?
O23 W6 O24 73.1(6) . . ?
O10 W6 O24 80.5(6) . . ?
O22 W7 O30 99.8(8) . . ?
O22 W7 O21 101.5(7) . . ?
O30 W7 O21 90.4(7) . . ?
O22 W7 O23 101.1(8) . . ?
O30 W7 O23 90.2(7) . . ?
O21 W7 O23 156.9(7) . . ?
O22 W7 O11 94.9(7) . . ?
O30 W7 O11 165.2(7) . . ?
O21 W7 O11 86.2(7) . . ?
O23 W7 O11 87.4(7) . . ?
O22 W7 O24 173.3(7) . . ?
O30 W7 O24 84.0(6) . . ?
O21 W7 O24 83.9(6) . . ?
O23 W7 O24 73.3(6) . . ?
O11 W7 O24 81.3(6) . . ?
O13 W8 O29 99.3(8) . . ?
O13 W8 O21 103.7(8) . . ?
O29 W8 O21 88.6(7) . . ?
O13 W8 O14 99.2(8) . . ?
O29 W8 O14 92.7(8) . . ?
O21 W8 O14 156.5(7) . . ?
O13 W8 O12 95.1(8) . . ?
O29 W8 O12 165.3(7) . . ?
O21 W8 O12 85.3(7) . . ?
O14 W8 O12 87.6(7) . . ?
O13 W8 O20 172.1(7) . . ?
O29 W8 O20 84.8(7) . . ?
O21 W8 O20 83.1(6) . . ?
O14 W8 O20 73.7(6) . . ?
O12 W8 O20 81.2(6) . . ?
O15 W9 O31 98.9(9) . . ?
O15 W9 O16 102.1(8) . . ?
O31 W9 O16 89.9(7) . . ?
O15 W9 O14 99.1(8) . . ?
O31 W9 O14 90.5(8) . . ?
O16 W9 O14 158.4(7) . . ?
O15 W9 O8 97.7(8) . . ?
O31 W9 O8 163.4(7) . . ?
O16 W9 O8 86.2(7) . . ?
O14 W9 O8 87.3(7) . . ?
O15 W9 O20 172.5(7) . . ?
O31 W9 O20 83.1(7) . . ?
O16 W9 O20 85.1(7) . . ?
O14 W9 O20 73.6(6) . . ?
O8 W9 O20 80.5(6) . . ?
O38 W10 O37 102.7(9) . . ?
O38 W10 O27 98.9(9) . . ?
O37 W10 O27 88.7(8) . . ?
O38 W10 O46 96.7(9) . . ?
O37 W10 O46 88.1(8) . . ?
O27 W10 O46 164.4(8) . . ?
O38 W10 O39 101.6(9) . . ?
O37 W10 O39 155.7(8) . . ?
O27 W10 O39 88.0(8) . . ?
O46 W10 O39 88.5(8) . . ?
O38 W10 O43 172.8(8) . . ?
O37 W10 O43 84.0(7) . . ?
O27 W10 O43 83.6(7) . . ?
O46 W10 O43 80.8(7) . . ?
O39 W10 O43 71.7(7) . . ?
O45 W11 O39 97.9(9) . . ?
O45 W11 O47 96.2(8) . . ?
O39 W11 O47 89.9(8) . . ?
O45 W11 O40 101.2(8) . . ?
O39 W11 O40 160.9(8) . . ?
O47 W11 O40 86.6(8) . . ?
O45 W11 O28 96.8(8) . . ?
O39 W11 O28 91.6(8) . . ?
O47 W11 O28 166.6(7) . . ?
O40 W11 O28 87.7(8) . . ?
O45 W11 O43 173.8(8) . . ?
O39 W11 O43 76.1(7) . . ?
O47 W11 O43 82.2(7) . . ?
O40 W11 O43 84.8(7) . . ?
O28 W11 O43 85.2(7) . . ?
O62 W12 O41 101.8(8) . . ?
O62 W12 O52 97.5(9) . . ?
O41 W12 O52 92.2(8) . . ?
O62 W12 O40 101.8(8) . . ?
O41 W12 O40 156.3(7) . . ?
O52 W12 O40 87.4(8) . . ?
O62 W12 O32 98.6(8) . . ?
O41 W12 O32 87.9(7) . . ?
O52 W12 O32 163.6(8) . . ?
O40 W12 O32 86.0(7) . . ?
O62 W12 O42 175.6(8) . . ?
O41 W12 O42 74.0(7) . . ?
O52 W12 O42 81.8(7) . . ?
O40 W12 O42 82.6(7) . . ?
O32 W12 O42 82.5(7) . . ?
O34 W13 O61 99.6(8) . . ?
O34 W13 O50 97.0(9) . . ?
O61 W13 O50 86.2(8) . . ?
O34 W13 O41 101.3(8) . . ?
O61 W13 O41 159.1(8) . . ?
O50 W13 O41 91.6(8) . . ?
O34 W13 O30 97.2(9) . . ?
O61 W13 O30 87.8(7) . . ?
O50 W13 O30 165.3(8) . . ?
O41 W13 O30 89.3(7) . . ?
O34 W13 O42 175.0(8) . . ?
O61 W13 O42 85.4(7) . . ?
O50 W13 O42 82.5(7) . . ?
O41 W13 O42 73.7(7) . . ?
O30 W13 O42 83.7(7) . . ?
O33 W14 O61 102.9(9) . . ?
O33 W14 O35 101.3(8) . . ?
O61 W14 O35 155.8(7) . . ?
O33 W14 O51 97.4(8) . . ?
O61 W14 O51 87.6(8) . . ?
O35 W14 O51 89.6(8) . . ?
O33 W14 O29 97.9(8) . . ?
O61 W14 O29 88.1(7) . . ?
O35 W14 O29 88.3(7) . . ?
O51 W14 O29 164.7(7) . . ?
O33 W14 O44 172.7(8) . . ?
O61 W14 O44 84.4(7) . . ?
O35 W14 O44 71.4(6) . . ?
O51 W14 O44 81.8(7) . . ?
O29 W14 O44 83.2(6) . . ?
O36 W15 O35 100.4(8) . . ?
O36 W15 O37 102.9(9) . . ?
O35 W15 O37 156.6(7) . . ?
O36 W15 O31 97.5(9) . . ?
O35 W15 O31 90.9(8) . . ?
O37 W15 O31 87.4(7) . . ?
O36 W15 O48 97.4(9) . . ?
O35 W15 O48 88.3(8) . . ?
O37 W15 O48 87.5(8) . . ?
O31 W15 O48 165.0(8) . . ?
O36 W15 O44 172.0(8) . . ?
O35 W15 O44 71.8(6) . . ?
O37 W15 O44 84.9(7) . . ?
O31 W15 O44 84.2(7) . . ?
O48 W15 O44 81.3(7) . . ?
O57 W16 O48 102.8(9) . . ?
O57 W16 O46 102.3(10) . . ?
O48 W16 O46 87.3(8) . . ?
O57 W16 O53 100.0(9) . . ?
O48 W16 O53 89.1(8) . . ?
O46 W16 O53 157.7(9) . . ?
O57 W16 O55 99.7(10) . . ?
O48 W16 O55 157.5(9) . . ?
O46 W16 O55 88.6(9) . . ?
O53 W16 O55 86.3(9) . . ?
O57 W16 O49 170.1(9) . . ?
O48 W16 O49 84.5(7) . . ?
O46 W16 O49 84.7(8) . . ?
O53 W16 O49 73.0(8) . . ?
O55 W16 O49 73.2(8) . . ?
O56 W17 O52 100.1(10) . . ?
O56 W17 O54 101.9(9) . . ?
O52 W17 O54 90.3(8) . . ?
O56 W17 O47 102.4(9) . . ?
O52 W17 O47 86.2(8) . . ?
O54 W17 O47 155.7(8) . . ?
O56 W17 O55 102.5(10) . . ?
O52 W17 O55 157.4(8) . . ?
O54 W17 O55 86.9(9) . . ?
O47 W17 O55 87.2(9) . . ?
O56 W17 O49 172.7(9) . . ?
O52 W17 O49 85.8(7) . . ?
O54 W17 O49 73.6(7) . . ?
O47 W17 O49 82.1(7) . . ?
O55 W17 O49 71.8(7) . . ?
O60 W18 O50 101.4(10) . . ?
O60 W18 O51 102.7(9) . . ?
O50 W18 O51 86.5(8) . . ?
O60 W18 O53 100.9(10) . . ?
O50 W18 O53 157.7(8) . . ?
O51 W18 O53 89.2(8) . . ?
O60 W18 O54 100.0(9) . . ?
O50 W18 O54 88.6(8) . . ?
O51 W18 O54 157.3(8) . . ?
O53 W18 O54 87.0(9) . . ?
O60 W18 O49 170.8(8) . . ?
O50 W18 O49 85.2(7) . . ?
O51 W18 O49 83.9(7) . . ?
O53 W18 O49 72.5(8) . . ?
O54 W18 O49 73.6(7) . . ?
N20 Na1 O13 93.0(13) 3_675 . ?
N20 Na1 K1B 59.8(11) 3_675 4_575 ?
O13 Na1 K1B 119.4(6) . 4_575 ?
N20 Na1 K1A 53.3(11) 3_675 4_575 ?
O13 Na1 K1A 139.1(6) . 4_575 ?
K1B Na1 K1A 27.6(3) 4_575 4_575 ?
O11W K1A K1B 132(2) . . ?
O11W K1A N21 95(2) . 2_645 ?
K1B K1A N21 75.5(16) . 2_645 ?
O11W K1A N20 110(2) . 2_645 ?
K1B K1A N20 79.6(12) . 2_645 ?
N21 K1A N20 23.9(10) 2_645 2_645 ?
O11W K1A C13 80(2) . 2_645 ?
K1B K1A C13 78.5(12) . 2_645 ?
N21 K1A C13 19.5(13) 2_645 2_645 ?
N20 K1A C13 43.1(12) 2_645 2_645 ?
O11W K1A Na1 138(2) . 4_676 ?
K1B K1A Na1 74.7(7) . 4_676 ?
N21 K1A Na1 55.8(11) 2_645 4_676 ?
N20 K1A Na1 33.2(8) 2_645 4_676 ?
C13 K1A Na1 75.3(10) 2_645 4_676 ?
K1A K1B N21 57.8(13) . 2_645 ?
K1A K1B O4 148.0(11) . . ?
N21 K1B O4 121.1(13) 2_645 . ?
K1A K1B O11W 15.6(8) . . ?
N21 K1B O11W 57.5(12) 2_645 . ?
O4 K1B O11W 132.8(10) . . ?
K1A K1B N20 67.4(11) . 2_645 ?
N21 K1B N20 23.4(9) 2_645 2_645 ?
O4 K1B N20 126.1(11) . 2_645 ?
O11W K1B N20 72.9(11) . 2_645 ?
K1A K1B C13 70.6(11) . 2_645 ?
N21 K1B C13 21.9(12) 2_645 2_645 ?
O4 K1B C13 100.5(11) . 2_645 ?
O11W K1B C13 64.5(11) . 2_645 ?
N20 K1B C13 41.0(11) 2_645 2_645 ?
K1A K1B Na1 77.7(7) . 4_676 ?
N21 K1B Na1 56.5(9) 2_645 4_676 ?
O4 K1B Na1 130.9(7) . 4_676 ?
O11W K1B Na1 90.0(8) . 4_676 ?
N20 K1B Na1 33.7(7) 2_645 4_676 ?
C13 K1B Na1 74.5(10) 2_645 4_676 ?
K1A K1B W3 138.8(9) . . ?
N21 K1B W3 102.5(11) 2_645 . ?
O4 K1B W3 18.6(5) . . ?
O11W K1B W3 123.6(8) . . ?
N20 K1B W3 109.9(9) 2_645 . ?
C13 K1B W3 81.9(9) 2_645 . ?
Na1 K1B W3 124.2(5) 4_676 . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
C5 H5A O61 0.93 2.54 3.32(3) 141.6 3_675
C6 H6A O5 0.93 2.58 3.35(3) 141.6 2_655

_refine_diff_density_max         4.569
_refine_diff_density_min         -4.743
_refine_diff_density_rms         0.440

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_6
_audit_block_doi                 10.5517/cc13897x
_database_code_depnum_ccdc_archive 'CCDC 1020868'
_audit_update_record             
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C24 H98 Cu12 N36 O108 P2 S2 W18'
_chemical_formula_sum            'C12 H49 Cu6 N18 O54 P S W9'
_chemical_formula_weight         3408.61

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_H-M_alt        'C 2/m'
_space_group_name_Hall           '-C 2y'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'

_cell_length_a                   24.8710(2)
_cell_length_b                   14.2534(1)
_cell_length_c                   20.8280(2)
_cell_angle_alpha                90
_cell_angle_beta                 125.026(3)
_cell_angle_gamma                90
_cell_volume                     6046.25(2)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.20
_cell_measurement_theta_max      25.000

_exptl_crystal_description       acicular
_exptl_crystal_colour            blue
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    3.745
_exptl_crystal_F_000             6200
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.15
_exptl_absorpt_coefficient_mu    19.298
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.0409
_exptl_absorpt_correction_T_max  0.0602
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            17477
_diffrn_reflns_av_unetI/netI     0.0776
_diffrn_reflns_av_R_equivalents  0.0724
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_theta_min         1.194
_diffrn_reflns_theta_max         24.994
_diffrn_reflns_theta_full        24.994
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             5539
_reflns_number_gt                3896
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
The restraint commands 'DELU', and 'SIMU' were refined the atoms S2 and o28, 
and the restraint command 'ISOR' was used to refine O8, O8A, O21, 
 O28, O29, O31, O33, O11, O12, O13, O14, N4 and N7 atoms.
 The restraint order 'SIMU' was refined the atoms O12, W1, W2,O29 and O30.
 The 'OMIT' order was used to confirm the data completeless.
 "Short Inter D...A Contact O13 .. O14 .. 2.61 Ang" is caused
 by the disorder of W. 
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.303 0.000 0.022 18 6 ' '
2 0.771 0.000 0.251 82 30 ' '
3 0.229 0.000 0.749 82 48 ' '
4 0.697 0.000 0.978 18 5 ' '
5 0.644 0.179 0.361 40 25 ' '
6 0.356 0.179 0.639 40 30 ' '
7 0.334 0.187 0.122 20 6 ' '
8 0.666 0.187 0.878 20 8 ' '
9 0.144 0.321 0.361 40 23 ' '
10 0.856 0.321 0.639 40 29 ' '
11 0.834 0.315 0.121 21 6 ' '
12 0.271 0.500 0.251 82 30 ' '
13 0.729 0.500 0.749 82 48 ' '
14 0.166 0.315 0.879 20 8 ' '
15 0.802 0.502 0.021 17 6 ' '
16 0.198 0.503 0.979 18 5 ' '
17 0.144 0.679 0.361 40 25 ' '
18 0.856 0.679 0.639 40 30 ' '
19 0.835 0.687 0.122 20 6 ' '
20 0.165 0.687 0.878 20 8 ' '
21 0.644 0.821 0.361 40 23 ' '
22 0.356 0.821 0.639 40 29 ' '
23 0.335 0.813 0.122 20 6 ' '
24 0.665 0.813 0.878 20 8 ' '
_platon_squeeze_details          
;
;

_computing_data_collection       'SMART (Bruker, 1997)'
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0854P)²+174.5586P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   mixed
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         5539
_refine_ls_number_parameters     493
_refine_ls_number_restraints     781
_refine_ls_R_factor_all          0.0835
_refine_ls_R_factor_gt           0.0536
_refine_ls_wR_factor_ref         0.1649
_refine_ls_wR_factor_gt          0.1430
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_restrained_S_all      1.009
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.02663(3) 0.13217(5) 0.18521(4) 0.0165(2) Uani 1 1 d . U . . .
W2 W 0.16068(3) 0.13206(5) 0.17138(4) 0.0162(2) Uani 1 1 d . U . . .
W3 W 0.13436(4) 0.13169(5) -0.01367(5) 0.0221(2) Uani 1 1 d . . . . .
W4 W -0.09241(7) 0.34495(11) -0.04713(10) 0.0167(3) Uani 0.5 1 d . . P . .
W5 W -0.03648(7) 0.34527(10) 0.06029(10) 0.0167(3) Uani 0.5 1 d . . P . .
W6 W 0.06208(7) 0.34587(10) 0.11741(10) 0.0174(3) Uani 0.5 1 d . . P . .
Cu1 Cu 0.39768(16) 0.0000 0.2961(2) 0.0236(8) Uani 1 2 d S T P . .
Cu2 Cu 0.33298(11) 0.11576(14) 0.37861(15) 0.0193(5) Uani 1 1 d . . . . .
Cu3 Cu 0.34507(15) 0.5000 0.5108(2) 0.0225(8) Uani 1 2 d S T P . .
Cu4 Cu 0.49016(11) 0.38566(14) 0.63615(15) 0.0200(5) Uani 1 1 d . . . . .
S1 S 0.5000 0.5000 0.5000 0.064(5) Uani 1 4 d S T P . .
S2 S 0.5000 0.0000 0.5000 0.060(3) Uani 1 4 d S TU P . .
P1 P 0.0000 0.1387(4) 0.0000 0.0103(12) Uani 1 2 d S T P . .
O1 O 0.1305(6) 0.2570(9) 0.1395(9) 0.029(2) Uani 1 1 d . U . . .
O2 O 0.1096(6) 0.2572(9) -0.0099(9) 0.026(2) Uani 1 1 d . U . . .
O3 O 0.0227(7) 0.2585(9) 0.1504(9) 0.032(2) Uani 1 1 d . U . . .
O4 O 0.0402(7) 0.1570(10) 0.2721(9) 0.038(3) Uani 1 1 d . U . . .
O5 O 0.2364(7) 0.1572(10) 0.2522(9) 0.036(3) Uani 1 1 d . U . . .
O6 O 0.1979(6) 0.1545(9) -0.0191(9) 0.029(3) Uani 1 1 d . U . . .
O7 O 0.0000 0.2495(12) 0.0000 0.024(3) Uani 1 2 d S TU P . .
O8 O 0.1584(13) 0.1064(19) 0.0822(18) 0.031(3) Uani 0.5 1 d . U P . .
O8A O 0.1940(13) 0.1504(19) 0.1040(18) 0.031(3) Uani 0.5 1 d . U P . .
O9 O 0.1024(12) 0.4254(18) 0.1958(17) 0.028(5) Uani 0.5 1 d . U P . .
O10 O -0.1555(12) 0.4249(18) -0.0813(17) 0.030(4) Uani 0.5 1 d . U P . .
O11 O 0.1699(10) 0.0000 0.1800(14) 0.041(3) Uani 1 2 d S TU P . .
O12 O 0.1114(7) 0.1254(10) 0.2097(10) 0.040(2) Uani 1 1 d . U . . .
O13 O 0.1397(10) 0.0000 -0.0110(14) 0.037(3) Uani 1 2 d S TU P . .
O14 O -0.0643(8) 0.1253(11) 0.1169(11) 0.055(3) Uani 1 1 d . U . . .
O15 O 0.0275(11) 0.0000 0.1935(14) 0.044(4) Uani 1 2 d S TU P . .
O16 O -0.0598(13) 0.4214(19) 0.1018(17) 0.031(4) Uani 0.5 1 d . U P . .
O17 O 0.0730(13) 0.1089(18) 0.0417(17) 0.029(2) Uani 0.5 1 d . U P . .
O18 O 0.0220(12) 0.1066(18) -0.0516(17) 0.026(3) Uani 0.5 1 d . U P . .
O19 O 0.0457(13) 0.1065(19) 0.0859(18) 0.032(3) Uani 0.5 1 d . U P . .
O20 O 0.0464(13) 0.395(2) 0.0872(18) 0.027(3) Uani 0.5 1 d . U P . .
O21 O -0.0252(13) 0.396(2) 0.0548(18) 0.029(3) Uani 0.5 1 d . U P . .
O22 O -0.0779(14) 0.394(2) -0.0459(18) 0.028(4) Uani 0.5 1 d . U P . .
O23 O 0.4545(13) 0.0000 0.2597(17) 0.065(7) Uani 1 2 d S TU P . .
O24 O 0.3058(12) 0.0000 0.1644(16) 0.055(5) Uani 1 2 d S TU P . .
O25 O 0.3293(9) 0.0000 0.3210(13) 0.028(3) Uani 1 2 d S TU P . .
O26 O 0.4331(8) 0.5000 0.6148(12) 0.022(4) Uani 1 2 d S TU P . .
O27 O 0.2615(10) 0.5000 0.3990(15) 0.047(6) Uani 1 2 d S TU P . .
O28 O 0.4831(18) 0.0000 0.419(2) 0.058(5) Uani 0.6666 2 d S TU P . .
O30 O 0.5000 0.108(3) 0.5000 0.077(9) Uani 0.6666 2 d S TU P . .
O32 O 0.5183(15) 0.5000 0.580(2) 0.029(5) Uani 0.6 2 d S TU P . .
O33 O 0.4173(17) 0.5000 0.456(2) 0.039(6) Uani 0.6 2 d S TU P . .
N1 N 0.3857(7) 0.1816(10) 0.3484(9) 0.017(3) Uani 1 1 d . . . . .
N2 N 0.4062(7) 0.1365(10) 0.3079(10) 0.024(4) Uani 1 1 d . . . . .
N3 N 0.4518(9) 0.2762(11) 0.3409(11) 0.032(4) Uani 1 1 d . . . . .
N4 N 0.3544(7) 0.3626(10) 0.5010(10) 0.022(4) Uani 1 1 d . U . . .
N5 N 0.4122(8) 0.3176(12) 0.5511(11) 0.029(4) Uiso 1 1 d . . . . .
N6 N 0.3495(8) 0.2232(10) 0.4514(11) 0.024(4) Uani 1 1 d . . . . .
N7 N 0.5656(7) 0.4512(9) 0.7256(11) 0.022(4) Uani 1 1 d . . . . .
N8 N 0.6554(11) 0.5000 0.8322(18) 0.048(8) Uani 1 2 d S T P . .
H8A H 0.6932 0.5000 0.8765 0.057 Uiso 1 2 d R U P . .
N9 N 0.2223(8) 0.5480(10) 0.5961(11) 0.030(4) Uani 1 1 d . . . . .
N10 N 0.2880(11) 0.5000 0.5631(14) 0.026(5) Uiso 1 2 d S . P . .
C1 C 0.3182(9) 0.3038(12) 0.4455(12) 0.020(4) Uani 1 1 d . . . . .
H1A H 0.2746 0.3156 0.4051 0.024 Uiso 1 1 calc R U . . .
C2 C 0.4078(11) 0.2343(13) 0.5189(14) 0.036(6) Uani 1 1 d . . . . .
H2A H 0.4413 0.1898 0.5409 0.043 Uiso 1 1 calc R U . . .
C3 C 0.6196(10) 0.4237(14) 0.7897(17) 0.045(7) Uani 1 1 d . . . . .
H3A H 0.6320 0.3616 0.8044 0.054 Uiso 1 1 calc R U . . .
C4 C 0.4129(9) 0.2650(12) 0.3651(13) 0.024(5) Uani 1 1 d . . . . .
H4A H 0.4059 0.3112 0.3910 0.029 Uiso 1 1 calc R U . . .
C5 C 0.4435(10) 0.1938(14) 0.3032(14) 0.034(5) Uani 1 1 d . . . . .
H5A H 0.4628 0.1806 0.2770 0.041 Uiso 1 1 calc R U . . .
C6 C 0.2617(11) 0.5718(15) 0.5773(15) 0.037(6) Uani 1 1 d . . . . .
H6A H 0.2711 0.6340 0.5739 0.045 Uiso 1 1 calc R U . . .
O31 O 0.4957(16) 0.413(2) 0.533(2) 0.029(5) Uani 0.4 1 d . U P . .
O29 O 0.428(2) 0.0000 0.477(3) 0.069(7) Uani 0.6666 2 d S TU P . .
O1W O 0.4134(15) 0.0000 0.603(2) 0.079(7) Uiso 1 2 d S U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O4 1.678(16) . ?
W1 O14 1.859(16) . ?
W1 O12 1.865(14) . ?
W1 O15 1.891(2) . ?
W1 O3 1.922(13) . ?
W1 O18 2.34(3) 2 ?
W1 O19 2.40(3) . ?
W2 O5 1.694(14) . ?
W2 O12 1.809(16) . ?
W2 O8 1.86(3) . ?
W2 O11 1.892(2) . ?
W2 O1 1.899(13) . ?
W2 O8A 2.01(3) . ?
W2 O17 2.32(3) . ?
W2 O19 2.37(3) . ?
W3 O6 1.681(13) . ?
W3 O8 1.76(3) . ?
W3 O14 1.835(17) 2 ?
W3 O13 1.8803(14) . ?
W3 O2 1.908(13) . ?
W3 O8A 2.03(3) . ?
W3 O17 2.41(3) . ?
W3 O18 2.46(2) . ?
W4 O22 0.78(3) . ?
W4 O10 1.73(2) . ?
W4 W5 1.835(2) . ?
W4 O20 1.90(3) 2 ?
W4 O2 1.934(14) 2 ?
W4 O21 1.94(3) . ?
W4 W6 1.995(2) 2 ?
W4 O1 2.019(14) 2 ?
W4 O7 2.347(10) . ?
W5 O21 0.80(3) . ?
W5 O16 1.69(3) . ?
W5 O20 1.93(3) . ?
W5 O2 1.948(13) 2 ?
W5 O22 1.95(3) . ?
W5 O3 2.012(14) . ?
W5 W6 2.019(2) . ?
W5 O7 2.361(10) . ?
W6 O20 0.87(3) . ?
W6 O9 1.75(3) . ?
W6 O22 1.88(3) 2 ?
W6 O21 1.91(3) . ?
W6 O3 1.939(14) . ?
W6 O1 1.952(13) . ?
W6 W4 1.995(2) 2 ?
W6 O7 2.433(10) . ?
Cu1 O23 1.95(3) . ?
Cu1 N2 1.957(15) 6 ?
Cu1 N2 1.957(15) . ?
Cu1 O25 2.043(19) . ?
Cu1 O28 2.20(4) . ?
Cu1 O24 2.36(3) . ?
Cu2 N9 1.983(15) 4_546 ?
Cu2 N1 1.986(14) . ?
Cu2 O25 2.011(12) . ?
Cu2 N6 2.024(16) . ?
Cu2 O5 2.406(15) . ?
Cu3 N4 1.996(14) 6_565 ?
Cu3 N4 1.996(14) . ?
Cu3 O26 2.010(19) . ?
Cu3 O27 2.05(2) . ?
Cu3 N10 2.23(2) . ?
Cu4 N7 1.962(16) . ?
Cu4 N5 1.973(17) . ?
Cu4 N3 1.989(16) 2_656 ?
Cu4 O26 2.036(10) . ?
Cu4 O31 2.26(3) . ?
Cu4 O32 2.34(3) . ?
S1 O32 1.44(4) 5_666 ?
S1 O32 1.44(4) . ?
S1 O31 1.45(3) 6_565 ?
S1 O31 1.45(3) 2_656 ?
S1 O31 1.45(3) 5_666 ?
S1 O31 1.45(3) . ?
S1 O33 1.71(3) . ?
S1 O33 1.71(3) 5_666 ?
S2 O28 1.48(4) 5_656 ?
S2 O28 1.48(4) . ?
S2 O30 1.53(4) . ?
S2 O30 1.53(4) 5_656 ?
S2 O29 1.56(4) . ?
S2 O29 1.56(4) 5_656 ?
P1 O18 1.53(3) . ?
P1 O18 1.53(3) 2 ?
P1 O19 1.54(3) . ?
P1 O19 1.54(3) 2 ?
P1 O17 1.56(3) . ?
P1 O17 1.56(3) 2 ?
P1 O7 1.579(18) . ?
O1 W4 2.019(14) 2 ?
O2 W4 1.934(14) 2 ?
O2 W5 1.947(13) 2 ?
O7 W4 2.347(10) 2 ?
O7 W5 2.361(10) 2 ?
O7 W6 2.433(10) 2 ?
O8 O8A 0.96(3) . ?
O8 O17 1.78(4) . ?
O10 O22 1.68(4) . ?
O11 W2 1.892(2) 6 ?
O13 W3 1.8804(14) 6 ?
O14 W3 1.835(17) 2 ?
O15 W1 1.891(2) 6 ?
O16 O21 1.67(4) . ?
O17 O19 1.42(4) . ?
O17 O18 1.60(4) . ?
O18 O19 1.40(4) 2 ?
O18 W1 2.34(3) 2 ?
O19 O18 1.40(4) 2 ?
O20 O22 1.46(4) 2 ?
O20 O21 1.50(4) . ?
O20 W4 1.90(3) 2 ?
O21 O22 1.72(4) . ?
O22 O20 1.46(4) 2 ?
O22 W6 1.88(3) 2 ?
O25 Cu2 2.011(12) 6 ?
O26 Cu4 2.036(10) 6_565 ?
O32 O31 1.47(4) . ?
O32 O31 1.47(4) 6_565 ?
O32 Cu4 2.34(2) 6_565 ?
N1 C4 1.31(2) . ?
N1 N2 1.37(2) . ?
N2 C5 1.28(2) . ?
N3 C4 1.33(2) . ?
N3 C5 1.36(3) . ?
N3 Cu4 1.989(16) 2_656 ?
N4 C1 1.29(2) . ?
N4 N5 1.36(2) . ?
N5 C2 1.34(3) . ?
N6 C2 1.33(3) . ?
N6 C1 1.35(2) . ?
N7 C3 1.30(3) . ?
N7 N7 1.39(3) 6_565 ?
N8 C3 1.36(3) . ?
N8 C3 1.36(3) 6_565 ?
N8 H8A 0.8599 . ?
N9 C6 1.29(3) . ?
N9 N9 1.37(3) 6_565 ?
N9 Cu2 1.983(15) 4_556 ?
N10 C6 1.33(3) 6_565 ?
N10 C6 1.34(3) . ?
C1 H1A 0.9300 . ?
C2 H2A 0.9300 . ?
C3 H3A 0.9300 . ?
C4 H4A 0.9300 . ?
C5 H5A 0.9300 . ?
C6 H6A 0.9300 . ?
O31 O31 1.52(7) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 W1 O14 103.9(8) . . ?
O4 W1 O12 102.7(7) . . ?
O14 W1 O12 153.5(8) . . ?
O4 W1 O15 97.3(9) . . ?
O14 W1 O15 87.8(8) . . ?
O12 W1 O15 88.4(8) . . ?
O4 W1 O3 98.3(7) . . ?
O14 W1 O3 89.1(6) . . ?
O12 W1 O3 87.5(6) . . ?
O15 W1 O3 164.4(9) . . ?
O4 W1 O18 164.3(8) . 2 ?
O14 W1 O18 60.7(9) . 2 ?
O12 W1 O18 92.8(8) . 2 ?
O15 W1 O18 85.6(10) . 2 ?
O3 W1 O18 79.5(8) . 2 ?
O4 W1 O19 160.9(8) . . ?
O14 W1 O19 95.1(9) . . ?
O12 W1 O19 58.5(8) . . ?
O15 W1 O19 85.9(10) . . ?
O3 W1 O19 79.1(8) . . ?
O18 W1 O19 34.4(9) 2 . ?
O5 W2 O12 102.7(8) . . ?
O5 W2 O8 114.4(10) . . ?
O12 W2 O8 142.2(10) . . ?
O5 W2 O11 96.4(8) . . ?
O12 W2 O11 89.0(9) . . ?
O8 W2 O11 80.3(11) . . ?
O5 W2 O1 98.1(6) . . ?
O12 W2 O1 88.3(6) . . ?
O8 W2 O1 93.2(9) . . ?
O11 W2 O1 165.6(8) . . ?
O5 W2 O8A 89.9(10) . . ?
O12 W2 O8A 165.5(9) . . ?
O8 W2 O8A 28.3(10) . . ?
O11 W2 O8A 96.8(11) . . ?
O1 W2 O8A 82.7(9) . . ?
O5 W2 O17 162.2(9) . . ?
O12 W2 O17 94.8(8) . . ?
O8 W2 O17 48.8(11) . . ?
O11 W2 O17 87.2(9) . . ?
O1 W2 O17 78.9(8) . . ?
O8A W2 O17 72.3(10) . . ?
O5 W2 O19 162.0(9) . . ?
O12 W2 O19 59.6(9) . . ?
O8 W2 O19 83.6(11) . . ?
O11 W2 O19 86.9(9) . . ?
O1 W2 O19 79.5(8) . . ?
O8A W2 O19 107.3(11) . . ?
O17 W2 O19 35.3(10) . . ?
O6 W3 O8 113.3(10) . . ?
O6 W3 O14 103.1(8) . 2 ?
O8 W3 O14 142.6(11) . 2 ?
O6 W3 O13 98.1(8) . . ?
O8 W3 O13 77.9(12) . . ?
O14 W3 O13 89.3(8) 2 . ?
O6 W3 O2 99.2(6) . . ?
O8 W3 O2 93.0(10) . . ?
O14 W3 O2 89.1(6) 2 . ?
O13 W3 O2 162.5(8) . . ?
O6 W3 O8A 89.6(9) . . ?
O8 W3 O8A 28.3(10) . . ?
O14 W3 O8A 165.4(10) 2 . ?
O13 W3 O8A 96.1(10) . . ?
O2 W3 O8A 81.7(9) . . ?
O6 W3 O17 159.9(8) . . ?
O8 W3 O17 47.5(11) . . ?
O14 W3 O17 96.8(9) 2 . ?
O13 W3 O17 84.5(9) . . ?
O2 W3 O17 78.3(7) . . ?
O8A W3 O17 70.3(10) . . ?
O6 W3 O18 161.4(8) . . ?
O8 W3 O18 85.3(11) . . ?
O14 W3 O18 58.4(9) 2 . ?
O13 W3 O18 85.0(8) . . ?
O2 W3 O18 79.3(7) . . ?
O8A W3 O18 108.4(10) . . ?
O17 W3 O18 38.4(9) . . ?
O22 W4 O10 74(2) . . ?
O22 W4 W5 87(2) . . ?
O10 W4 W5 112.0(10) . . ?
O22 W4 O20 45(2) . 2 ?
O10 W4 O20 101.9(12) . 2 ?
W5 W4 O20 108.0(9) . 2 ?
O22 W4 O2 145(2) . 2 ?
O10 W4 O2 102.2(10) . 2 ?
W5 W4 O2 62.2(4) . 2 ?
O20 W4 O2 155.9(9) 2 2 ?
O22 W4 O21 62(2) . . ?
O10 W4 O21 102.4(12) . . ?
W5 W4 O21 24.4(9) . . ?
O20 W4 O21 89.0(13) 2 . ?
O2 W4 O21 85.7(11) 2 . ?
O22 W4 W6 70(2) . 2 ?
O10 W4 W6 109.2(10) . 2 ?
W5 W4 W6 123.59(10) . 2 ?
O20 W4 W6 25.6(9) 2 2 ?
O2 W4 W6 139.9(4) 2 2 ?
O21 W4 W6 110.5(9) . 2 ?
O22 W4 O1 123(2) . 2 ?
O10 W4 O1 101.5(10) . 2 ?
W5 W4 O1 140.9(4) . 2 ?
O20 W4 O1 83.4(10) 2 2 ?
O2 W4 O1 92.0(6) 2 2 ?
O21 W4 O1 156.0(9) . 2 ?
W6 W4 O1 58.2(4) 2 2 ?
O22 W4 O7 100(2) . . ?
O10 W4 O7 174.0(9) . . ?
W5 W4 O7 67.45(12) . . ?
O20 W4 O7 73.0(9) 2 . ?
O2 W4 O7 82.9(4) 2 . ?
O21 W4 O7 74.7(9) . . ?
W6 W4 O7 67.59(12) 2 . ?
O1 W4 O7 81.3(4) 2 . ?
O21 W5 O16 75(2) . . ?
O21 W5 W4 85(2) . . ?
O16 W5 W4 112.6(9) . . ?
O21 W5 O20 47(2) . . ?
O16 W5 O20 103.9(12) . . ?
W4 W5 O20 106.9(9) . . ?
O21 W5 O2 143(2) . 2 ?
O16 W5 O2 101.6(10) . 2 ?
W4 W5 O2 61.4(4) . 2 ?
O20 W5 O2 154.4(9) . 2 ?
O21 W5 O22 61(2) . . ?
O16 W5 O22 103.8(13) . . ?
W4 W5 O22 23.5(9) . . ?
O20 W5 O22 88.9(13) . . ?
O2 W5 O22 84.0(10) 2 . ?
O21 W5 O3 124(2) . . ?
O16 W5 O3 101.5(11) . . ?
W4 W5 O3 140.6(4) . . ?
O20 W5 O3 82.4(10) . . ?
O2 W5 O3 93.6(6) 2 . ?
O22 W5 O3 154.5(9) . . ?
O21 W5 W6 71.0(19) . . ?
O16 W5 W6 110.8(9) . . ?
W4 W5 W6 122.18(11) . . ?
O20 W5 W6 25.2(9) . . ?
O2 W5 W6 139.7(4) 2 . ?
O22 W5 W6 109.8(8) . . ?
O3 W5 W6 57.5(4) . . ?
O21 W5 O7 100(2) . . ?
O16 W5 O7 175.2(10) . . ?
W4 W5 O7 66.66(12) . . ?
O20 W5 O7 72.2(9) . . ?
O2 W5 O7 82.2(5) 2 . ?
O22 W5 O7 73.6(9) . . ?
O3 W5 O7 80.9(5) . . ?
W6 W5 O7 66.95(12) . . ?
O20 W6 O9 86(2) . . ?
O20 W6 O22 49(2) . 2 ?
O9 W6 O22 103.6(13) . 2 ?
O20 W6 O21 49.2(19) . . ?
O9 W6 O21 102.3(12) . . ?
O22 W6 O21 89.8(13) 2 . ?
O20 W6 O3 131.7(18) . . ?
O9 W6 O3 102.7(10) . . ?
O22 W6 O3 153.6(10) 2 . ?
O21 W6 O3 82.7(10) . . ?
O20 W6 O1 131.3(18) . . ?
O9 W6 O1 104.2(9) . . ?
O22 W6 O1 82.7(10) 2 . ?
O21 W6 O1 153.5(10) . . ?
O3 W6 O1 92.8(6) . . ?
O20 W6 W4 71.0(18) . 2 ?
O9 W6 W4 115.6(9) . 2 ?
O22 W6 W4 23.0(9) 2 2 ?
O21 W6 W4 105.1(10) . 2 ?
O3 W6 W4 137.5(4) . 2 ?
O1 W6 W4 61.5(5) . 2 ?
O20 W6 W5 71.8(17) . . ?
O9 W6 W5 113.8(8) . . ?
O22 W6 W5 105.7(9) 2 . ?
O21 W6 W5 23.4(9) . . ?
O3 W6 W5 61.1(4) . . ?
O1 W6 W5 137.3(4) . . ?
W4 W6 W5 114.22(10) 2 . ?
O20 W6 O7 87.9(19) . . ?
O9 W6 O7 174.0(9) . . ?
O22 W6 O7 73.1(9) 2 . ?
O21 W6 O7 73.0(9) . . ?
O3 W6 O7 80.5(5) . . ?
O1 W6 O7 80.5(5) . . ?
W4 W6 O7 63.12(13) 2 . ?
W5 W6 O7 63.25(13) . . ?
O23 Cu1 N2 89.9(5) . 6 ?
O23 Cu1 N2 89.9(5) . . ?
N2 Cu1 N2 167.5(10) 6 . ?
O23 Cu1 O25 173.4(10) . . ?
N2 Cu1 O25 90.8(5) 6 . ?
N2 Cu1 O25 90.8(5) . . ?
O23 Cu1 O28 91.3(14) . . ?
N2 Cu1 O28 83.8(5) 6 . ?
N2 Cu1 O28 83.8(5) . . ?
O25 Cu1 O28 95.3(12) . . ?
O23 Cu1 O24 89.0(11) . . ?
N2 Cu1 O24 96.2(5) 6 . ?
N2 Cu1 O24 96.2(5) . . ?
O25 Cu1 O24 84.5(9) . . ?
O28 Cu1 O24 179.7(13) . . ?
N9 Cu2 N1 177.5(7) 4_546 . ?
N9 Cu2 O25 87.6(7) 4_546 . ?
N1 Cu2 O25 90.6(6) . . ?
N9 Cu2 N6 92.5(7) 4_546 . ?
N1 Cu2 N6 89.6(6) . . ?
O25 Cu2 N6 171.0(7) . . ?
N9 Cu2 O5 90.1(6) 4_546 . ?
N1 Cu2 O5 87.9(6) . . ?
O25 Cu2 O5 82.8(7) . . ?
N6 Cu2 O5 106.3(6) . . ?
N4 Cu3 N4 157.7(10) 6_565 . ?
N4 Cu3 O26 89.5(5) 6_565 . ?
N4 Cu3 O26 89.5(5) . . ?
N4 Cu3 O27 89.2(5) 6_565 . ?
N4 Cu3 O27 89.2(5) . . ?
O26 Cu3 O27 173.2(9) . . ?
N4 Cu3 N10 101.1(5) 6_565 . ?
N4 Cu3 N10 101.1(5) . . ?
O26 Cu3 N10 94.5(8) . . ?
O27 Cu3 N10 92.3(10) . . ?
N7 Cu4 N5 175.8(7) . . ?
N7 Cu4 N3 88.8(7) . 2_656 ?
N5 Cu4 N3 91.9(7) . 2_656 ?
N7 Cu4 O26 89.6(6) . . ?
N5 Cu4 O26 89.7(7) . . ?
N3 Cu4 O26 178.3(7) 2_656 . ?
N7 Cu4 O31 105.7(10) . . ?
N5 Cu4 O31 78.4(10) . . ?
N3 Cu4 O31 86.2(10) 2_656 . ?
O26 Cu4 O31 93.9(10) . . ?
N7 Cu4 O32 75.4(9) . . ?
N5 Cu4 O32 108.3(10) . . ?
N3 Cu4 O32 106.3(8) 2_656 . ?
O26 Cu4 O32 72.9(7) . . ?
O31 Cu4 O32 37.1(11) . . ?
O32 S1 O32 180.0 5_666 . ?
O32 S1 O31 119.1(14) 5_666 6_565 ?
O32 S1 O31 60.9(14) . 6_565 ?
O32 S1 O31 60.9(14) 5_666 2_656 ?
O32 S1 O31 119.1(14) . 2_656 ?
O31 S1 O31 180.0 6_565 2_656 ?
O32 S1 O31 60.9(14) 5_666 5_666 ?
O32 S1 O31 119.1(14) . 5_666 ?
O31 S1 O31 63(3) 6_565 5_666 ?
O31 S1 O31 117(3) 2_656 5_666 ?
O32 S1 O31 119.1(14) 5_666 . ?
O32 S1 O31 60.9(14) . . ?
O31 S1 O31 117(3) 6_565 . ?
O31 S1 O31 63(3) 2_656 . ?
O31 S1 O31 180.0 5_666 . ?
O32 S1 O33 84.2(18) 5_666 . ?
O32 S1 O33 95.8(18) . . ?
O31 S1 O33 81.8(15) 6_565 . ?
O31 S1 O33 98.2(15) 2_656 . ?
O31 S1 O33 98.2(15) 5_666 . ?
O31 S1 O33 81.8(15) . . ?
O32 S1 O33 95.8(18) 5_666 5_666 ?
O32 S1 O33 84.2(18) . 5_666 ?
O31 S1 O33 98.2(15) 6_565 5_666 ?
O31 S1 O33 81.8(15) 2_656 5_666 ?
O31 S1 O33 81.8(15) 5_666 5_666 ?
O31 S1 O33 98.2(15) . 5_666 ?
O33 S1 O33 180.0 . 5_666 ?
O28 S2 O28 180.0 5_656 . ?
O28 S2 O30 90.000(11) 5_656 . ?
O28 S2 O30 90.000(9) . . ?
O28 S2 O30 90.000(9) 5_656 5_656 ?
O28 S2 O30 90.000(10) . 5_656 ?
O30 S2 O30 180.0 . 5_656 ?
O28 S2 O29 83(2) 5_656 . ?
O28 S2 O29 97(2) . . ?
O30 S2 O29 90.000(4) . . ?
O30 S2 O29 90.000(15) 5_656 . ?
O28 S2 O29 97(2) 5_656 5_656 ?
O28 S2 O29 83(2) . 5_656 ?
O30 S2 O29 90.000(15) . 5_656 ?
O30 S2 O29 90.000(5) 5_656 5_656 ?
O29 S2 O29 180.0 . 5_656 ?
O18 P1 O18 145.2(19) . 2 ?
O18 P1 O19 113.8(15) . . ?
O18 P1 O19 54.4(14) 2 . ?
O18 P1 O19 54.4(14) . 2 ?
O18 P1 O19 113.8(15) 2 2 ?
O19 P1 O19 145(2) . 2 ?
O18 P1 O17 62.5(14) . . ?
O18 P1 O17 107.4(14) 2 . ?
O19 P1 O17 54.7(14) . . ?
O19 P1 O17 114.5(14) 2 . ?
O18 P1 O17 107.4(14) . 2 ?
O18 P1 O17 62.5(14) 2 2 ?
O19 P1 O17 114.5(14) . 2 ?
O19 P1 O17 54.7(14) 2 2 ?
O17 P1 O17 148(2) . 2 ?
O18 P1 O7 107.4(10) . . ?
O18 P1 O7 107.4(10) 2 . ?
O19 P1 O7 107.4(10) . . ?
O19 P1 O7 107.4(10) 2 . ?
O17 P1 O7 105.8(10) . . ?
O17 P1 O7 105.8(10) 2 . ?
W2 O1 W6 143.8(8) . . ?
W2 O1 W4 142.3(8) . 2 ?
W6 O1 W4 60.3(4) . 2 ?
W3 O2 W4 145.3(8) . 2 ?
W3 O2 W5 143.7(8) . 2 ?
W4 O2 W5 56.4(4) 2 2 ?
W1 O3 W6 144.0(8) . . ?
W1 O3 W5 141.2(8) . . ?
W6 O3 W5 61.4(4) . . ?
W2 O5 Cu2 151.4(8) . . ?
P1 O7 W4 125.4(4) . . ?
P1 O7 W4 125.4(4) . 2 ?
W4 O7 W4 109.1(7) . 2 ?
P1 O7 W5 125.3(3) . . ?
W4 O7 W5 45.9(2) . . ?
W4 O7 W5 91.4(5) 2 . ?
P1 O7 W5 125.3(3) . 2 ?
W4 O7 W5 91.4(5) . 2 ?
W4 O7 W5 45.9(2) 2 2 ?
W5 O7 W5 109.3(7) . 2 ?
P1 O7 W6 124.4(3) . 2 ?
W4 O7 W6 49.3(2) . 2 ?
W4 O7 W6 89.8(5) 2 2 ?
W5 O7 W6 89.5(5) . 2 ?
W5 O7 W6 49.8(2) 2 2 ?
P1 O7 W6 124.4(3) . . ?
W4 O7 W6 89.8(5) . . ?
W4 O7 W6 49.3(2) 2 . ?
W5 O7 W6 49.8(2) . . ?
W5 O7 W6 89.5(5) 2 . ?
W6 O7 W6 111.2(7) 2 . ?
O8A O8 W3 91(3) . . ?
O8A O8 O17 137(3) . . ?
W3 O8 O17 85.6(15) . . ?
O8A O8 W2 85(3) . . ?
W3 O8 W2 152.4(16) . . ?
O17 O8 W2 79.2(15) . . ?
O8 O8A W2 67(2) . . ?
O8 O8A W3 60(2) . . ?
W2 O8A W3 121.2(14) . . ?
O22 O10 W4 26.4(11) . . ?
W2 O11 W2 168.2(13) . 6 ?
W2 O12 W1 145.3(10) . . ?
W3 O13 W3 173.2(12) . 6 ?
W3 O14 W1 144.4(12) 2 . ?
W1 O15 W1 170.3(15) . 6 ?
O21 O16 W5 27.7(11) . . ?
O19 O17 P1 62.0(15) . . ?
O19 O17 O18 116(2) . . ?
P1 O17 O18 58.0(13) . . ?
O19 O17 O8 125(2) . . ?
P1 O17 O8 164(2) . . ?
O18 O17 O8 118(2) . . ?
O19 O17 W2 74.3(17) . . ?
P1 O17 W2 128.8(16) . . ?
O18 O17 W2 167.5(18) . . ?
O8 O17 W2 51.9(12) . . ?
O19 O17 W3 169(2) . . ?
P1 O17 W3 123.6(16) . . ?
O18 O17 W3 72.5(14) . . ?
O8 O17 W3 46.9(12) . . ?
W2 O17 W3 96.2(9) . . ?
O19 O18 P1 63.2(16) 2 . ?
O19 O18 O17 120(2) 2 . ?
P1 O18 O17 59.6(14) . . ?
O19 O18 W1 75.2(17) 2 2 ?
P1 O18 W1 129.8(14) . 2 ?
O17 O18 W1 161.8(18) . 2 ?
O19 O18 W3 168(2) 2 . ?
P1 O18 W3 122.0(15) . . ?
O17 O18 W3 69.1(13) . . ?
W1 O18 W3 94.3(9) 2 . ?
O18 O19 O17 123(3) 2 . ?
O18 O19 P1 62.4(16) 2 . ?
O17 O19 P1 63.2(17) . . ?
O18 O19 W2 164(2) 2 . ?
O17 O19 W2 70.4(15) . . ?
P1 O19 W2 126.4(15) . . ?
O18 O19 W1 70.5(16) 2 . ?
O17 O19 W1 163(2) . . ?
P1 O19 W1 125.2(15) . . ?
W2 O19 W1 94.5(11) . . ?
W6 O20 O22 105(3) . 2 ?
W6 O20 O21 105(3) . . ?
O22 O20 O21 129(3) 2 . ?
W6 O20 W4 83.4(19) . 2 ?
O22 O20 W4 22.3(13) 2 2 ?
O21 O20 W4 132(2) . 2 ?
W6 O20 W5 82.9(19) . . ?
O22 O20 W5 132(2) 2 . ?
O21 O20 W5 22.9(12) . . ?
W4 O20 W5 123.2(15) 2 . ?
W5 O21 O20 111(3) . . ?
W5 O21 O16 77(2) . . ?
O20 O21 O16 128(3) . . ?
W5 O21 O22 94(3) . . ?
O20 O21 O22 115(2) . . ?
O16 O21 O22 115(2) . . ?
W5 O21 W6 86(2) . . ?
O20 O21 W6 26.0(13) . . ?
O16 O21 W6 116(2) . . ?
O22 O21 W6 126.7(19) . . ?
W5 O21 W4 71(2) . . ?
O20 O21 W4 123(2) . . ?
O16 O21 W4 108.2(17) . . ?
O22 O21 W4 23.7(11) . . ?
W6 O21 W4 122.4(15) . . ?
W4 O22 O20 112(3) . 2 ?
W4 O22 O10 80(2) . . ?
O20 O22 O10 127(2) 2 . ?
W4 O22 O21 94(3) . . ?
O20 O22 O21 115(2) 2 . ?
O10 O22 O21 114(2) . . ?
W4 O22 W6 87(2) . 2 ?
O20 O22 W6 26.6(13) 2 2 ?
O10 O22 W6 117.3(19) . 2 ?
O21 O22 W6 127.8(18) . 2 ?
W4 O22 W5 70(2) . . ?
O20 O22 W5 124(2) 2 . ?
O10 O22 W5 108.5(19) . . ?
O21 O22 W5 24.2(11) . . ?
W6 O22 W5 123.7(15) 2 . ?
Cu2 O25 Cu2 110.3(10) 6 . ?
Cu2 O25 Cu1 113.1(6) 6 . ?
Cu2 O25 Cu1 113.1(6) . . ?
Cu3 O26 Cu4 115.3(6) . 6_565 ?
Cu3 O26 Cu4 115.3(6) . . ?
Cu4 O26 Cu4 106.4(8) 6_565 . ?
S2 O28 Cu1 141(2) . . ?
S1 O32 O31 59.7(18) . . ?
S1 O32 O31 59.7(18) . 6_565 ?
O31 O32 O31 115(4) . 6_565 ?
S1 O32 Cu4 126.1(11) . 6_565 ?
O31 O32 Cu4 144(2) . 6_565 ?
O31 O32 Cu4 68.4(15) 6_565 6_565 ?
S1 O32 Cu4 126.1(11) . . ?
O31 O32 Cu4 68.4(15) . . ?
O31 O32 Cu4 144(2) 6_565 . ?
Cu4 O32 Cu4 88.2(12) 6_565 . ?
C4 N1 N2 105.7(14) . . ?
C4 N1 Cu2 132.7(14) . . ?
N2 N1 Cu2 121.3(11) . . ?
C5 N2 N1 106.8(16) . . ?
C5 N2 Cu1 131.0(14) . . ?
N1 N2 Cu1 119.4(12) . . ?
C4 N3 C5 102.2(16) . . ?
C4 N3 Cu4 126.0(13) . 2_656 ?
C5 N3 Cu4 131.6(14) . 2_656 ?
C1 N4 N5 105.6(15) . . ?
C1 N4 Cu3 131.9(13) . . ?
N5 N4 Cu3 121.2(12) . . ?
C2 N5 N4 106.7(17) . . ?
C2 N5 Cu4 129.9(15) . . ?
N4 N5 Cu4 121.3(12) . . ?
C2 N6 C1 102.5(16) . . ?
C2 N6 Cu2 120.8(13) . . ?
C1 N6 Cu2 135.7(15) . . ?
C3 N7 N7 107.6(11) . 6_565 ?
C3 N7 Cu4 134.0(13) . . ?
N7 N7 Cu4 118.4(4) 6_565 . ?
C3 N8 C3 106(3) . 6_565 ?
C3 N8 H8A 127.0 . . ?
C3 N8 H8A 127.0 6_565 . ?
C6 N9 N9 105.2(12) . 6_565 ?
C6 N9 Cu2 135.6(14) . 4_556 ?
N9 N9 Cu2 119.2(5) 6_565 4_556 ?
C6 N10 C6 100(2) 6_565 . ?
C6 N10 Cu3 129.6(12) 6_565 . ?
C6 N10 Cu3 129.6(12) . . ?
N4 C1 N6 113.7(16) . . ?
N4 C1 H1A 123.2 . . ?
N6 C1 H1A 123.2 . . ?
N6 C2 N5 111.2(18) . . ?
N6 C2 H2A 124.4 . . ?
N5 C2 H2A 124.4 . . ?
N7 C3 N8 109.4(19) . . ?
N7 C3 H3A 125.3 . . ?
N8 C3 H3A 125.3 . . ?
N1 C4 N3 112.6(17) . . ?
N1 C4 H4A 123.7 . . ?
N3 C4 H4A 123.7 . . ?
N2 C5 N3 113(2) . . ?
N2 C5 H5A 123.7 . . ?
N3 C5 H5A 123.7 . . ?
N9 C6 N10 114.8(18) . . ?
N9 C6 H6A 122.6 . . ?
N10 C6 H6A 122.6 . . ?
S1 O31 O32 59.4(18) . . ?
S1 O31 O31 58.4(13) . 2_656 ?
O32 O31 O31 114(2) . 2_656 ?
S1 O31 Cu4 132(2) . . ?
O32 O31 Cu4 74.5(19) . . ?
O31 O31 Cu4 169.3(14) 2_656 . ?

_refine_diff_density_max         3.749
_refine_diff_density_min         -4.020
_refine_diff_density_rms         0.517

